 
data_1
 
_audit_creation_method            SHELXL-97 
_chemical_name_systematic 
; 
 ? 
; 
_chemical_name_common             ? 
_chemical_melting_point           ? 
_chemical_formula_moiety          ? 
_chemical_formula_sum 
 'H40 Co2 Mo10 O56 Sm2' 
_chemical_formula_weight          2314.28 
 
loop_ 
 _atom_type_symbol 
 _atom_type_description 
 _atom_type_scat_dispersion_real 
 _atom_type_scat_dispersion_imag 
 _atom_type_scat_source 
 'Co'  'Co'   0.3494   0.9721 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'H'  'H'   0.0000   0.0000 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Mo'  'Mo'  -1.6832   0.6857 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'O'  'O'   0.0106   0.0060 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Sm'  'Sm'  -0.1638   3.4418 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 
_symmetry_cell_setting            Triclinic
_symmetry_space_group_name_H-M    P-1
 
loop_ 
 _symmetry_equiv_pos_as_xyz 
 'x, y, z' 
 '-x, -y, -z' 
 
_cell_length_a                    12.458(3) 
_cell_length_b                    13.915(3) 
_cell_length_c                    14.341(3) 
_cell_angle_alpha                 74.555(3) 
_cell_angle_beta                  85.531(3) 
_cell_angle_gamma                 89.871(2) 
_cell_volume                      2388.5(9) 
_cell_formula_units_Z             2 
_cell_measurement_temperature     293(2) 
_cell_measurement_reflns_used     13309
_cell_measurement_theta_min       1.52
_cell_measurement_theta_max       25.00  
 
_exptl_crystal_description        'plate' 
_exptl_crystal_colour             'dark green' 
_exptl_crystal_size_max           0.28  
_exptl_crystal_size_mid           0.13  
_exptl_crystal_size_min           0.10 
_exptl_crystal_density_meas       ? 
_exptl_crystal_density_diffrn     3.218 
_exptl_crystal_density_method     'not measured' 
_exptl_crystal_F_000              2172 
_exptl_absorpt_coefficient_mu     5.750 
_exptl_absorpt_correction_type    empirical 
_exptl_absorpt_correction_T_min   0.412
_exptl_absorpt_correction_T_max   0.563 
_exptl_absorpt_process_details     'ABSCOR by T.Higashi 8 March, 1995' 
 
_exptl_special_details 
; 
 ? 
; 
 
_diffrn_ambient_temperature       293(2) 
_diffrn_radiation_wavelength      0.71073 
_diffrn_radiation_type            MoK\a 
_diffrn_radiation_source          'fine-focus sealed tube' 
_diffrn_radiation_monochromator   graphite 
_diffrn_measurement_device_type   'Bruker Smart Apex CCD' 
_diffrn_measurement_method        'ω-2θ' 
_diffrn_detector_area_resol_mean  0.01 
_diffrn_standards_number          0 
_diffrn_standards_interval_count  0 
_diffrn_standards_interval_time   0
_diffrn_standards_decay_%         none  
_diffrn_reflns_number             13309 
_diffrn_reflns_av_R_equivalents   0.0319 
_diffrn_reflns_av_sigmaI/netI     0.0563 
_diffrn_reflns_limit_h_min        -14 
_diffrn_reflns_limit_h_max        14 
_diffrn_reflns_limit_k_min        -16 
_diffrn_reflns_limit_k_max        16 
_diffrn_reflns_limit_l_min        -14 
_diffrn_reflns_limit_l_max        17 
_diffrn_reflns_theta_min          1.52 
_diffrn_reflns_theta_max          25.00 
_reflns_number_total              8270 
_reflns_number_gt                 6892 
_reflns_threshold_expression      >2sigma(I) 
 
_computing_data_collection        ? 
_computing_cell_refinement        ? 
_computing_data_reduction         ? 
_computing_structure_solution     'SHELXS-97 (Sheldrick, 1990)' 
_computing_structure_refinement   'SHELXL-97 (Sheldrick, 1997)' 
_computing_molecular_graphics     'Bruker SHELXTL' 
_computing_publication_material   'Bruker SHELXTL'
 
_refine_special_details 
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
; 
 
_refine_ls_structure_factor_coef  Fsqd  
_refine_ls_matrix_type            full 
_refine_ls_weighting_scheme       calc  
_refine_ls_weighting_details 
 'calc w=1/[σ²(Fo²)+(0.0457P)²+11.7308P] where P=(Fo²+2Fc²)/3' 
_atom_sites_solution_primary      direct 
_atom_sites_solution_secondary    difmap 
_atom_sites_solution_hydrogens    '.' 
_refine_ls_hydrogen_treatment     none 
_refine_ls_extinction_method      none 
_refine_ls_extinction_coef        ? 
_refine_ls_number_reflns          8270 
_refine_ls_number_parameters      640 
_refine_ls_number_restraints      114 
_refine_ls_R_factor_all           0.0478 
_refine_ls_R_factor_gt            0.0384 
_refine_ls_wR_factor_ref          0.1039 
_refine_ls_wR_factor_gt           0.0981 
_refine_ls_goodness_of_fit_ref    1.024 
_refine_ls_restrained_S_all       1.038 
_refine_ls_shift/su_max           0.001 
_refine_ls_shift/su_mean          0.000 
 
loop_ 
 _atom_site_label 
 _atom_site_type_symbol 
 _atom_site_fract_x 
 _atom_site_fract_y 
 _atom_site_fract_z 
 _atom_site_U_iso_or_equiv 
 _atom_site_adp_type 
 _atom_site_occupancy 
 _atom_site_symmetry_multiplicity 
 _atom_site_calc_flag 
 _atom_site_refinement_flags 
 _atom_site_disorder_assembly 
 _atom_site_disorder_group 
Mo1 Mo 0.07543(5) 0.89562(5) 0.17297(5) 0.01799(16) Uani 1 1 d . . . 
Mo2 Mo 0.02840(6) 0.73616(6) 0.46540(5) 0.02640(18) Uani 1 1 d . . . 
Mo3 Mo 0.18927(6) 0.56350(5) 0.41727(6) 0.02585(18) Uani 1 1 d . . . 
Mo4 Mo 0.39881(6) 0.63497(5) 0.25647(5) 0.02253(17) Uani 1 1 d . . . 
Mo5 Mo 0.43440(5) 0.87257(5) 0.14075(5) 0.01858(16) Uani 1 1 d . . . 
Mo6 Mo 0.43824(5) 0.87360(5) 0.37630(5) 0.01865(16) Uani 1 1 d . . . 
Mo7 Mo 0.50560(6) 1.10712(5) 0.26243(5) 0.02205(17) Uani 1 1 d . . . 
Mo8 Mo 0.33428(6) 1.24356(6) 0.11997(6) 0.02857(19) Uani 1 1 d . . . 
Mo9 Mo 0.11715(6) 1.13400(5) 0.07574(5) 0.02243(17) Uani 1 1 d . . . 
Mo10 Mo 0.09527(5) 0.97223(5) 0.37350(5) 0.01897(16) Uani 1 1 d . . . 
Co1 Co 0.23739(8) 0.80188(8) 0.31078(8) 0.0166(2) Uani 1 1 d . . . 
Co2 Co 0.28277(8) 1.00359(7) 0.22225(7) 0.0157(2) Uani 1 1 d . . . 
Sm1 Sm -0.16380(3) 1.07494(3) 0.23750(3) 0.02150(12) Uani 1 1 d . . . 
Sm2 Sm 0.71104(4) 0.54869(4) 0.30625(3) 0.02822(13) Uani 1 1 d . . . 
O1 O 0.2084(4) 0.7171(4) 0.4410(4) 0.0220(12) Uani 1 1 d . . . 
O2 O 0.0891(4) 0.8336(4) 0.3145(4) 0.0202(12) Uani 1 1 d . . . 
O3 O 0.1327(4) 1.0233(4) 0.2306(4) 0.0179(11) Uani 1 1 d . . . 
O4 O 0.2896(4) 1.0953(4) 0.0920(4) 0.0199(12) Uani 1 1 d . . . 
O5 O 0.2521(4) 0.8872(4) 0.1851(4) 0.0177(11) Uani 1 1 d . . . 
O6 O 0.2228(4) 0.6780(4) 0.2732(4) 0.0208(12) Uani 1 1 d . . . 
O7 O 0.3884(4) 0.7848(4) 0.2988(4) 0.0193(12) Uani 1 1 d . . . 
O8 O 0.2639(4) 0.9184(4) 0.3478(4) 0.0184(12) Uani 1 1 d . . . 
O9 O 0.0814(5) 0.8625(5) 0.4844(4) 0.0276(14) Uani 1 1 d . . . 
O10 O -0.0381(4) 0.9985(4) 0.3577(4) 0.0236(13) Uani 1 1 d . . . 
O11 O -0.0560(4) 0.9300(5) 0.1901(4) 0.0256(13) Uani 1 1 d . . . 
O12 O 0.1332(5) 1.1968(5) -0.0422(4) 0.0359(16) Uani 1 1 d . . . 
O13 O 0.3441(5) 0.5799(4) 0.3894(4) 0.0255(13) Uani 1 1 d . . . 
O14 O 0.3885(5) 0.8109(5) 0.4921(4) 0.0293(14) Uani 1 1 d . . . 
O15 O 0.5709(5) 0.8606(4) 0.1341(4) 0.0291(14) Uani 1 1 d . . . 
O16 O 0.3933(5) 0.7403(4) 0.1385(4) 0.0234(13) Uani 1 1 d . . . 
O17 O 0.4610(5) 1.0051(4) 0.3815(4) 0.0237(13) Uani 1 1 d . . . 
O18 O 0.1645(6) 0.4708(5) 0.3644(5) 0.0423(17) Uani 1 1 d . . . 
O19 O 0.1778(5) 1.2261(4) 0.1345(4) 0.0289(14) Uani 1 1 d . . . 
O20 O 0.4311(4) 0.9705(4) 0.2197(4) 0.0167(11) Uani 1 1 d . . . 
O21 O 0.1142(4) 1.0001(4) 0.0588(4) 0.0216(12) Uani 1 1 d . . . 
O22 O 0.0237(5) 0.6759(5) 0.5861(5) 0.0420(17) Uani 1 1 d . . . 
O23 O 0.1448(5) 1.0646(5) 0.4166(5) 0.0378(16) Uani 1 1 d . . . 
O24 O 0.0500(5) 0.6250(4) 0.4098(5) 0.0297(14) Uani 1 1 d . . . 
O25 O 0.4047(5) 0.9405(5) 0.0287(4) 0.0287(14) Uani 1 1 d . . . 
O26 O 0.0746(5) 0.7906(5) 0.1327(5) 0.0335(15) Uani 1 1 d . . . 
O27 O -0.0178(5) 1.1405(5) 0.1113(5) 0.0344(15) Uani 1 1 d . . . 
O28 O 0.5340(5) 0.6266(5) 0.2708(4) 0.0301(14) Uani 1 1 d . . . 
O29 O 0.5686(4) 0.8353(4) 0.3644(4) 0.0278(14) Uani 1 1 d . . . 
O30 O 0.3695(6) 0.5393(5) 0.2094(5) 0.0412(17) Uani 1 1 d . . . 
O31 O 0.4740(5) 1.1815(4) 0.1350(4) 0.0270(13) Uani 1 1 d . . . 
O32 O 0.3248(4) 1.1197(4) 0.2622(4) 0.0225(12) Uani 1 1 d . . . 
O33 O 0.5217(6) 1.2012(5) 0.3148(5) 0.0403(17) Uani 1 1 d . . . 
O34 O 0.6345(5) 1.0703(5) 0.2390(4) 0.0286(14) Uani 1 1 d . . . 
O35 O -0.0997(5) 0.7649(5) 0.4404(5) 0.0400(17) Uani 1 1 d . . . 
O36 O 0.3529(6) 1.3042(5) -0.0004(5) 0.049(2) Uani 1 1 d . . . 
O37 O 0.3420(6) 1.3326(5) 0.1800(6) 0.050(2) Uani 1 1 d . . . 
O38 O 0.1948(5) 0.5079(5) 0.5392(5) 0.0337(15) Uani 1 1 d . . . 
O1W O -0.2366(7) 1.1148(8) 0.3852(6) 0.073(3) Uani 1 1 d U . . 
O2W O -0.0418(9) 1.2028(7) 0.2788(8) 0.080(3) Uani 1 1 d U . . 
O3W O -0.2310(5) 0.9127(5) 0.3293(5) 0.0442(18) Uani 1 1 d U . . 
O4W O -0.2254(5) 1.0498(5) 0.0912(5) 0.0382(16) Uani 1 1 d U . . 
O5W O -0.2173(5) 1.2467(5) 0.1660(5) 0.0394(16) Uani 1 1 d U . . 
O6W O 0.7767(7) 0.5629(6) 0.1346(5) 0.058(2) Uani 1 1 d U . . 
O7W O 0.5991(7) 0.4381(6) 0.2345(6) 0.060(2) Uani 1 1 d U . . 
O8W O 0.7306(6) 0.7277(5) 0.2164(5) 0.0447(18) Uani 1 1 d U . . 
O9W O 0.6719(6) 0.6523(5) 0.4182(5) 0.0480(19) Uani 1 1 d U . . 
O10W O 0.9035(5) 0.5947(6) 0.2818(5) 0.0476(19) Uani 1 1 d U . . 
O11W O 0.5847(5) 0.4460(5) 0.4303(5) 0.0426(17) Uani 1 1 d U . . 
O12W O 0.7946(7) 0.3869(6) 0.3124(6) 0.058(2) Uani 1 1 d U . . 
OW1 O 0.4024(7) 0.3566(6) 0.3855(6) 0.057(2) Uani 1 1 d U . . 
OW2 O 0.3246(12) 0.1623(10) 0.4498(10) 0.124(4) Uani 1 1 d U . . 
OW3 O 0.9254(9) 0.4064(8) 0.0975(8) 0.090(3) Uani 1 1 d U . . 
OW4 O 0.6433(7) 0.2992(8) 0.0294(6) 0.071(3) Uani 1 1 d U . . 
OW5 O 0.0228(13) 0.6127(11) 0.0961(11) 0.142(5) Uani 1 1 d U . . 
OW6 O 0.581(2) 0.4840(15) 0.0394(15) 0.095(6) Uani 0.50 1 d PU . . 
OW7 O 0.0977(16) 0.3890(16) 0.2149(14) 0.084(6) Uani 0.50 1 d PU . . 
 
 
_geom_special_details 
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
; 
 
loop_ 
 _geom_bond_atom_site_label_1 
 _geom_bond_atom_site_label_2 
 _geom_bond_distance 
 _geom_bond_site_symmetry_2 
 _geom_bond_publ_flag 
Mo1 O26 1.709(6) . ? 
Mo1 O11 1.722(5) . ? 
Mo1 O21 1.907(5) . ? 
Mo1 O2 2.004(5) . ? 
Mo1 O5 2.222(5) . ? 
Mo1 O3 2.286(5) . ? 
Mo1 Co1 2.9859(13) . ? 
Mo2 O35 1.687(6) . ? 
Mo2 O22 1.707(6) . ? 
Mo2 O24 1.929(6) . ? 
Mo2 O9 1.972(6) . ? 
Mo2 O1 2.269(6) . ? 
Mo2 O2 2.297(5) . ? 
Mo3 O18 1.700(7) . ? 
Mo3 O38 1.720(6) . ? 
Mo3 O24 1.931(6) . ? 
Mo3 O13 1.941(6) . ? 
Mo3 O6 2.258(6) . ? 
Mo3 O1 2.268(6) . ? 
Mo4 O30 1.697(6) . ? 
Mo4 O28 1.713(6) . ? 
Mo4 O13 1.926(6) . ? 
Mo4 O16 1.927(5) . ? 
Mo4 O6 2.283(5) . ? 
Mo4 O7 2.322(5) . ? 
Mo5 O25 1.701(6) . ? 
Mo5 O15 1.706(6) . ? 
Mo5 O16 1.920(6) . ? 
Mo5 O20 1.989(5) . ? 
Mo5 O7 2.298(5) . ? 
Mo5 O5 2.333(5) . ? 
Mo5 Co2 3.0056(13) . ? 
Mo6 O29 1.718(6) . ? 
Mo6 O14 1.725(6) . ? 
Mo6 O17 1.874(6) . ? 
Mo6 O7 1.998(5) . ? 
Mo6 O8 2.295(5) . ? 
Mo6 O20 2.300(5) . ? 
Mo6 Co1 3.0028(14) . ? 
Mo7 O33 1.693(6) . ? 
Mo7 O34 1.720(6) . ? 
Mo7 O31 1.916(6) . ? 
Mo7 O17 1.951(6) . ? 
Mo7 O32 2.259(6) . ? 
Mo7 O20 2.360(5) . ? 
Mo8 O37 1.694(7) . ? 
Mo8 O36 1.705(7) . ? 
Mo8 O31 1.942(6) . ? 
Mo8 O19 1.953(6) . ? 
Mo8 O4 2.282(5) . ? 
Mo8 O32 2.288(6) . ? 
Mo9 O12 1.681(6) . ? 
Mo9 O27 1.728(6) . ? 
Mo9 O19 1.897(6) . ? 
Mo9 O21 1.943(6) . ? 
Mo9 O4 2.229(5) . ? 
Mo9 O3 2.363(5) . ? 
Mo10 O23 1.703(6) . ? 
Mo10 O10 1.720(5) . ? 
Mo10 O9 1.886(6) . ? 
Mo10 O3 2.000(5) . ? 
Mo10 O8 2.265(5) . ? 
Mo10 O2 2.307(6) . ? 
Mo10 Co2 3.0105(13) . ? 
Co1 O5 1.871(5) . ? 
Co1 O8 1.873(5) . ? 
Co1 O7 1.896(5) . ? 
Co1 O2 1.899(5) . ? 
Co1 O1 1.932(5) . ? 
Co1 O6 1.950(5) . ? 
Co1 Co2 2.7942(15) . ? 
Co2 O8 1.871(5) . ? 
Co2 O5 1.883(5) . ? 
Co2 O3 1.889(5) . ? 
Co2 O20 1.903(5) . ? 
Co2 O32 1.939(5) . ? 
Co2 O4 1.958(5) . ? 
Sm1 O4W 2.399(6) . ? 
Sm1 O3W 2.405(7) . ? 
Sm1 O1W 2.437(8) . ? 
Sm1 O10 2.448(5) . ? 
Sm1 O5W 2.450(6) . ? 
Sm1 O27 2.456(6) . ? 
Sm1 O34 2.511(6) 1_455 ? 
Sm1 O2W 2.557(8) . ? 
Sm1 O11 2.628(6) . ? 
Sm2 O11W 2.430(7) . ? 
Sm2 O9W 2.450(7) . ? 
Sm2 O10W 2.457(7) . ? 
Sm2 O12W 2.461(8) . ? 
Sm2 O28 2.483(6) . ? 
Sm2 O8W 2.483(7) . ? 
Sm2 O6W 2.489(8) . ? 
Sm2 O38 2.526(6) 2_666 ? 
Sm2 O7W 2.539(8) . ? 
O34 Sm1 2.511(6) 1_655 ? 
O38 Sm2 2.526(6) 2_666 ? 
 
loop_ 
 _geom_angle_atom_site_label_1 
 _geom_angle_atom_site_label_2 
 _geom_angle_atom_site_label_3 
 _geom_angle 
 _geom_angle_site_symmetry_1 
 _geom_angle_site_symmetry_3 
 _geom_angle_publ_flag 
O26 Mo1 O11 108.1(3) . . ? 
O26 Mo1 O21 104.1(3) . . ? 
O11 Mo1 O21 96.9(3) . . ? 
O26 Mo1 O2 99.7(3) . . ? 
O11 Mo1 O2 94.0(2) . . ? 
O21 Mo1 O2 149.1(2) . . ? 
O26 Mo1 O5 91.6(3) . . ? 
O11 Mo1 O5 159.3(2) . . ? 
O21 Mo1 O5 83.8(2) . . ? 
O2 Mo1 O5 76.1(2) . . ? 
O26 Mo1 O3 161.8(3) . . ? 
O11 Mo1 O3 89.8(2) . . ? 
O21 Mo1 O3 75.9(2) . . ? 
O2 Mo1 O3 75.3(2) . . ? 
O5 Mo1 O3 70.19(19) . . ? 
O26 Mo1 Co1 89.1(2) . . ? 
O11 Mo1 Co1 132.6(2) . . ? 
O21 Mo1 Co1 121.81(16) . . ? 
O2 Mo1 Co1 38.80(15) . . ? 
O5 Mo1 Co1 38.74(14) . . ? 
O3 Mo1 Co1 76.03(13) . . ? 
O35 Mo2 O22 106.3(3) . . ? 
O35 Mo2 O24 100.7(3) . . ? 
O22 Mo2 O24 100.4(3) . . ? 
O35 Mo2 O9 101.2(3) . . ? 
O22 Mo2 O9 93.5(3) . . ? 
O24 Mo2 O9 149.6(2) . . ? 
O35 Mo2 O1 159.7(3) . . ? 
O22 Mo2 O1 93.8(3) . . ? 
O24 Mo2 O1 72.2(2) . . ? 
O9 Mo2 O1 80.0(2) . . ? 
O35 Mo2 O2 90.1(3) . . ? 
O22 Mo2 O2 161.0(3) . . ? 
O24 Mo2 O2 85.6(2) . . ? 
O9 Mo2 O2 73.5(2) . . ? 
O1 Mo2 O2 70.65(19) . . ? 
O18 Mo3 O38 106.6(3) . . ? 
O18 Mo3 O24 99.0(3) . . ? 
O38 Mo3 O24 103.6(3) . . ? 
O18 Mo3 O13 100.6(3) . . ? 
O38 Mo3 O13 95.1(3) . . ? 
O24 Mo3 O13 147.6(2) . . ? 
O18 Mo3 O6 93.1(3) . . ? 
O38 Mo3 O6 158.1(3) . . ? 
O24 Mo3 O6 81.9(2) . . ? 
O13 Mo3 O6 71.6(2) . . ? 
O18 Mo3 O1 161.7(3) . . ? 
O38 Mo3 O1 91.2(3) . . ? 
O24 Mo3 O1 72.2(2) . . ? 
O13 Mo3 O1 81.4(2) . . ? 
O6 Mo3 O1 70.05(19) . . ? 
O30 Mo4 O28 105.0(3) . . ? 
O30 Mo4 O13 100.1(3) . . ? 
O28 Mo4 O13 99.2(3) . . ? 
O30 Mo4 O16 97.0(3) . . ? 
O28 Mo4 O16 102.6(3) . . ? 
O13 Mo4 O16 147.7(2) . . ? 
O30 Mo4 O6 93.5(3) . . ? 
O28 Mo4 O6 160.6(3) . . ? 
O13 Mo4 O6 71.3(2) . . ? 
O16 Mo4 O6 80.5(2) . . ? 
O30 Mo4 O7 161.6(3) . . ? 
O28 Mo4 O7 92.2(2) . . ? 
O13 Mo4 O7 83.2(2) . . ? 
O16 Mo4 O7 72.4(2) . . ? 
O6 Mo4 O7 70.24(19) . . ? 
O25 Mo5 O15 105.8(3) . . ? 
O25 Mo5 O16 101.5(3) . . ? 
O15 Mo5 O16 99.1(3) . . ? 
O25 Mo5 O20 104.4(3) . . ? 
O15 Mo5 O20 95.6(3) . . ? 
O16 Mo5 O20 145.2(2) . . ? 
O25 Mo5 O7 153.0(2) . . ? 
O15 Mo5 O7 101.1(2) . . ? 
O16 Mo5 O7 73.1(2) . . ? 
O20 Mo5 O7 73.2(2) . . ? 
O25 Mo5 O5 85.0(2) . . ? 
O15 Mo5 O5 167.5(2) . . ? 
O16 Mo5 O5 84.3(2) . . ? 
O20 Mo5 O5 75.35(19) . . ? 
O7 Mo5 O5 68.27(18) . . ? 
O25 Mo5 Co2 87.1(2) . . ? 
O15 Mo5 Co2 133.8(2) . . ? 
O16 Mo5 Co2 121.92(17) . . ? 
O20 Mo5 Co2 38.42(15) . . ? 
O7 Mo5 Co2 74.54(14) . . ? 
O5 Mo5 Co2 38.80(13) . . ? 
O29 Mo6 O14 105.8(3) . . ? 
O29 Mo6 O17 100.9(3) . . ? 
O14 Mo6 O17 104.8(3) . . ? 
O29 Mo6 O7 91.4(2) . . ? 
O14 Mo6 O7 101.7(3) . . ? 
O17 Mo6 O7 146.4(2) . . ? 
O29 Mo6 O8 163.3(2) . . ? 
O14 Mo6 O8 86.6(2) . . ? 
O17 Mo6 O8 86.3(2) . . ? 
O7 Mo6 O8 74.9(2) . . ? 
O29 Mo6 O20 97.3(2) . . ? 
O14 Mo6 O20 156.5(2) . . ? 
O17 Mo6 O20 74.4(2) . . ? 
O7 Mo6 O20 73.0(2) . . ? 
O8 Mo6 O20 69.97(18) . . ? 
O29 Mo6 Co1 129.5(2) . . ? 
O14 Mo6 Co1 85.9(2) . . ? 
O17 Mo6 Co1 123.77(18) . . ? 
O7 Mo6 Co1 38.33(15) . . ? 
O8 Mo6 Co1 38.58(13) . . ? 
O20 Mo6 Co1 75.89(13) . . ? 
O33 Mo7 O34 104.5(3) . . ? 
O33 Mo7 O31 100.3(3) . . ? 
O34 Mo7 O31 100.6(3) . . ? 
O33 Mo7 O17 96.7(3) . . ? 
O34 Mo7 O17 100.7(3) . . ? 
O31 Mo7 O17 148.4(2) . . ? 
O33 Mo7 O32 94.9(3) . . ? 
O34 Mo7 O32 160.4(3) . . ? 
O31 Mo7 O32 72.5(2) . . ? 
O17 Mo7 O32 79.7(2) . . ? 
O33 Mo7 O20 161.9(3) . . ? 
O34 Mo7 O20 91.6(2) . . ? 
O31 Mo7 O20 84.6(2) . . ? 
O17 Mo7 O20 71.7(2) . . ? 
O32 Mo7 O20 69.70(18) . . ? 
O37 Mo8 O36 105.9(4) . . ? 
O37 Mo8 O31 102.7(3) . . ? 
O36 Mo8 O31 98.3(3) . . ? 
O37 Mo8 O19 97.5(3) . . ? 
O36 Mo8 O19 100.3(3) . . ? 
O31 Mo8 O19 147.5(2) . . ? 
O37 Mo8 O4 158.8(3) . . ? 
O36 Mo8 O4 93.7(3) . . ? 
O31 Mo8 O4 81.8(2) . . ? 
O19 Mo8 O4 70.7(2) . . ? 
O37 Mo8 O32 91.6(3) . . ? 
O36 Mo8 O32 161.5(3) . . ? 
O31 Mo8 O32 71.3(2) . . ? 
O19 Mo8 O32 83.0(2) . . ? 
O4 Mo8 O32 70.03(19) . . ? 
O12 Mo9 O27 106.3(3) . . ? 
O12 Mo9 O19 101.2(3) . . ? 
O27 Mo9 O19 100.8(3) . . ? 
O12 Mo9 O21 97.8(3) . . ? 
O27 Mo9 O21 97.7(3) . . ? 
O19 Mo9 O21 148.4(2) . . ? 
O12 Mo9 O4 96.4(3) . . ? 
O27 Mo9 O4 157.3(3) . . ? 
O19 Mo9 O4 72.8(2) . . ? 
O21 Mo9 O4 80.2(2) . . ? 
O12 Mo9 O3 165.4(3) . . ? 
O27 Mo9 O3 86.7(2) . . ? 
O19 Mo9 O3 82.4(2) . . ? 
O21 Mo9 O3 73.4(2) . . ? 
O4 Mo9 O3 70.99(18) . . ? 
O23 Mo10 O10 106.0(3) . . ? 
O23 Mo10 O9 103.1(3) . . ? 
O10 Mo10 O9 100.4(3) . . ? 
O23 Mo10 O3 102.3(3) . . ? 
O10 Mo10 O3 90.6(2) . . ? 
O9 Mo10 O3 148.2(2) . . ? 
O23 Mo10 O8 90.8(3) . . ? 
O10 Mo10 O8 159.8(2) . . ? 
O9 Mo10 O8 86.2(2) . . ? 
O3 Mo10 O8 74.7(2) . . ? 
O23 Mo10 O2 160.5(3) . . ? 
O10 Mo10 O2 93.3(2) . . ? 
O9 Mo10 O2 74.7(2) . . ? 
O3 Mo10 O2 74.9(2) . . ? 
O8 Mo10 O2 69.78(19) . . ? 
O23 Mo10 Co2 89.9(2) . . ? 
O10 Mo10 Co2 128.55(19) . . ? 
O9 Mo10 Co2 123.60(18) . . ? 
O3 Mo10 Co2 37.95(15) . . ? 
O8 Mo10 Co2 38.37(13) . . ? 
O2 Mo10 Co2 76.03(13) . . ? 
O5 Co1 O8 83.8(2) . . ? 
O5 Co1 O7 87.2(2) . . ? 
O8 Co1 O7 88.1(2) . . ? 
O5 Co1 O2 87.6(2) . . ? 
O8 Co1 O2 87.8(2) . . ? 
O7 Co1 O2 173.7(2) . . ? 
O5 Co1 O1 174.7(2) . . ? 
O8 Co1 O1 95.9(2) . . ? 
O7 Co1 O1 98.0(2) . . ? 
O2 Co1 O1 87.1(2) . . ? 
O5 Co1 O6 96.8(2) . . ? 
O8 Co1 O6 175.1(2) . . ? 
O7 Co1 O6 87.1(2) . . ? 
O2 Co1 O6 97.1(2) . . ? 
O1 Co1 O6 84.0(2) . . ? 
O5 Co1 Co2 42.07(16) . . ? 
O8 Co1 Co2 41.71(16) . . ? 
O7 Co1 Co2 85.84(17) . . ? 
O2 Co1 Co2 87.94(17) . . ? 
O1 Co1 Co2 137.45(18) . . ? 
O6 Co1 Co2 138.55(17) . . ? 
O5 Co1 Mo1 47.99(16) . . ? 
O8 Co1 Mo1 94.22(16) . . ? 
O7 Co1 Mo1 134.34(17) . . ? 
O2 Co1 Mo1 41.41(16) . . ? 
O1 Co1 Mo1 126.93(17) . . ? 
O6 Co1 Mo1 89.77(16) . . ? 
Co2 Co1 Mo1 67.35(3) . . ? 
O5 Co1 Mo6 95.74(16) . . ? 
O8 Co1 Mo6 49.82(16) . . ? 
O7 Co1 Mo6 40.79(17) . . ? 
O2 Co1 Mo6 136.48(17) . . ? 
O1 Co1 Mo6 87.96(17) . . ? 
O6 Co1 Mo6 125.29(16) . . ? 
Co2 Co1 Mo6 67.59(3) . . ? 
Mo1 Co1 Mo6 134.94(4) . . ? 
O8 Co2 O5 83.5(2) . . ? 
O8 Co2 O3 87.4(2) . . ? 
O5 Co2 O3 86.8(2) . . ? 
O8 Co2 O20 88.5(2) . . ? 
O5 Co2 O20 89.1(2) . . ? 
O3 Co2 O20 174.5(2) . . ? 
O8 Co2 O32 95.6(2) . . ? 
O5 Co2 O32 175.8(2) . . ? 
O3 Co2 O32 97.2(2) . . ? 
O20 Co2 O32 86.8(2) . . ? 
O8 Co2 O4 175.2(2) . . ? 
O5 Co2 O4 96.7(2) . . ? 
O3 Co2 O4 87.9(2) . . ? 
O20 Co2 O4 96.3(2) . . ? 
O32 Co2 O4 84.6(2) . . ? 
O8 Co2 Co1 41.77(16) . . ? 
O5 Co2 Co1 41.75(16) . . ? 
O3 Co2 Co1 87.12(17) . . ? 
O20 Co2 Co1 87.35(16) . . ? 
O32 Co2 Co1 137.06(18) . . ? 
O4 Co2 Co1 138.34(17) . . ? 
O8 Co2 Mo5 96.23(16) . . ? 
O5 Co2 Mo5 50.92(16) . . ? 
O3 Co2 Mo5 136.51(17) . . ? 
O20 Co2 Mo5 40.49(16) . . ? 
O32 Co2 Mo5 125.30(17) . . ? 
O4 Co2 Mo5 87.57(16) . . ? 
Co1 Co2 Mo5 68.69(4) . . ? 
O8 Co2 Mo10 48.72(16) . . ? 
O5 Co2 Mo10 93.94(16) . . ? 
O3 Co2 Mo10 40.63(16) . . ? 
O20 Co2 Mo10 136.22(16) . . ? 
O32 Co2 Mo10 88.46(17) . . ? 
O4 Co2 Mo10 126.52(16) . . ? 
Co1 Co2 Mo10 67.50(3) . . ? 
Mo5 Co2 Mo10 136.19(4) . . ? 
O4W Sm1 O3W 91.3(3) . . ? 
O4W Sm1 O1W 139.2(3) . . ? 
O3W Sm1 O1W 80.3(3) . . ? 
O4W Sm1 O10 138.1(2) . . ? 
O3W Sm1 O10 70.2(2) . . ? 
O1W Sm1 O10 76.1(2) . . ? 
O4W Sm1 O5W 82.6(2) . . ? 
O3W Sm1 O5W 143.5(2) . . ? 
O1W Sm1 O5W 81.2(3) . . ? 
O10 Sm1 O5W 134.1(2) . . ? 
O4W Sm1 O27 74.8(2) . . ? 
O3W Sm1 O27 136.2(2) . . ? 
O1W Sm1 O27 135.9(3) . . ? 
O10 Sm1 O27 92.7(2) . . ? 
O5W Sm1 O27 76.7(2) . . ? 
O4W Sm1 O34 67.0(2) . 1_455 ? 
O3W Sm1 O34 70.7(2) . 1_455 ? 
O1W Sm1 O34 72.6(3) . 1_455 ? 
O10 Sm1 O34 133.03(19) . 1_455 ? 
O5W Sm1 O34 73.8(2) . 1_455 ? 
O27 Sm1 O34 133.9(2) . 1_455 ? 
O4W Sm1 O2W 135.4(3) . . ? 
O3W Sm1 O2W 132.2(3) . . ? 
O1W Sm1 O2W 69.7(4) . . ? 
O10 Sm1 O2W 67.1(2) . . ? 
O5W Sm1 O2W 67.7(3) . . ? 
O27 Sm1 O2W 66.7(3) . . ? 
O34 Sm1 O2W 129.0(3) 1_455 . ? 
O4W Sm1 O11 70.4(2) . . ? 
O3W Sm1 O11 67.5(2) . . ? 
O1W Sm1 O11 137.7(3) . . ? 
O10 Sm1 O11 67.78(18) . . ? 
O5W Sm1 O11 140.4(2) . . ? 
O27 Sm1 O11 68.7(2) . . ? 
O34 Sm1 O11 118.13(18) 1_455 . ? 
O2W Sm1 O11 112.8(3) . . ? 
O11W Sm2 O9W 76.7(3) . . ? 
O11W Sm2 O10W 139.1(2) . . ? 
O9W Sm2 O10W 93.3(3) . . ? 
O11W Sm2 O12W 82.6(3) . . ? 
O9W Sm2 O12W 137.0(2) . . ? 
O10W Sm2 O12W 78.3(3) . . ? 
O11W Sm2 O28 75.7(2) . . ? 
O9W Sm2 O28 72.5(2) . . ? 
O10W Sm2 O28 139.4(2) . . ? 
O12W Sm2 O28 137.3(2) . . ? 
O11W Sm2 O8W 136.6(2) . . ? 
O9W Sm2 O8W 70.3(2) . . ? 
O10W Sm2 O8W 71.4(2) . . ? 
O12W Sm2 O8W 140.7(3) . . ? 
O28 Sm2 O8W 68.0(2) . . ? 
O11W Sm2 O6W 138.2(3) . . ? 
O9W Sm2 O6W 140.9(3) . . ? 
O10W Sm2 O6W 70.6(3) . . ? 
O12W Sm2 O6W 76.1(3) . . ? 
O28 Sm2 O6W 96.4(2) . . ? 
O8W Sm2 O6W 70.7(3) . . ? 
O11W Sm2 O38 72.0(2) . 2_666 ? 
O9W Sm2 O38 66.8(2) . 2_666 ? 
O10W Sm2 O38 67.6(2) . 2_666 ? 
O12W Sm2 O38 71.0(2) . 2_666 ? 
O28 Sm2 O38 132.5(2) . 2_666 ? 
O8W Sm2 O38 117.1(2) . 2_666 ? 
O6W Sm2 O38 130.7(2) . 2_666 ? 
O11W Sm2 O7W 69.4(3) . . ? 
O9W Sm2 O7W 134.8(3) . . ? 
O10W Sm2 O7W 131.9(3) . . ? 
O12W Sm2 O7W 67.3(3) . . ? 
O28 Sm2 O7W 70.8(2) . . ? 
O8W Sm2 O7W 117.3(3) . . ? 
O6W Sm2 O7W 69.2(3) . . ? 
O38 Sm2 O7W 125.6(2) 2_666 . ? 
Co1 O1 Mo3 103.1(2) . . ? 
Co1 O1 Mo2 101.1(2) . . ? 
Mo3 O1 Mo2 93.5(2) . . ? 
Co1 O2 Mo1 99.8(2) . . ? 
Co1 O2 Mo2 101.1(2) . . ? 
Mo1 O2 Mo2 153.3(3) . . ? 
Co1 O2 Mo10 99.9(2) . . ? 
Mo1 O2 Mo10 101.7(2) . . ? 
Mo2 O2 Mo10 90.85(19) . . ? 
Co2 O3 Mo10 101.4(2) . . ? 
Co2 O3 Mo1 100.0(2) . . ? 
Mo10 O3 Mo1 102.6(2) . . ? 
Co2 O3 Mo9 99.3(2) . . ? 
Mo10 O3 Mo9 153.9(3) . . ? 
Mo1 O3 Mo9 89.14(18) . . ? 
Co2 O4 Mo9 101.9(2) . . ? 
Co2 O4 Mo8 102.5(2) . . ? 
Mo9 O4 Mo8 93.8(2) . . ? 
Co1 O5 Co2 96.2(2) . . ? 
Co1 O5 Mo1 93.3(2) . . ? 
Co2 O5 Mo1 102.5(2) . . ? 
Co1 O5 Mo5 101.8(2) . . ? 
Co2 O5 Mo5 90.3(2) . . ? 
Mo1 O5 Mo5 159.1(3) . . ? 
Co1 O6 Mo3 102.9(2) . . ? 
Co1 O6 Mo4 101.2(2) . . ? 
Mo3 O6 Mo4 93.7(2) . . ? 
Co1 O7 Mo6 100.9(2) . . ? 
Co1 O7 Mo5 102.3(2) . . ? 
Mo6 O7 Mo5 103.8(2) . . ? 
Co1 O7 Mo4 101.5(2) . . ? 
Mo6 O7 Mo4 149.8(3) . . ? 
Mo5 O7 Mo4 90.95(19) . . ? 
Co2 O8 Co1 96.5(2) . . ? 
Co2 O8 Mo10 92.9(2) . . ? 
Co1 O8 Mo10 102.2(2) . . ? 
Co2 O8 Mo6 101.1(2) . . ? 
Co1 O8 Mo6 91.6(2) . . ? 
Mo10 O8 Mo6 159.1(3) . . ? 
Mo10 O9 Mo2 116.5(3) . . ? 
Mo10 O10 Sm1 143.8(3) . . ? 
Mo1 O11 Sm1 139.2(3) . . ? 
Mo4 O13 Mo3 117.9(3) . . ? 
Mo5 O16 Mo4 117.8(3) . . ? 
Mo6 O17 Mo7 119.4(3) . . ? 
Mo9 O19 Mo8 117.6(3) . . ? 
Co2 O20 Mo5 101.1(2) . . ? 
Co2 O20 Mo6 100.0(2) . . ? 
Mo5 O20 Mo6 104.1(2) . . ? 
Co2 O20 Mo7 100.5(2) . . ? 
Mo5 O20 Mo7 151.5(3) . . ? 
Mo6 O20 Mo7 90.25(18) . . ? 
Mo1 O21 Mo9 115.9(3) . . ? 
Mo2 O24 Mo3 117.7(3) . . ? 
Mo9 O27 Sm1 145.9(3) . . ? 
Mo4 O28 Sm2 158.9(3) . . ? 
Mo7 O31 Mo8 117.9(3) . . ? 
Co2 O32 Mo7 102.9(2) . . ? 
Co2 O32 Mo8 102.9(2) . . ? 
Mo7 O32 Mo8 93.3(2) . . ? 
Mo7 O34 Sm1 155.6(3) . 1_655 ? 
Mo3 O38 Sm2 154.2(3) . 2_666 ? 
 
loop_ 
 _geom_torsion_atom_site_label_1 
 _geom_torsion_atom_site_label_2 
 _geom_torsion_atom_site_label_3 
 _geom_torsion_atom_site_label_4 
 _geom_torsion 
 _geom_torsion_site_symmetry_1 
 _geom_torsion_site_symmetry_2 
 _geom_torsion_site_symmetry_3 
 _geom_torsion_site_symmetry_4 
 _geom_torsion_publ_flag 
O26 Mo1 Co1 O5 93.7(3) . . . . ? 
O11 Mo1 Co1 O5 -152.2(3) . . . . ? 
O21 Mo1 Co1 O5 -12.4(3) . . . . ? 
O2 Mo1 Co1 O5 -159.5(3) . . . . ? 
O3 Mo1 Co1 O5 -75.6(3) . . . . ? 
O26 Mo1 Co1 O8 171.4(3) . . . . ? 
O11 Mo1 Co1 O8 -74.5(3) . . . . ? 
O21 Mo1 Co1 O8 65.3(3) . . . . ? 
O2 Mo1 Co1 O8 -81.8(3) . . . . ? 
O5 Mo1 Co1 O8 77.7(3) . . . . ? 
O3 Mo1 Co1 O8 2.1(2) . . . . ? 
O26 Mo1 Co1 O7 79.9(3) . . . . ? 
O11 Mo1 Co1 O7 -166.0(4) . . . . ? 
O21 Mo1 Co1 O7 -26.2(3) . . . . ? 
O2 Mo1 Co1 O7 -173.3(3) . . . . ? 
O5 Mo1 Co1 O7 -13.8(3) . . . . ? 
O3 Mo1 Co1 O7 -89.4(3) . . . . ? 
O26 Mo1 Co1 O2 -106.8(3) . . . . ? 
O11 Mo1 Co1 O2 7.3(4) . . . . ? 
O21 Mo1 Co1 O2 147.1(3) . . . . ? 
O5 Mo1 Co1 O2 159.5(3) . . . . ? 
O3 Mo1 Co1 O2 83.9(3) . . . . ? 
O26 Mo1 Co1 O1 -88.0(3) . . . . ? 
O11 Mo1 Co1 O1 26.1(3) . . . . ? 
O21 Mo1 Co1 O1 165.9(3) . . . . ? 
O2 Mo1 Co1 O1 18.7(3) . . . . ? 
O5 Mo1 Co1 O1 178.3(3) . . . . ? 
O3 Mo1 Co1 O1 102.6(3) . . . . ? 
O26 Mo1 Co1 O6 -5.7(3) . . . . ? 
O11 Mo1 Co1 O6 108.4(3) . . . . ? 
O21 Mo1 Co1 O6 -111.8(3) . . . . ? 
O2 Mo1 Co1 O6 101.0(3) . . . . ? 
O5 Mo1 Co1 O6 -99.4(3) . . . . ? 
O3 Mo1 Co1 O6 -175.1(2) . . . . ? 
O26 Mo1 Co1 Co2 138.7(2) . . . . ? 
O11 Mo1 Co1 Co2 -107.1(3) . . . . ? 
O21 Mo1 Co1 Co2 32.7(2) . . . . ? 
O2 Mo1 Co1 Co2 -114.5(3) . . . . ? 
O5 Mo1 Co1 Co2 45.0(2) . . . . ? 
O3 Mo1 Co1 Co2 -30.60(13) . . . . ? 
O26 Mo1 Co1 Mo6 138.6(2) . . . . ? 
O11 Mo1 Co1 Mo6 -107.3(3) . . . . ? 
O21 Mo1 Co1 Mo6 32.5(2) . . . . ? 
O2 Mo1 Co1 Mo6 -114.7(3) . . . . ? 
O5 Mo1 Co1 Mo6 44.9(2) . . . . ? 
O3 Mo1 Co1 Mo6 -30.78(14) . . . . ? 
O29 Mo6 Co1 O5 -86.4(3) . . . . ? 
O14 Mo6 Co1 O5 166.4(3) . . . . ? 
O17 Mo6 Co1 O5 61.3(3) . . . . ? 
O7 Mo6 Co1 O5 -79.0(3) . . . . ? 
O8 Mo6 Co1 O5 76.8(3) . . . . ? 
O20 Mo6 Co1 O5 1.4(2) . . . . ? 
O29 Mo6 Co1 O8 -163.3(3) . . . . ? 
O14 Mo6 Co1 O8 89.6(3) . . . . ? 
O17 Mo6 Co1 O8 -15.5(3) . . . . ? 
O7 Mo6 Co1 O8 -155.8(3) . . . . ? 
O20 Mo6 Co1 O8 -75.4(2) . . . . ? 
O29 Mo6 Co1 O7 -7.4(4) . . . . ? 
O14 Mo6 Co1 O7 -114.6(3) . . . . ? 
O17 Mo6 Co1 O7 140.3(3) . . . . ? 
O8 Mo6 Co1 O7 155.8(3) . . . . ? 
O20 Mo6 Co1 O7 80.4(3) . . . . ? 
O29 Mo6 Co1 O2 -179.0(4) . . . . ? 
O14 Mo6 Co1 O2 73.8(3) . . . . ? 
O17 Mo6 Co1 O2 -31.3(3) . . . . ? 
O7 Mo6 Co1 O2 -171.6(3) . . . . ? 
O8 Mo6 Co1 O2 -15.7(3) . . . . ? 
O20 Mo6 Co1 O2 -91.2(3) . . . . ? 
O29 Mo6 Co1 O1 97.3(3) . . . . ? 
O14 Mo6 Co1 O1 -9.9(3) . . . . ? 
O17 Mo6 Co1 O1 -115.0(3) . . . . ? 
O7 Mo6 Co1 O1 104.7(3) . . . . ? 
O8 Mo6 Co1 O1 -99.4(3) . . . . ? 
O20 Mo6 Co1 O1 -174.9(2) . . . . ? 
O29 Mo6 Co1 O6 16.1(3) . . . . ? 
O14 Mo6 Co1 O6 -91.0(3) . . . . ? 
O17 Mo6 Co1 O6 163.9(3) . . . . ? 
O7 Mo6 Co1 O6 23.6(3) . . . . ? 
O8 Mo6 Co1 O6 179.4(3) . . . . ? 
O20 Mo6 Co1 O6 104.0(2) . . . . ? 
O29 Mo6 Co1 Co2 -118.4(3) . . . . ? 
O14 Mo6 Co1 Co2 134.4(2) . . . . ? 
O17 Mo6 Co1 Co2 29.3(2) . . . . ? 
O7 Mo6 Co1 Co2 -111.0(2) . . . . ? 
O8 Mo6 Co1 Co2 44.9(2) . . . . ? 
O20 Mo6 Co1 Co2 -30.57(13) . . . . ? 
O29 Mo6 Co1 Mo1 -118.2(3) . . . . ? 
O14 Mo6 Co1 Mo1 134.6(2) . . . . ? 
O17 Mo6 Co1 Mo1 29.5(2) . . . . ? 
O7 Mo6 Co1 Mo1 -110.8(3) . . . . ? 
O8 Mo6 Co1 Mo1 45.0(2) . . . . ? 
O20 Mo6 Co1 Mo1 -30.40(14) . . . . ? 
O5 Co1 Co2 O8 177.7(3) . . . . ? 
O7 Co1 Co2 O8 -91.8(3) . . . . ? 
O2 Co1 Co2 O8 89.0(3) . . . . ? 
O1 Co1 Co2 O8 5.5(3) . . . . ? 
O6 Co1 Co2 O8 -172.6(3) . . . . ? 
Mo1 Co1 Co2 O8 126.0(2) . . . . ? 
Mo6 Co1 Co2 O8 -54.1(2) . . . . ? 
O8 Co1 Co2 O5 -177.7(3) . . . . ? 
O7 Co1 Co2 O5 90.5(3) . . . . ? 
O2 Co1 Co2 O5 -88.7(3) . . . . ? 
O1 Co1 Co2 O5 -172.2(3) . . . . ? 
O6 Co1 Co2 O5 9.7(3) . . . . ? 
Mo1 Co1 Co2 O5 -51.7(2) . . . . ? 
Mo6 Co1 Co2 O5 128.2(2) . . . . ? 
O5 Co1 Co2 O3 88.5(3) . . . . ? 
O8 Co1 Co2 O3 -89.2(3) . . . . ? 
O7 Co1 Co2 O3 178.9(2) . . . . ? 
O2 Co1 Co2 O3 -0.3(2) . . . . ? 
O1 Co1 Co2 O3 -83.8(3) . . . . ? 
O6 Co1 Co2 O3 98.2(3) . . . . ? 
Mo1 Co1 Co2 O3 36.78(16) . . . . ? 
Mo6 Co1 Co2 O3 -143.36(16) . . . . ? 
O5 Co1 Co2 O20 -91.6(3) . . . . ? 
O8 Co1 Co2 O20 90.7(3) . . . . ? 
O7 Co1 Co2 O20 -1.1(2) . . . . ? 
O2 Co1 Co2 O20 179.7(2) . . . . ? 
O1 Co1 Co2 O20 96.2(3) . . . . ? 
O6 Co1 Co2 O20 -81.9(3) . . . . ? 
Mo1 Co1 Co2 O20 -143.24(16) . . . . ? 
Mo6 Co1 Co2 O20 36.63(16) . . . . ? 
O5 Co1 Co2 O32 -174.0(3) . . . . ? 
O8 Co1 Co2 O32 8.3(3) . . . . ? 
O7 Co1 Co2 O32 -83.6(3) . . . . ? 
O2 Co1 Co2 O32 97.3(3) . . . . ? 
O1 Co1 Co2 O32 13.7(4) . . . . ? 
O6 Co1 Co2 O32 -164.3(3) . . . . ? 
Mo1 Co1 Co2 O32 134.3(2) . . . . ? 
Mo6 Co1 Co2 O32 -45.8(2) . . . . ? 
O5 Co1 Co2 O4 4.9(3) . . . . ? 
O8 Co1 Co2 O4 -172.8(3) . . . . ? 
O7 Co1 Co2 O4 95.4(3) . . . . ? 
O2 Co1 Co2 O4 -83.8(3) . . . . ? 
O1 Co1 Co2 O4 -167.3(3) . . . . ? 
O6 Co1 Co2 O4 14.6(4) . . . . ? 
Mo1 Co1 Co2 O4 -46.7(2) . . . . ? 
Mo6 Co1 Co2 O4 133.1(2) . . . . ? 
O5 Co1 Co2 Mo5 -54.6(2) . . . . ? 
O8 Co1 Co2 Mo5 127.7(2) . . . . ? 
O7 Co1 Co2 Mo5 35.87(17) . . . . ? 
O2 Co1 Co2 Mo5 -143.32(17) . . . . ? 
O1 Co1 Co2 Mo5 133.2(2) . . . . ? 
O6 Co1 Co2 Mo5 -44.9(2) . . . . ? 
Mo1 Co1 Co2 Mo5 -106.28(4) . . . . ? 
Mo6 Co1 Co2 Mo5 73.58(3) . . . . ? 
O5 Co1 Co2 Mo10 125.2(2) . . . . ? 
O8 Co1 Co2 Mo10 -52.5(2) . . . . ? 
O7 Co1 Co2 Mo10 -144.36(17) . . . . ? 
O2 Co1 Co2 Mo10 36.45(17) . . . . ? 
O1 Co1 Co2 Mo10 -47.1(2) . . . . ? 
O6 Co1 Co2 Mo10 134.9(3) . . . . ? 
Mo1 Co1 Co2 Mo10 73.48(3) . . . . ? 
Mo6 Co1 Co2 Mo10 -106.65(4) . . . . ? 
O25 Mo5 Co2 O8 162.0(3) . . . . ? 
O15 Mo5 Co2 O8 -88.7(3) . . . . ? 
O16 Mo5 Co2 O8 60.2(3) . . . . ? 
O20 Mo5 Co2 O8 -80.3(3) . . . . ? 
O7 Mo5 Co2 O8 2.0(2) . . . . ? 
O5 Mo5 Co2 O8 76.4(3) . . . . ? 
O25 Mo5 Co2 O5 85.6(3) . . . . ? 
O15 Mo5 Co2 O5 -165.1(4) . . . . ? 
O16 Mo5 Co2 O5 -16.2(3) . . . . ? 
O20 Mo5 Co2 O5 -156.7(3) . . . . ? 
O7 Mo5 Co2 O5 -74.4(2) . . . . ? 
O25 Mo5 Co2 O3 69.3(3) . . . . ? 
O15 Mo5 Co2 O3 178.6(4) . . . . ? 
O16 Mo5 Co2 O3 -32.5(3) . . . . ? 
O20 Mo5 Co2 O3 -173.1(3) . . . . ? 
O7 Mo5 Co2 O3 -90.7(3) . . . . ? 
O5 Mo5 Co2 O3 -16.3(3) . . . . ? 
O25 Mo5 Co2 O20 -117.7(3) . . . . ? 
O15 Mo5 Co2 O20 -8.4(4) . . . . ? 
O16 Mo5 Co2 O20 140.5(3) . . . . ? 
O7 Mo5 Co2 O20 82.3(3) . . . . ? 
O5 Mo5 Co2 O20 156.7(3) . . . . ? 
O25 Mo5 Co2 O32 -96.7(3) . . . . ? 
O15 Mo5 Co2 O32 12.6(4) . . . . ? 
O16 Mo5 Co2 O32 161.5(3) . . . . ? 
O20 Mo5 Co2 O32 21.0(3) . . . . ? 
O7 Mo5 Co2 O32 103.4(3) . . . . ? 
O5 Mo5 Co2 O32 177.7(3) . . . . ? 
O25 Mo5 Co2 O4 -15.0(3) . . . . ? 
O15 Mo5 Co2 O4 94.3(3) . . . . ? 
O16 Mo5 Co2 O4 -116.8(3) . . . . ? 
O20 Mo5 Co2 O4 102.6(3) . . . . ? 
O7 Mo5 Co2 O4 -175.0(2) . . . . ? 
O5 Mo5 Co2 O4 -100.6(3) . . . . ? 
O25 Mo5 Co2 Co1 130.0(2) . . . . ? 
O15 Mo5 Co2 Co1 -120.7(3) . . . . ? 
O16 Mo5 Co2 Co1 28.2(2) . . . . ? 
O20 Mo5 Co2 Co1 -112.4(2) . . . . ? 
O7 Mo5 Co2 Co1 -30.02(14) . . . . ? 
O5 Mo5 Co2 Co1 44.4(2) . . . . ? 
O25 Mo5 Co2 Mo10 129.7(2) . . . . ? 
O15 Mo5 Co2 Mo10 -121.0(3) . . . . ? 
O16 Mo5 Co2 Mo10 27.9(2) . . . . ? 
O20 Mo5 Co2 Mo10 -112.7(2) . . . . ? 
O7 Mo5 Co2 Mo10 -30.33(15) . . . . ? 
O5 Mo5 Co2 Mo10 44.1(2) . . . . ? 
O23 Mo10 Co2 O8 91.4(3) . . . . ? 
O10 Mo10 Co2 O8 -158.0(3) . . . . ? 
O9 Mo10 Co2 O8 -14.3(3) . . . . ? 
O3 Mo10 Co2 O8 -158.3(3) . . . . ? 
O2 Mo10 Co2 O8 -75.0(3) . . . . ? 
O23 Mo10 Co2 O5 169.2(3) . . . . ? 
O10 Mo10 Co2 O5 -80.2(3) . . . . ? 
O9 Mo10 Co2 O5 63.4(3) . . . . ? 
O3 Mo10 Co2 O5 -80.5(3) . . . . ? 
O8 Mo10 Co2 O5 77.8(3) . . . . ? 
O2 Mo10 Co2 O5 2.8(2) . . . . ? 
O23 Mo10 Co2 O3 -110.4(3) . . . . ? 
O10 Mo10 Co2 O3 0.3(4) . . . . ? 
O9 Mo10 Co2 O3 143.9(3) . . . . ? 
O8 Mo10 Co2 O3 158.3(3) . . . . ? 
O2 Mo10 Co2 O3 83.3(3) . . . . ? 
O23 Mo10 Co2 O20 76.4(3) . . . . ? 
O10 Mo10 Co2 O20 -173.0(3) . . . . ? 
O9 Mo10 Co2 O20 -29.3(3) . . . . ? 
O3 Mo10 Co2 O20 -173.2(3) . . . . ? 
O8 Mo10 Co2 O20 -15.0(3) . . . . ? 
O2 Mo10 Co2 O20 -89.9(3) . . . . ? 
O23 Mo10 Co2 O32 -7.4(3) . . . . ? 
O10 Mo10 Co2 O32 103.2(3) . . . . ? 
O9 Mo10 Co2 O32 -113.1(3) . . . . ? 
O3 Mo10 Co2 O32 103.0(3) . . . . ? 
O8 Mo10 Co2 O32 -98.8(3) . . . . ? 
O2 Mo10 Co2 O32 -173.7(2) . . . . ? 
O23 Mo10 Co2 O4 -89.5(3) . . . . ? 
O10 Mo10 Co2 O4 21.1(3) . . . . ? 
O9 Mo10 Co2 O4 164.8(3) . . . . ? 
O3 Mo10 Co2 O4 20.8(3) . . . . ? 
O8 Mo10 Co2 O4 179.1(3) . . . . ? 
O2 Mo10 Co2 O4 104.2(2) . . . . ? 
O23 Mo10 Co2 Co1 136.1(2) . . . . ? 
O10 Mo10 Co2 Co1 -113.3(3) . . . . ? 
O9 Mo10 Co2 Co1 30.4(2) . . . . ? 
O3 Mo10 Co2 Co1 -113.5(3) . . . . ? 
O8 Mo10 Co2 Co1 44.7(2) . . . . ? 
O2 Mo10 Co2 Co1 -30.23(14) . . . . ? 
O23 Mo10 Co2 Mo5 136.4(2) . . . . ? 
O10 Mo10 Co2 Mo5 -113.0(3) . . . . ? 
O9 Mo10 Co2 Mo5 30.7(2) . . . . ? 
O3 Mo10 Co2 Mo5 -113.2(3) . . . . ? 
O8 Mo10 Co2 Mo5 45.0(2) . . . . ? 
O2 Mo10 Co2 Mo5 -29.92(15) . . . . ? 
O5 Co1 O1 Mo3 100(3) . . . . ? 
O8 Co1 O1 Mo3 -174.5(2) . . . . ? 
O7 Co1 O1 Mo3 -85.6(2) . . . . ? 
O2 Co1 O1 Mo3 98.0(2) . . . . ? 
O6 Co1 O1 Mo3 0.5(2) . . . . ? 
Co2 Co1 O1 Mo3 -178.18(7) . . . . ? 
Mo1 Co1 O1 Mo3 85.7(2) . . . . ? 
Mo6 Co1 O1 Mo3 -125.26(18) . . . . ? 
O5 Co1 O1 Mo2 4(3) . . . . ? 
O8 Co1 O1 Mo2 89.3(2) . . . . ? 
O7 Co1 O1 Mo2 178.2(2) . . . . ? 
O2 Co1 O1 Mo2 1.8(2) . . . . ? 
O6 Co1 O1 Mo2 -95.7(2) . . . . ? 
Co2 Co1 O1 Mo2 85.6(3) . . . . ? 
Mo1 Co1 O1 Mo2 -10.5(3) . . . . ? 
Mo6 Co1 O1 Mo2 138.52(19) . . . . ? 
O18 Mo3 O1 Co1 -24.7(10) . . . . ? 
O38 Mo3 O1 Co1 167.9(3) . . . . ? 
O24 Mo3 O1 Co1 -88.1(3) . . . . ? 
O13 Mo3 O1 Co1 73.0(3) . . . . ? 
O6 Mo3 O1 Co1 -0.5(2) . . . . ? 
O18 Mo3 O1 Mo2 77.5(9) . . . . ? 
O38 Mo3 O1 Mo2 -89.9(2) . . . . ? 
O24 Mo3 O1 Mo2 14.1(2) . . . . ? 
O13 Mo3 O1 Mo2 175.2(2) . . . . ? 
O6 Mo3 O1 Mo2 101.7(2) . . . . ? 
O35 Mo2 O1 Co1 17.8(9) . . . . ? 
O22 Mo2 O1 Co1 -170.3(3) . . . . ? 
O24 Mo2 O1 Co1 90.0(3) . . . . ? 
O9 Mo2 O1 Co1 -77.4(3) . . . . ? 
O2 Mo2 O1 Co1 -1.6(2) . . . . ? 
O35 Mo2 O1 Mo3 -86.2(8) . . . . ? 
O22 Mo2 O1 Mo3 85.6(3) . . . . ? 
O24 Mo2 O1 Mo3 -14.1(2) . . . . ? 
O9 Mo2 O1 Mo3 178.5(2) . . . . ? 
O2 Mo2 O1 Mo3 -105.6(2) . . . . ? 
O5 Co1 O2 Mo1 15.1(2) . . . . ? 
O8 Co1 O2 Mo1 98.9(2) . . . . ? 
O7 Co1 O2 Mo1 50(2) . . . . ? 
O1 Co1 O2 Mo1 -165.1(3) . . . . ? 
O6 Co1 O2 Mo1 -81.5(3) . . . . ? 
Co2 Co1 O2 Mo1 57.18(19) . . . . ? 
Mo6 Co1 O2 Mo1 110.9(2) . . . . ? 
O5 Co1 O2 Mo2 178.4(2) . . . . ? 
O8 Co1 O2 Mo2 -97.7(2) . . . . ? 
O7 Co1 O2 Mo2 -147(2) . . . . ? 
O1 Co1 O2 Mo2 -1.8(2) . . . . ? 
O6 Co1 O2 Mo2 81.8(2) . . . . ? 
Co2 Co1 O2 Mo2 -139.47(18) . . . . ? 
Mo1 Co1 O2 Mo2 163.3(4) . . . . ? 
Mo6 Co1 O2 Mo2 -85.8(3) . . . . ? 
O5 Co1 O2 Mo10 -88.7(2) . . . . ? 
O8 Co1 O2 Mo10 -4.9(2) . . . . ? 
O7 Co1 O2 Mo10 -54(2) . . . . ? 
O1 Co1 O2 Mo10 91.1(2) . . . . ? 
O6 Co1 O2 Mo10 174.7(2) . . . . ? 
Co2 Co1 O2 Mo10 -46.64(16) . . . . ? 
Mo1 Co1 O2 Mo10 -103.8(3) . . . . ? 
Mo6 Co1 O2 Mo10 7.1(3) . . . . ? 
O26 Mo1 O2 Co1 76.2(3) . . . . ? 
O11 Mo1 O2 Co1 -174.6(3) . . . . ? 
O21 Mo1 O2 Co1 -63.9(5) . . . . ? 
O5 Mo1 O2 Co1 -13.0(2) . . . . ? 
O3 Mo1 O2 Co1 -85.8(2) . . . . ? 
O26 Mo1 O2 Mo2 -65.0(7) . . . . ? 
O11 Mo1 O2 Mo2 44.2(7) . . . . ? 
O21 Mo1 O2 Mo2 154.9(5) . . . . ? 
O5 Mo1 O2 Mo2 -154.2(7) . . . . ? 
O3 Mo1 O2 Mo2 133.0(6) . . . . ? 
Co1 Mo1 O2 Mo2 -141.2(8) . . . . ? 
O26 Mo1 O2 Mo10 178.6(3) . . . . ? 
O11 Mo1 O2 Mo10 -72.3(3) . . . . ? 
O21 Mo1 O2 Mo10 38.4(5) . . . . ? 
O5 Mo1 O2 Mo10 89.3(2) . . . . ? 
O3 Mo1 O2 Mo10 16.52(19) . . . . ? 
Co1 Mo1 O2 Mo10 102.3(3) . . . . ? 
O35 Mo2 O2 Co1 -171.8(3) . . . . ? 
O22 Mo2 O2 Co1 38.3(10) . . . . ? 
O24 Mo2 O2 Co1 -71.1(3) . . . . ? 
O9 Mo2 O2 Co1 86.6(3) . . . . ? 
O1 Mo2 O2 Co1 1.6(2) . . . . ? 
O35 Mo2 O2 Mo1 -30.8(7) . . . . ? 
O22 Mo2 O2 Mo1 179.3(8) . . . . ? 
O24 Mo2 O2 Mo1 69.9(6) . . . . ? 
O9 Mo2 O2 Mo1 -132.4(7) . . . . ? 
O1 Mo2 O2 Mo1 142.6(7) . . . . ? 
O35 Mo2 O2 Mo10 88.0(3) . . . . ? 
O22 Mo2 O2 Mo10 -62.0(9) . . . . ? 
O24 Mo2 O2 Mo10 -171.3(2) . . . . ? 
O9 Mo2 O2 Mo10 -13.7(2) . . . . ? 
O1 Mo2 O2 Mo10 -98.7(2) . . . . ? 
O23 Mo10 O2 Co1 -1.0(9) . . . . ? 
O10 Mo10 O2 Co1 173.0(3) . . . . ? 
O9 Mo10 O2 Co1 -87.2(3) . . . . ? 
O3 Mo10 O2 Co1 83.3(2) . . . . ? 
O8 Mo10 O2 Co1 4.3(2) . . . . ? 
Co2 Mo10 O2 Co1 44.02(17) . . . . ? 
O23 Mo10 O2 Mo1 -103.3(8) . . . . ? 
O10 Mo10 O2 Mo1 70.7(3) . . . . ? 
O9 Mo10 O2 Mo1 170.5(3) . . . . ? 
O3 Mo10 O2 Mo1 -19.0(2) . . . . ? 
O8 Mo10 O2 Mo1 -98.0(2) . . . . ? 
Co2 Mo10 O2 Mo1 -58.24(17) . . . . ? 
O23 Mo10 O2 Mo2 100.4(8) . . . . ? 
O10 Mo10 O2 Mo2 -85.6(2) . . . . ? 
O9 Mo10 O2 Mo2 14.2(2) . . . . ? 
O3 Mo10 O2 Mo2 -175.3(2) . . . . ? 
O8 Mo10 O2 Mo2 105.7(2) . . . . ? 
Co2 Mo10 O2 Mo2 145.45(16) . . . . ? 
O8 Co2 O3 Mo10 16.2(2) . . . . ? 
O5 Co2 O3 Mo10 99.8(3) . . . . ? 
O20 Co2 O3 Mo10 58(2) . . . . ? 
O32 Co2 O3 Mo10 -79.1(3) . . . . ? 
O4 Co2 O3 Mo10 -163.4(3) . . . . ? 
Co1 Co2 O3 Mo10 58.00(19) . . . . ? 
Mo5 Co2 O3 Mo10 112.4(2) . . . . ? 
O8 Co2 O3 Mo1 -89.0(2) . . . . ? 
O5 Co2 O3 Mo1 -5.3(2) . . . . ? 
O20 Co2 O3 Mo1 -47(2) . . . . ? 
O32 Co2 O3 Mo1 175.8(2) . . . . ? 
O4 Co2 O3 Mo1 91.5(2) . . . . ? 
Co1 Co2 O3 Mo1 -47.13(16) . . . . ? 
Mo5 Co2 O3 Mo1 7.3(3) . . . . ? 
Mo10 Co2 O3 Mo1 -105.1(3) . . . . ? 
O8 Co2 O3 Mo9 -179.7(2) . . . . ? 
O5 Co2 O3 Mo9 -96.1(2) . . . . ? 
O20 Co2 O3 Mo9 -138(2) . . . . ? 
O32 Co2 O3 Mo9 85.0(2) . . . . ? 
O4 Co2 O3 Mo9 0.7(2) . . . . ? 
Co1 Co2 O3 Mo9 -137.90(17) . . . . ? 
Mo5 Co2 O3 Mo9 -83.5(3) . . . . ? 
Mo10 Co2 O3 Mo9 164.1(3) . . . . ? 
O23 Mo10 O3 Co2 73.6(3) . . . . ? 
O10 Mo10 O3 Co2 -179.8(3) . . . . ? 
O9 Mo10 O3 Co2 -68.8(5) . . . . ? 
O8 Mo10 O3 Co2 -13.8(2) . . . . ? 
O2 Mo10 O3 Co2 -86.5(2) . . . . ? 
O23 Mo10 O3 Mo1 176.8(3) . . . . ? 
O10 Mo10 O3 Mo1 -76.7(3) . . . . ? 
O9 Mo10 O3 Mo1 34.3(5) . . . . ? 
O8 Mo10 O3 Mo1 89.3(2) . . . . ? 
O2 Mo10 O3 Mo1 16.65(19) . . . . ? 
Co2 Mo10 O3 Mo1 103.1(3) . . . . ? 
O23 Mo10 O3 Mo9 -68.4(6) . . . . ? 
O10 Mo10 O3 Mo9 38.2(6) . . . . ? 
O9 Mo10 O3 Mo9 149.2(5) . . . . ? 
O8 Mo10 O3 Mo9 -155.8(7) . . . . ? 
O2 Mo10 O3 Mo9 131.5(6) . . . . ? 
Co2 Mo10 O3 Mo9 -142.0(8) . . . . ? 
O26 Mo1 O3 Co2 8.6(9) . . . . ? 
O11 Mo1 O3 Co2 179.2(3) . . . . ? 
O21 Mo1 O3 Co2 -83.6(3) . . . . ? 
O2 Mo1 O3 Co2 85.0(2) . . . . ? 
O5 Mo1 O3 Co2 4.8(2) . . . . ? 
Co1 Mo1 O3 Co2 44.90(17) . . . . ? 
O26 Mo1 O3 Mo10 -95.6(8) . . . . ? 
O11 Mo1 O3 Mo10 75.0(3) . . . . ? 
O21 Mo1 O3 Mo10 172.2(3) . . . . ? 
O2 Mo1 O3 Mo10 -19.2(2) . . . . ? 
O5 Mo1 O3 Mo10 -99.4(2) . . . . ? 
Co1 Mo1 O3 Mo10 -59.31(17) . . . . ? 
O26 Mo1 O3 Mo9 107.9(8) . . . . ? 
O11 Mo1 O3 Mo9 -81.5(2) . . . . ? 
O21 Mo1 O3 Mo9 15.67(19) . . . . ? 
O2 Mo1 O3 Mo9 -175.7(2) . . . . ? 
O5 Mo1 O3 Mo9 104.1(2) . . . . ? 
Co1 Mo1 O3 Mo9 144.18(15) . . . . ? 
O12 Mo9 O3 Co2 30.1(11) . . . . ? 
O27 Mo9 O3 Co2 -176.5(3) . . . . ? 
O19 Mo9 O3 Co2 -75.1(3) . . . . ? 
O21 Mo9 O3 Co2 84.5(2) . . . . ? 
O4 Mo9 O3 Co2 -0.7(2) . . . . ? 
O12 Mo9 O3 Mo10 172.4(9) . . . . ? 
O27 Mo9 O3 Mo10 -34.2(6) . . . . ? 
O19 Mo9 O3 Mo10 67.2(6) . . . . ? 
O21 Mo9 O3 Mo10 -133.2(7) . . . . ? 
O4 Mo9 O3 Mo10 141.6(7) . . . . ? 
O12 Mo9 O3 Mo1 -69.9(11) . . . . ? 
O27 Mo9 O3 Mo1 83.5(3) . . . . ? 
O19 Mo9 O3 Mo1 -175.1(2) . . . . ? 
O21 Mo9 O3 Mo1 -15.56(19) . . . . ? 
O4 Mo9 O3 Mo1 -100.7(2) . . . . ? 
O8 Co2 O4 Mo9 -6(3) . . . . ? 
O5 Co2 O4 Mo9 85.8(2) . . . . ? 
O3 Co2 O4 Mo9 -0.8(2) . . . . ? 
O20 Co2 O4 Mo9 175.6(2) . . . . ? 
O32 Co2 O4 Mo9 -98.2(2) . . . . ? 
Co1 Co2 O4 Mo9 82.5(3) . . . . ? 
Mo5 Co2 O4 Mo9 135.96(18) . . . . ? 
Mo10 Co2 O4 Mo9 -14.2(3) . . . . ? 
O8 Co2 O4 Mo8 90(3) . . . . ? 
O5 Co2 O4 Mo8 -177.6(2) . . . . ? 
O3 Co2 O4 Mo8 95.9(2) . . . . ? 
O20 Co2 O4 Mo8 -87.8(2) . . . . ? 
O32 Co2 O4 Mo8 -1.6(2) . . . . ? 
Co1 Co2 O4 Mo8 179.10(7) . . . . ? 
Mo5 Co2 O4 Mo8 -127.41(18) . . . . ? 
Mo10 Co2 O4 Mo8 82.4(2) . . . . ? 
O12 Mo9 O4 Co2 -171.9(3) . . . . ? 
O27 Mo9 O4 Co2 11.6(8) . . . . ? 
O19 Mo9 O4 Co2 88.3(3) . . . . ? 
O21 Mo9 O4 Co2 -75.0(2) . . . . ? 
O3 Mo9 O4 Co2 0.7(2) . . . . ? 
O12 Mo9 O4 Mo8 84.5(3) . . . . ? 
O27 Mo9 O4 Mo8 -92.0(7) . . . . ? 
O19 Mo9 O4 Mo8 -15.3(2) . . . . ? 
O21 Mo9 O4 Mo8 -178.6(2) . . . . ? 
O3 Mo9 O4 Mo8 -102.9(2) . . . . ? 
O37 Mo8 O4 Co2 -29.6(9) . . . . ? 
O36 Mo8 O4 Co2 172.4(3) . . . . ? 
O31 Mo8 O4 Co2 74.5(3) . . . . ? 
O19 Mo8 O4 Co2 -88.0(3) . . . . ? 
O32 Mo8 O4 Co2 1.4(2) . . . . ? 
O37 Mo8 O4 Mo9 73.5(8) . . . . ? 
O36 Mo8 O4 Mo9 -84.6(3) . . . . ? 
O31 Mo8 O4 Mo9 177.5(2) . . . . ? 
O19 Mo8 O4 Mo9 15.0(2) . . . . ? 
O32 Mo8 O4 Mo9 104.5(2) . . . . ? 
O8 Co1 O5 Co2 1.5(2) . . . . ? 
O7 Co1 O5 Co2 -86.9(2) . . . . ? 
O2 Co1 O5 Co2 89.6(2) . . . . ? 
O1 Co1 O5 Co2 88(3) . . . . ? 
O6 Co1 O5 Co2 -173.6(2) . . . . ? 
Mo1 Co1 O5 Co2 103.0(3) . . . . ? 
Mo6 Co1 O5 Co2 -46.91(19) . . . . ? 
O8 Co1 O5 Mo1 -101.4(2) . . . . ? 
O7 Co1 O5 Mo1 170.2(2) . . . . ? 
O2 Co1 O5 Mo1 -13.4(2) . . . . ? 
O1 Co1 O5 Mo1 -15(3) . . . . ? 
O6 Co1 O5 Mo1 83.5(2) . . . . ? 
Co2 Co1 O5 Mo1 -103.0(3) . . . . ? 
Mo6 Co1 O5 Mo1 -149.88(13) . . . . ? 
O8 Co1 O5 Mo5 93.1(2) . . . . ? 
O7 Co1 O5 Mo5 4.7(2) . . . . ? 
O2 Co1 O5 Mo5 -178.8(2) . . . . ? 
O1 Co1 O5 Mo5 179(100) . . . . ? 
O6 Co1 O5 Mo5 -82.0(2) . . . . ? 
Co2 Co1 O5 Mo5 91.6(2) . . . . ? 
Mo1 Co1 O5 Mo5 -165.4(3) . . . . ? 
Mo6 Co1 O5 Mo5 44.68(18) . . . . ? 
O8 Co2 O5 Co1 -1.5(2) . . . . ? 
O3 Co2 O5 Co1 -89.2(2) . . . . ? 
O20 Co2 O5 Co1 87.1(2) . . . . ? 
O32 Co2 O5 Co1 76(3) . . . . ? 
O4 Co2 O5 Co1 -176.7(2) . . . . ? 
Mo5 Co2 O5 Co1 101.9(2) . . . . ? 
Mo10 Co2 O5 Co1 -49.21(19) . . . . ? 
O8 Co2 O5 Mo1 93.2(2) . . . . ? 
O3 Co2 O5 Mo1 5.5(2) . . . . ? 
O20 Co2 O5 Mo1 -178.2(2) . . . . ? 
O32 Co2 O5 Mo1 170(3) . . . . ? 
O4 Co2 O5 Mo1 -81.9(2) . . . . ? 
Co1 Co2 O5 Mo1 94.8(3) . . . . ? 
Mo5 Co2 O5 Mo1 -163.3(3) . . . . ? 
Mo10 Co2 O5 Mo1 45.55(18) . . . . ? 
O8 Co2 O5 Mo5 -103.5(2) . . . . ? 
O3 Co2 O5 Mo5 168.8(2) . . . . ? 
O20 Co2 O5 Mo5 -14.9(2) . . . . ? 
O32 Co2 O5 Mo5 -26(3) . . . . ? 
O4 Co2 O5 Mo5 81.4(2) . . . . ? 
Co1 Co2 O5 Mo5 -101.9(2) . . . . ? 
Mo10 Co2 O5 Mo5 -151.15(12) . . . . ? 
O26 Mo1 O5 Co1 -86.6(3) . . . . ? 
O11 Mo1 O5 Co1 76.2(7) . . . . ? 
O21 Mo1 O5 Co1 169.4(2) . . . . ? 
O2 Mo1 O5 Co1 13.1(2) . . . . ? 
O3 Mo1 O5 Co1 92.2(2) . . . . ? 
O26 Mo1 O5 Co2 176.4(3) . . . . ? 
O11 Mo1 O5 Co2 -20.8(8) . . . . ? 
O21 Mo1 O5 Co2 72.4(3) . . . . ? 
O2 Mo1 O5 Co2 -84.0(3) . . . . ? 
O3 Mo1 O5 Co2 -4.8(2) . . . . ? 
Co1 Mo1 O5 Co2 -97.1(3) . . . . ? 
O26 Mo1 O5 Mo5 49.9(8) . . . . ? 
O11 Mo1 O5 Mo5 -147.3(7) . . . . ? 
O21 Mo1 O5 Mo5 -54.1(7) . . . . ? 
O2 Mo1 O5 Mo5 149.5(8) . . . . ? 
O3 Mo1 O5 Mo5 -131.3(8) . . . . ? 
Co1 Mo1 O5 Mo5 136.5(8) . . . . ? 
O25 Mo5 O5 Co1 172.0(3) . . . . ? 
O15 Mo5 O5 Co1 -37.1(12) . . . . ? 
O16 Mo5 O5 Co1 69.9(2) . . . . ? 
O20 Mo5 O5 Co1 -81.7(2) . . . . ? 
O7 Mo5 O5 Co1 -4.2(2) . . . . ? 
Co2 Mo5 O5 Co1 -96.4(3) . . . . ? 
O25 Mo5 O5 Co2 -91.6(3) . . . . ? 
O15 Mo5 O5 Co2 59.3(12) . . . . ? 
O16 Mo5 O5 Co2 166.2(2) . . . . ? 
O20 Mo5 O5 Co2 14.7(2) . . . . ? 
O7 Mo5 O5 Co2 92.2(2) . . . . ? 
O25 Mo5 O5 Mo1 36.6(7) . . . . ? 
O15 Mo5 O5 Mo1 -172.4(10) . . . . ? 
O16 Mo5 O5 Mo1 -65.5(7) . . . . ? 
O20 Mo5 O5 Mo1 143.0(8) . . . . ? 
O7 Mo5 O5 Mo1 -139.6(8) . . . . ? 
Co2 Mo5 O5 Mo1 128.2(8) . . . . ? 
O5 Co1 O6 Mo3 -175.3(2) . . . . ? 
O8 Co1 O6 Mo3 88(3) . . . . ? 
O7 Co1 O6 Mo3 97.8(2) . . . . ? 
O2 Co1 O6 Mo3 -86.9(2) . . . . ? 
O1 Co1 O6 Mo3 -0.5(2) . . . . ? 
Co2 Co1 O6 Mo3 178.15(7) . . . . ? 
Mo1 Co1 O6 Mo3 -127.75(18) . . . . ? 
Mo6 Co1 O6 Mo3 82.7(2) . . . . ? 
O5 Co1 O6 Mo4 88.2(2) . . . . ? 
O8 Co1 O6 Mo4 -9(3) . . . . ? 
O7 Co1 O6 Mo4 1.4(2) . . . . ? 
O2 Co1 O6 Mo4 176.7(2) . . . . ? 
O1 Co1 O6 Mo4 -97.0(2) . . . . ? 
Co2 Co1 O6 Mo4 81.7(3) . . . . ? 
Mo1 Co1 O6 Mo4 135.81(17) . . . . ? 
Mo6 Co1 O6 Mo4 -13.8(3) . . . . ? 
O18 Mo3 O6 Co1 173.1(3) . . . . ? 
O38 Mo3 O6 Co1 -32.0(8) . . . . ? 
O24 Mo3 O6 Co1 74.4(3) . . . . ? 
O13 Mo3 O6 Co1 -86.8(3) . . . . ? 
O1 Mo3 O6 Co1 0.5(2) . . . . ? 
O18 Mo3 O6 Mo4 -84.6(3) . . . . ? 
O38 Mo3 O6 Mo4 70.3(7) . . . . ? 
O24 Mo3 O6 Mo4 176.8(2) . . . . ? 
O13 Mo3 O6 Mo4 15.5(2) . . . . ? 
O1 Mo3 O6 Mo4 102.8(2) . . . . ? 
O30 Mo4 O6 Co1 -172.4(3) . . . . ? 
O28 Mo4 O6 Co1 25.1(8) . . . . ? 
O13 Mo4 O6 Co1 88.2(3) . . . . ? 
O16 Mo4 O6 Co1 -75.8(3) . . . . ? 
O7 Mo4 O6 Co1 -1.2(2) . . . . ? 
O30 Mo4 O6 Mo3 83.8(3) . . . . ? 
O28 Mo4 O6 Mo3 -78.8(8) . . . . ? 
O13 Mo4 O6 Mo3 -15.7(2) . . . . ? 
O16 Mo4 O6 Mo3 -179.7(2) . . . . ? 
O7 Mo4 O6 Mo3 -105.1(2) . . . . ? 
O5 Co1 O7 Mo6 102.1(2) . . . . ? 
O8 Co1 O7 Mo6 18.2(2) . . . . ? 
O2 Co1 O7 Mo6 67(2) . . . . ? 
O1 Co1 O7 Mo6 -77.4(3) . . . . ? 
O6 Co1 O7 Mo6 -160.9(3) . . . . ? 
Co2 Co1 O7 Mo6 59.95(18) . . . . ? 
Mo1 Co1 O7 Mo6 112.3(2) . . . . ? 
O5 Co1 O7 Mo5 -4.8(2) . . . . ? 
O8 Co1 O7 Mo5 -88.7(2) . . . . ? 
O2 Co1 O7 Mo5 -40(2) . . . . ? 
O1 Co1 O7 Mo5 175.7(2) . . . . ? 
O6 Co1 O7 Mo5 92.2(2) . . . . ? 
Co2 Co1 O7 Mo5 -46.95(17) . . . . ? 
Mo1 Co1 O7 Mo5 5.4(3) . . . . ? 
Mo6 Co1 O7 Mo5 -106.9(3) . . . . ? 
O5 Co1 O7 Mo4 -98.4(2) . . . . ? 
O8 Co1 O7 Mo4 177.8(2) . . . . ? 
O2 Co1 O7 Mo4 -133(2) . . . . ? 
O1 Co1 O7 Mo4 82.2(2) . . . . ? 
O6 Co1 O7 Mo4 -1.4(2) . . . . ? 
Co2 Co1 O7 Mo4 -140.49(18) . . . . ? 
Mo1 Co1 O7 Mo4 -88.1(2) . . . . ? 
Mo6 Co1 O7 Mo4 159.6(3) . . . . ? 
O29 Mo6 O7 Co1 174.3(3) . . . . ? 
O14 Mo6 O7 Co1 67.8(3) . . . . ? 
O17 Mo6 O7 Co1 -73.5(5) . . . . ? 
O8 Mo6 O7 Co1 -15.3(2) . . . . ? 
O20 Mo6 O7 Co1 -88.6(2) . . . . ? 
O29 Mo6 O7 Mo5 -80.0(3) . . . . ? 
O14 Mo6 O7 Mo5 173.5(2) . . . . ? 
O17 Mo6 O7 Mo5 32.2(5) . . . . ? 
O8 Mo6 O7 Mo5 90.4(2) . . . . ? 
O20 Mo6 O7 Mo5 17.16(19) . . . . ? 
Co1 Mo6 O7 Mo5 105.7(3) . . . . ? 
O29 Mo6 O7 Mo4 37.1(6) . . . . ? 
O14 Mo6 O7 Mo4 -69.4(6) . . . . ? 
O17 Mo6 O7 Mo4 149.3(5) . . . . ? 
O8 Mo6 O7 Mo4 -152.5(6) . . . . ? 
O20 Mo6 O7 Mo4 134.3(6) . . . . ? 
Co1 Mo6 O7 Mo4 -137.2(7) . . . . ? 
O25 Mo5 O7 Co1 -4.3(7) . . . . ? 
O15 Mo5 O7 Co1 177.3(3) . . . . ? 
O16 Mo5 O7 Co1 -86.4(3) . . . . ? 
O20 Mo5 O7 Co1 84.7(2) . . . . ? 
O5 Mo5 O7 Co1 4.2(2) . . . . ? 
Co2 Mo5 O7 Co1 44.66(18) . . . . ? 
O25 Mo5 O7 Mo6 -108.9(5) . . . . ? 
O15 Mo5 O7 Mo6 72.7(3) . . . . ? 
O16 Mo5 O7 Mo6 168.9(3) . . . . ? 
O20 Mo5 O7 Mo6 -19.9(2) . . . . ? 
O5 Mo5 O7 Mo6 -100.5(2) . . . . ? 
Co2 Mo5 O7 Mo6 -59.97(17) . . . . ? 
O25 Mo5 O7 Mo4 97.7(5) . . . . ? 
O15 Mo5 O7 Mo4 -80.7(3) . . . . ? 
O16 Mo5 O7 Mo4 15.6(2) . . . . ? 
O20 Mo5 O7 Mo4 -173.3(2) . . . . ? 
O5 Mo5 O7 Mo4 106.1(2) . . . . ? 
Co2 Mo5 O7 Mo4 146.66(16) . . . . ? 
O30 Mo4 O7 Co1 30.3(10) . . . . ? 
O28 Mo4 O7 Co1 -170.3(3) . . . . ? 
O13 Mo4 O7 Co1 -71.3(3) . . . . ? 
O16 Mo4 O7 Co1 87.2(3) . . . . ? 
O6 Mo4 O7 Co1 1.2(2) . . . . ? 
O30 Mo4 O7 Mo6 167.4(8) . . . . ? 
O28 Mo4 O7 Mo6 -33.2(6) . . . . ? 
O13 Mo4 O7 Mo6 65.8(5) . . . . ? 
O16 Mo4 O7 Mo6 -135.7(6) . . . . ? 
O6 Mo4 O7 Mo6 138.3(6) . . . . ? 
O30 Mo4 O7 Mo5 -72.5(9) . . . . ? 
O28 Mo4 O7 Mo5 86.9(2) . . . . ? 
O13 Mo4 O7 Mo5 -174.0(2) . . . . ? 
O16 Mo4 O7 Mo5 -15.6(2) . . . . ? 
O6 Mo4 O7 Mo5 -101.5(2) . . . . ? 
O5 Co2 O8 Co1 1.5(2) . . . . ? 
O3 Co2 O8 Co1 88.6(2) . . . . ? 
O20 Co2 O8 Co1 -87.7(2) . . . . ? 
O32 Co2 O8 Co1 -174.4(2) . . . . ? 
O4 Co2 O8 Co1 94(3) . . . . ? 
Mo5 Co2 O8 Co1 -47.9(2) . . . . ? 
Mo10 Co2 O8 Co1 102.6(3) . . . . ? 
O5 Co2 O8 Mo10 -101.1(2) . . . . ? 
O3 Co2 O8 Mo10 -14.0(2) . . . . ? 
O20 Co2 O8 Mo10 169.7(2) . . . . ? 
O32 Co2 O8 Mo10 83.0(2) . . . . ? 
O4 Co2 O8 Mo10 -9(3) . . . . ? 
Co1 Co2 O8 Mo10 -102.6(3) . . . . ? 
Mo5 Co2 O8 Mo10 -150.48(13) . . . . ? 
O5 Co2 O8 Mo6 94.5(2) . . . . ? 
O3 Co2 O8 Mo6 -178.4(2) . . . . ? 
O20 Co2 O8 Mo6 5.2(2) . . . . ? 
O32 Co2 O8 Mo6 -81.4(2) . . . . ? 
O4 Co2 O8 Mo6 -173(3) . . . . ? 
Co1 Co2 O8 Mo6 92.9(2) . . . . ? 
Mo5 Co2 O8 Mo6 45.06(18) . . . . ? 
Mo10 Co2 O8 Mo6 -164.5(3) . . . . ? 
O5 Co1 O8 Co2 -1.5(2) . . . . ? 
O7 Co1 O8 Co2 85.9(2) . . . . ? 
O2 Co1 O8 Co2 -89.4(2) . . . . ? 
O1 Co1 O8 Co2 -176.3(2) . . . . ? 
O6 Co1 O8 Co2 96(3) . . . . ? 
Mo1 Co1 O8 Co2 -48.45(19) . . . . ? 
Mo6 Co1 O8 Co2 101.4(2) . . . . ? 
O5 Co1 O8 Mo10 92.9(2) . . . . ? 
O7 Co1 O8 Mo10 -179.7(2) . . . . ? 
O2 Co1 O8 Mo10 5.0(2) . . . . ? 
O1 Co1 O8 Mo10 -81.9(2) . . . . ? 
O6 Co1 O8 Mo10 -170(3) . . . . ? 
Co2 Co1 O8 Mo10 94.4(3) . . . . ? 
Mo1 Co1 O8 Mo10 45.96(18) . . . . ? 
Mo6 Co1 O8 Mo10 -164.2(3) . . . . ? 
O5 Co1 O8 Mo6 -102.9(2) . . . . ? 
O7 Co1 O8 Mo6 -15.5(2) . . . . ? 
O2 Co1 O8 Mo6 169.2(2) . . . . ? 
O1 Co1 O8 Mo6 82.3(2) . . . . ? 
O6 Co1 O8 Mo6 -6(3) . . . . ? 
Co2 Co1 O8 Mo6 -101.4(2) . . . . ? 
Mo1 Co1 O8 Mo6 -149.85(13) . . . . ? 
O23 Mo10 O8 Co2 -88.9(3) . . . . ? 
O10 Mo10 O8 Co2 58.2(7) . . . . ? 
O9 Mo10 O8 Co2 168.1(3) . . . . ? 
O3 Mo10 O8 Co2 13.7(2) . . . . ? 
O2 Mo10 O8 Co2 92.9(2) . . . . ? 
O23 Mo10 O8 Co1 173.8(3) . . . . ? 
O10 Mo10 O8 Co1 -39.1(8) . . . . ? 
O9 Mo10 O8 Co1 70.8(3) . . . . ? 
O3 Mo10 O8 Co1 -83.7(2) . . . . ? 
O2 Mo10 O8 Co1 -4.4(2) . . . . ? 
Co2 Mo10 O8 Co1 -97.3(3) . . . . ? 
O23 Mo10 O8 Mo6 43.6(8) . . . . ? 
O10 Mo10 O8 Mo6 -169.3(7) . . . . ? 
O9 Mo10 O8 Mo6 -59.5(7) . . . . ? 
O3 Mo10 O8 Mo6 146.1(8) . . . . ? 
O2 Mo10 O8 Mo6 -134.6(8) . . . . ? 
Co2 Mo10 O8 Mo6 132.5(8) . . . . ? 
O29 Mo6 O8 Co2 -46.2(9) . . . . ? 
O14 Mo6 O8 Co2 175.2(3) . . . . ? 
O17 Mo6 O8 Co2 70.1(3) . . . . ? 
O7 Mo6 O8 Co2 -81.7(2) . . . . ? 
O20 Mo6 O8 Co2 -4.6(2) . . . . ? 
Co1 Mo6 O8 Co2 -97.0(3) . . . . ? 
O29 Mo6 O8 Co1 50.8(9) . . . . ? 
O14 Mo6 O8 Co1 -87.8(3) . . . . ? 
O17 Mo6 O8 Co1 167.1(2) . . . . ? 
O7 Mo6 O8 Co1 15.2(2) . . . . ? 
O20 Mo6 O8 Co1 92.3(2) . . . . ? 
O29 Mo6 O8 Mo10 -177.5(7) . . . . ? 
O14 Mo6 O8 Mo10 43.9(8) . . . . ? 
O17 Mo6 O8 Mo10 -61.2(7) . . . . ? 
O7 Mo6 O8 Mo10 146.9(8) . . . . ? 
O20 Mo6 O8 Mo10 -136.0(8) . . . . ? 
Co1 Mo6 O8 Mo10 131.7(8) . . . . ? 
O23 Mo10 O9 Mo2 -178.7(3) . . . . ? 
O10 Mo10 O9 Mo2 72.0(4) . . . . ? 
O3 Mo10 O9 Mo2 -36.4(6) . . . . ? 
O8 Mo10 O9 Mo2 -88.7(3) . . . . ? 
O2 Mo10 O9 Mo2 -18.6(3) . . . . ? 
Co2 Mo10 O9 Mo2 -79.9(3) . . . . ? 
O35 Mo2 O9 Mo10 -67.9(4) . . . . ? 
O22 Mo2 O9 Mo10 -175.3(3) . . . . ? 
O24 Mo2 O9 Mo10 67.3(6) . . . . ? 
O1 Mo2 O9 Mo10 91.5(3) . . . . ? 
O2 Mo2 O9 Mo10 18.9(3) . . . . ? 
O23 Mo10 O10 Sm1 97.5(6) . . . . ? 
O9 Mo10 O10 Sm1 -155.5(5) . . . . ? 
O3 Mo10 O10 Sm1 -5.4(5) . . . . ? 
O8 Mo10 O10 Sm1 -48.0(10) . . . . ? 
O2 Mo10 O10 Sm1 -80.4(5) . . . . ? 
Co2 Mo10 O10 Sm1 -5.6(7) . . . . ? 
O4W Sm1 O10 Mo10 62.6(7) . . . . ? 
O3W Sm1 O10 Mo10 131.2(6) . . . . ? 
O1W Sm1 O10 Mo10 -144.3(6) . . . . ? 
O5W Sm1 O10 Mo10 -81.6(6) . . . . ? 
O27 Sm1 O10 Mo10 -7.5(5) . . . . ? 
O34 Sm1 O10 Mo10 166.5(4) 1_455 . . . ? 
O2W Sm1 O10 Mo10 -70.8(6) . . . . ? 
O11 Sm1 O10 Mo10 58.1(5) . . . . ? 
O26 Mo1 O11 Sm1 -175.5(4) . . . . ? 
O21 Mo1 O11 Sm1 -68.2(5) . . . . ? 
O2 Mo1 O11 Sm1 82.9(5) . . . . ? 
O5 Mo1 O11 Sm1 22.6(10) . . . . ? 
O3 Mo1 O11 Sm1 7.6(4) . . . . ? 
Co1 Mo1 O11 Sm1 78.3(5) . . . . ? 
O4W Sm1 O11 Mo1 128.6(5) . . . . ? 
O3W Sm1 O11 Mo1 -131.5(5) . . . . ? 
O1W Sm1 O11 Mo1 -88.0(6) . . . . ? 
O10 Sm1 O11 Mo1 -54.6(4) . . . . ? 
O5W Sm1 O11 Mo1 78.6(5) . . . . ? 
O27 Sm1 O11 Mo1 47.8(5) . . . . ? 
O34 Sm1 O11 Mo1 177.3(4) 1_455 . . . ? 
O2W Sm1 O11 Mo1 -3.5(6) . . . . ? 
O30 Mo4 O13 Mo3 -69.5(4) . . . . ? 
O28 Mo4 O13 Mo3 -176.6(3) . . . . ? 
O16 Mo4 O13 Mo3 51.3(6) . . . . ? 
O6 Mo4 O13 Mo3 20.8(3) . . . . ? 
O7 Mo4 O13 Mo3 92.2(3) . . . . ? 
O18 Mo3 O13 Mo4 68.8(4) . . . . ? 
O38 Mo3 O13 Mo4 176.8(3) . . . . ? 
O24 Mo3 O13 Mo4 -57.6(6) . . . . ? 
O6 Mo3 O13 Mo4 -21.0(3) . . . . ? 
O1 Mo3 O13 Mo4 -92.8(3) . . . . ? 
O25 Mo5 O16 Mo4 -174.2(3) . . . . ? 
O15 Mo5 O16 Mo4 77.5(4) . . . . ? 
O20 Mo5 O16 Mo4 -36.5(6) . . . . ? 
O7 Mo5 O16 Mo4 -21.4(3) . . . . ? 
O5 Mo5 O16 Mo4 -90.4(3) . . . . ? 
Co2 Mo5 O16 Mo4 -80.3(3) . . . . ? 
O30 Mo4 O16 Mo5 -174.2(4) . . . . ? 
O28 Mo4 O16 Mo5 -67.1(4) . . . . ? 
O13 Mo4 O16 Mo5 64.3(6) . . . . ? 
O6 Mo4 O16 Mo5 93.4(3) . . . . ? 
O7 Mo4 O16 Mo5 21.3(3) . . . . ? 
O29 Mo6 O17 Mo7 75.7(4) . . . . ? 
O14 Mo6 O17 Mo7 -174.6(3) . . . . ? 
O7 Mo6 O17 Mo7 -33.8(6) . . . . ? 
O8 Mo6 O17 Mo7 -89.1(3) . . . . ? 
O20 Mo6 O17 Mo7 -18.9(3) . . . . ? 
Co1 Mo6 O17 Mo7 -79.5(3) . . . . ? 
O33 Mo7 O17 Mo6 -175.7(4) . . . . ? 
O34 Mo7 O17 Mo6 -69.5(4) . . . . ? 
O31 Mo7 O17 Mo6 62.1(6) . . . . ? 
O32 Mo7 O17 Mo6 90.5(3) . . . . ? 
O20 Mo7 O17 Mo6 18.7(3) . . . . ? 
O12 Mo9 O19 Mo8 -73.0(4) . . . . ? 
O27 Mo9 O19 Mo8 177.8(3) . . . . ? 
O21 Mo9 O19 Mo8 52.9(6) . . . . ? 
O4 Mo9 O19 Mo8 20.2(3) . . . . ? 
O3 Mo9 O19 Mo8 92.6(3) . . . . ? 
O37 Mo8 O19 Mo9 178.1(4) . . . . ? 
O36 Mo8 O19 Mo9 70.4(4) . . . . ? 
O31 Mo8 O19 Mo9 -53.7(6) . . . . ? 
O4 Mo8 O19 Mo9 -20.0(3) . . . . ? 
O32 Mo8 O19 Mo9 -91.2(3) . . . . ? 
O8 Co2 O20 Mo5 101.4(2) . . . . ? 
O5 Co2 O20 Mo5 17.9(2) . . . . ? 
O3 Co2 O20 Mo5 60(2) . . . . ? 
O32 Co2 O20 Mo5 -163.0(3) . . . . ? 
O4 Co2 O20 Mo5 -78.8(2) . . . . ? 
Co1 Co2 O20 Mo5 59.60(18) . . . . ? 
Mo10 Co2 O20 Mo5 112.6(2) . . . . ? 
O8 Co2 O20 Mo6 -5.2(2) . . . . ? 
O5 Co2 O20 Mo6 -88.7(2) . . . . ? 
O3 Co2 O20 Mo6 -47(2) . . . . ? 
O32 Co2 O20 Mo6 90.4(2) . . . . ? 
O4 Co2 O20 Mo6 174.6(2) . . . . ? 
Co1 Co2 O20 Mo6 -47.00(16) . . . . ? 
Mo5 Co2 O20 Mo6 -106.6(3) . . . . ? 
Mo10 Co2 O20 Mo6 6.0(3) . . . . ? 
O8 Co2 O20 Mo7 -97.3(2) . . . . ? 
O5 Co2 O20 Mo7 179.1(2) . . . . ? 
O3 Co2 O20 Mo7 -139(2) . . . . ? 
O32 Co2 O20 Mo7 -1.7(2) . . . . ? 
O4 Co2 O20 Mo7 82.5(2) . . . . ? 
Co1 Co2 O20 Mo7 -139.12(16) . . . . ? 
Mo5 Co2 O20 Mo7 161.3(3) . . . . ? 
Mo10 Co2 O20 Mo7 -86.1(2) . . . . ? 
O25 Mo5 O20 Co2 66.0(3) . . . . ? 
O15 Mo5 O20 Co2 173.9(3) . . . . ? 
O16 Mo5 O20 Co2 -71.1(4) . . . . ? 
O7 Mo5 O20 Co2 -86.1(2) . . . . ? 
O5 Mo5 O20 Co2 -14.8(2) . . . . ? 
O25 Mo5 O20 Mo6 169.3(2) . . . . ? 
O15 Mo5 O20 Mo6 -82.7(3) . . . . ? 
O16 Mo5 O20 Mo6 32.3(5) . . . . ? 
O7 Mo5 O20 Mo6 17.25(19) . . . . ? 
O5 Mo5 O20 Mo6 88.5(2) . . . . ? 
Co2 Mo5 O20 Mo6 103.4(3) . . . . ? 
O25 Mo5 O20 Mo7 -72.6(6) . . . . ? 
O15 Mo5 O20 Mo7 35.4(6) . . . . ? 
O16 Mo5 O20 Mo7 150.3(5) . . . . ? 
O7 Mo5 O20 Mo7 135.3(6) . . . . ? 
O5 Mo5 O20 Mo7 -153.4(6) . . . . ? 
Co2 Mo5 O20 Mo7 -138.6(7) . . . . ? 
O29 Mo6 O20 Co2 173.5(3) . . . . ? 
O14 Mo6 O20 Co2 4.1(7) . . . . ? 
O17 Mo6 O20 Co2 -87.2(3) . . . . ? 
O7 Mo6 O20 Co2 84.2(2) . . . . ? 
O8 Mo6 O20 Co2 4.5(2) . . . . ? 
Co1 Mo6 O20 Co2 44.50(17) . . . . ? 
O29 Mo6 O20 Mo5 69.3(3) . . . . ? 
O14 Mo6 O20 Mo5 -100.1(6) . . . . ? 
O17 Mo6 O20 Mo5 168.6(3) . . . . ? 
O7 Mo6 O20 Mo5 -20.0(2) . . . . ? 
O8 Mo6 O20 Mo5 -99.7(2) . . . . ? 
Co1 Mo6 O20 Mo5 -59.70(17) . . . . ? 
O29 Mo6 O20 Mo7 -85.8(2) . . . . ? 
O14 Mo6 O20 Mo7 104.8(6) . . . . ? 
O17 Mo6 O20 Mo7 13.5(2) . . . . ? 
O7 Mo6 O20 Mo7 -175.1(2) . . . . ? 
O8 Mo6 O20 Mo7 105.2(2) . . . . ? 
Co1 Mo6 O20 Mo7 145.18(15) . . . . ? 
O33 Mo7 O20 Co2 35.0(9) . . . . ? 
O34 Mo7 O20 Co2 -172.2(3) . . . . ? 
O31 Mo7 O20 Co2 -71.7(2) . . . . ? 
O17 Mo7 O20 Co2 87.1(3) . . . . ? 
O32 Mo7 O20 Co2 1.5(2) . . . . ? 
O33 Mo7 O20 Mo5 173.7(8) . . . . ? 
O34 Mo7 O20 Mo5 -33.6(6) . . . . ? 
O31 Mo7 O20 Mo5 66.9(6) . . . . ? 
O17 Mo7 O20 Mo5 -134.3(6) . . . . ? 
O32 Mo7 O20 Mo5 140.2(6) . . . . ? 
O33 Mo7 O20 Mo6 -65.2(9) . . . . ? 
O34 Mo7 O20 Mo6 87.6(2) . . . . ? 
O31 Mo7 O20 Mo6 -171.9(2) . . . . ? 
O17 Mo7 O20 Mo6 -13.14(19) . . . . ? 
O32 Mo7 O20 Mo6 -98.7(2) . . . . ? 
O26 Mo1 O21 Mo9 177.4(3) . . . . ? 
O11 Mo1 O21 Mo9 66.7(3) . . . . ? 
O2 Mo1 O21 Mo9 -43.3(6) . . . . ? 
O5 Mo1 O21 Mo9 -92.5(3) . . . . ? 
O3 Mo1 O21 Mo9 -21.4(3) . . . . ? 
Co1 Mo1 O21 Mo9 -84.7(3) . . . . ? 
O12 Mo9 O21 Mo1 -171.0(3) . . . . ? 
O27 Mo9 O21 Mo1 -63.3(3) . . . . ? 
O19 Mo9 O21 Mo1 62.4(6) . . . . ? 
O4 Mo9 O21 Mo1 93.9(3) . . . . ? 
O3 Mo9 O21 Mo1 20.9(2) . . . . ? 
O35 Mo2 O24 Mo3 179.1(3) . . . . ? 
O22 Mo2 O24 Mo3 -71.9(4) . . . . ? 
O9 Mo2 O24 Mo3 43.9(6) . . . . ? 
O1 Mo2 O24 Mo3 18.8(3) . . . . ? 
O2 Mo2 O24 Mo3 89.9(3) . . . . ? 
O18 Mo3 O24 Mo2 177.8(4) . . . . ? 
O38 Mo3 O24 Mo2 68.1(4) . . . . ? 
O13 Mo3 O24 Mo2 -55.5(6) . . . . ? 
O6 Mo3 O24 Mo2 -90.4(3) . . . . ? 
O1 Mo3 O24 Mo2 -18.8(3) . . . . ? 
O12 Mo9 O27 Sm1 167.0(6) . . . . ? 
O19 Mo9 O27 Sm1 -87.8(6) . . . . ? 
O21 Mo9 O27 Sm1 66.5(7) . . . . ? 
O4 Mo9 O27 Sm1 -16.6(12) . . . . ? 
O3 Mo9 O27 Sm1 -6.2(6) . . . . ? 
O4W Sm1 O27 Mo9 -123.5(7) . . . . ? 
O3W Sm1 O27 Mo9 -48.0(8) . . . . ? 
O1W Sm1 O27 Mo9 88.6(7) . . . . ? 
O10 Sm1 O27 Mo9 15.9(7) . . . . ? 
O5W Sm1 O27 Mo9 150.7(7) . . . . ? 
O34 Sm1 O27 Mo9 -158.0(5) 1_455 . . . ? 
O2W Sm1 O27 Mo9 79.5(7) . . . . ? 
O11 Sm1 O27 Mo9 -48.9(6) . . . . ? 
O30 Mo4 O28 Sm2 -35.9(10) . . . . ? 
O13 Mo4 O28 Sm2 67.2(10) . . . . ? 
O16 Mo4 O28 Sm2 -136.8(9) . . . . ? 
O6 Mo4 O28 Sm2 126.0(9) . . . . ? 
O7 Mo4 O28 Sm2 150.7(9) . . . . ? 
O11W Sm2 O28 Mo4 -41.2(9) . . . . ? 
O9W Sm2 O28 Mo4 -121.5(10) . . . . ? 
O10W Sm2 O28 Mo4 164.4(8) . . . . ? 
O12W Sm2 O28 Mo4 20.6(11) . . . . ? 
O8W Sm2 O28 Mo4 163.2(10) . . . . ? 
O6W Sm2 O28 Mo4 96.9(10) . . . . ? 
O38 Sm2 O28 Mo4 -89.5(10) 2_666 . . . ? 
O7W Sm2 O28 Mo4 31.6(9) . . . . ? 
O33 Mo7 O31 Mo8 -72.0(4) . . . . ? 
O34 Mo7 O31 Mo8 -179.0(3) . . . . ? 
O17 Mo7 O31 Mo8 49.4(6) . . . . ? 
O32 Mo7 O31 Mo8 19.9(3) . . . . ? 
O20 Mo7 O31 Mo8 90.3(3) . . . . ? 
O37 Mo8 O31 Mo7 67.5(4) . . . . ? 
O36 Mo8 O31 Mo7 176.0(4) . . . . ? 
O19 Mo8 O31 Mo7 -59.5(6) . . . . ? 
O4 Mo8 O31 Mo7 -91.4(3) . . . . ? 
O32 Mo8 O31 Mo7 -19.8(3) . . . . ? 
O8 Co2 O32 Mo7 90.0(3) . . . . ? 
O5 Co2 O32 Mo7 13(3) . . . . ? 
O3 Co2 O32 Mo7 178.0(2) . . . . ? 
O20 Co2 O32 Mo7 1.8(2) . . . . ? 
O4 Co2 O32 Mo7 -94.9(3) . . . . ? 
Co1 Co2 O32 Mo7 84.4(3) . . . . ? 
Mo5 Co2 O32 Mo7 -11.7(3) . . . . ? 
Mo10 Co2 O32 Mo7 138.2(2) . . . . ? 
O8 Co2 O32 Mo8 -173.6(2) . . . . ? 
O5 Co2 O32 Mo8 110(3) . . . . ? 
O3 Co2 O32 Mo8 -85.5(2) . . . . ? 
O20 Co2 O32 Mo8 98.2(2) . . . . ? 
O4 Co2 O32 Mo8 1.6(2) . . . . ? 
Co1 Co2 O32 Mo8 -179.08(7) . . . . ? 
Mo5 Co2 O32 Mo8 84.8(2) . . . . ? 
Mo10 Co2 O32 Mo8 -125.30(18) . . . . ? 
O33 Mo7 O32 Co2 -171.6(3) . . . . ? 
O34 Mo7 O32 Co2 17.4(9) . . . . ? 
O31 Mo7 O32 Co2 89.2(3) . . . . ? 
O17 Mo7 O32 Co2 -75.7(3) . . . . ? 
O20 Mo7 O32 Co2 -1.5(2) . . . . ? 
O33 Mo7 O32 Mo8 84.4(3) . . . . ? 
O34 Mo7 O32 Mo8 -86.6(7) . . . . ? 
O31 Mo7 O32 Mo8 -14.8(2) . . . . ? 
O17 Mo7 O32 Mo8 -179.7(2) . . . . ? 
O20 Mo7 O32 Mo8 -105.5(2) . . . . ? 
O37 Mo8 O32 Co2 167.8(3) . . . . ? 
O36 Mo8 O32 Co2 -31.3(10) . . . . ? 
O31 Mo8 O32 Co2 -89.3(3) . . . . ? 
O19 Mo8 O32 Co2 70.4(3) . . . . ? 
O4 Mo8 O32 Co2 -1.5(2) . . . . ? 
O37 Mo8 O32 Mo7 -88.1(3) . . . . ? 
O36 Mo8 O32 Mo7 72.8(9) . . . . ? 
O31 Mo8 O32 Mo7 14.7(2) . . . . ? 
O19 Mo8 O32 Mo7 174.5(2) . . . . ? 
O4 Mo8 O32 Mo7 102.6(2) . . . . ? 
O33 Mo7 O34 Sm1 0.2(9) . . . 1_655 ? 
O31 Mo7 O34 Sm1 103.9(8) . . . 1_655 ? 
O17 Mo7 O34 Sm1 -99.6(8) . . . 1_655 ? 
O32 Mo7 O34 Sm1 171.0(5) . . . 1_655 ? 
O20 Mo7 O34 Sm1 -171.3(8) . . . 1_655 ? 
O18 Mo3 O38 Sm2 111.1(8) . . . 2_666 ? 
O24 Mo3 O38 Sm2 -144.9(8) . . . 2_666 ? 
O13 Mo3 O38 Sm2 8.5(8) . . . 2_666 ? 
O6 Mo3 O38 Sm2 -42.6(13) . . . 2_666 ? 
O1 Mo3 O38 Sm2 -73.0(8) . . . 2_666 ? 
 
_diffrn_measured_fraction_theta_max    0.984 
_diffrn_reflns_theta_full              25.00 
_diffrn_measured_fraction_theta_full   0.984 
_refine_diff_density_max    1.946 
_refine_diff_density_min   -1.967 
_refine_diff_density_rms    0.205 


#=====================END 

 
data_2 
 
_audit_creation_method            SHELXL-97 
_chemical_name_systematic 
; 
 ? 
; 
_chemical_name_common             ? 
_chemical_melting_point           ? 
_chemical_formula_moiety          ? 
_chemical_formula_sum 
 'H40 Co2 Eu2 Mo10 O56' 
_chemical_formula_weight          2317.50 
 
loop_ 
 _atom_type_symbol 
 _atom_type_description 
 _atom_type_scat_dispersion_real 
 _atom_type_scat_dispersion_imag 
 _atom_type_scat_source 
 'H'  'H'   0.0000   0.0000 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'O'  'O'   0.0106   0.0060 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Co'  'Co'   0.3494   0.9721 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Mo'  'Mo'  -1.6832   0.6857 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Eu'  'Eu'  -0.1578   3.6682 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 
_symmetry_cell_setting            Triclinic  
_symmetry_space_group_name_H-M    P-1 
 
loop_ 
 _symmetry_equiv_pos_as_xyz 
 'x, y, z' 
 '-x, -y, -z' 
 
_cell_length_a                    12.360(4) 
_cell_length_b                    13.803(4) 
_cell_length_c                    14.183(4) 
_cell_angle_alpha                 74.436(5) 
_cell_angle_beta                  85.442(5) 
_cell_angle_gamma                 89.734(5) 
_cell_volume                      2323.2(12) 
_cell_formula_units_Z             2 
_cell_measurement_temperature     296(2) 
_cell_measurement_reflns_used     11088 
_cell_measurement_theta_min       1.50 
_cell_measurement_theta_max       25.00 
 
_exptl_crystal_description        'plate'
_exptl_crystal_colour             'dark green' 
_exptl_crystal_size_max           0.30 
_exptl_crystal_size_mid           0.16
_exptl_crystal_size_min           0.13 
_exptl_crystal_density_meas       ? 
_exptl_crystal_density_diffrn     3.313 
_exptl_crystal_density_method     'not measured' 
_exptl_crystal_F_000              2176 
_exptl_absorpt_coefficient_mu     6.084 
_exptl_absorpt_correction_type    empirical 
_exptl_absorpt_correction_T_min   0.323 
_exptl_absorpt_correction_T_max   0.453 
_exptl_absorpt_process_details    'ABSCOR by T.Higashi 8 March, 1995' 
 
_exptl_special_details 
; 
 ? 
; 
 
_diffrn_ambient_temperature       296(2) 
_diffrn_radiation_wavelength      0.71073 
_diffrn_radiation_type            MoK\a 
_diffrn_radiation_source          'fine-focus sealed tube' 
_diffrn_radiation_monochromator   graphite 
_diffrn_measurement_device_type   'Bruker Smart Apex CCD' 
_diffrn_measurement_method        'ω-2θ' 
_diffrn_detector_area_resol_mean  0.01 
_diffrn_standards_number          0 
_diffrn_standards_interval_count  0 
_diffrn_standards_interval_time   0
_diffrn_standards_decay_%         none 
_diffrn_reflns_number             11088 
_diffrn_reflns_av_R_equivalents   0.0581 
_diffrn_reflns_av_sigmaI/netI     0.1156 
_diffrn_reflns_limit_h_min        -9 
_diffrn_reflns_limit_h_max        14 
_diffrn_reflns_limit_k_min        -13 
_diffrn_reflns_limit_k_max        16 
_diffrn_reflns_limit_l_min        -16 
_diffrn_reflns_limit_l_max        16 
_diffrn_reflns_theta_min          1.50 
_diffrn_reflns_theta_max          25.00 
_reflns_number_total              7967 
_reflns_number_gt                 5499 
_reflns_threshold_expression      >2sigma(I) 
 
_computing_data_collection        ? 
_computing_cell_refinement        ? 
_computing_data_reduction         ? 
_computing_structure_solution     'SHELXS-97 (Sheldrick, 1990)' 
_computing_structure_refinement   'SHELXL-97 (Sheldrick, 1997)' 
_computing_molecular_graphics     'Bruker SHELXTL'
_computing_publication_material   'Bruker SHELXTL' 
 
_refine_special_details 
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
; 
 
_refine_ls_structure_factor_coef  Fsqd  
_refine_ls_matrix_type            full 
_refine_ls_weighting_scheme       calc  
_refine_ls_weighting_details 
 'calc w=1/[σ²(Fo²)+(0.0331P)²+363.8127P] where P=(Fo²+2Fc²)/3' 
_atom_sites_solution_primary      direct 
_atom_sites_solution_secondary    difmap 
_atom_sites_solution_hydrogens    '.'
_refine_ls_hydrogen_treatment     none
_refine_ls_extinction_method      none 
_refine_ls_extinction_coef        ? 
_refine_ls_number_reflns          7967 
_refine_ls_number_parameters      640 
_refine_ls_number_restraints      174 
_refine_ls_R_factor_all           0.1363 
_refine_ls_R_factor_gt            0.0977 
_refine_ls_wR_factor_ref          0.2496 
_refine_ls_wR_factor_gt           0.2268 
_refine_ls_goodness_of_fit_ref    1.072 
_refine_ls_restrained_S_all       1.064 
_refine_ls_shift/su_max           0.000 
_refine_ls_shift/su_mean          0.000 
 
loop_ 
 _atom_site_label 
 _atom_site_type_symbol 
 _atom_site_fract_x 
 _atom_site_fract_y 
 _atom_site_fract_z 
 _atom_site_U_iso_or_equiv 
 _atom_site_adp_type 
 _atom_site_occupancy 
 _atom_site_symmetry_multiplicity 
 _atom_site_calc_flag 
 _atom_site_refinement_flags 
 _atom_site_disorder_assembly 
 _atom_site_disorder_group 
Eu1 Eu 0.66497(11) 0.92658(11) 0.26177(10) 0.0235(4) Uani 1 1 d . . . 
Eu2 Eu -0.21173(12) 1.45070(12) 0.19366(11) 0.0300(4) Uani 1 1 d . . . 
Mo1 Mo 0.06277(18) 1.12776(18) 0.12307(17) 0.0204(5) Uani 1 1 d . . . 
Mo2 Mo 0.10016(19) 1.36516(18) 0.24382(18) 0.0239(6) Uani 1 1 d . . . 
Mo3 Mo 0.3106(2) 1.43720(19) 0.08321(19) 0.0282(6) Uani 1 1 d . . . 
Mo4 Mo 0.47253(19) 1.2654(2) 0.03493(18) 0.0285(6) Uani 1 1 d . . . 
Mo5 Mo 0.40604(18) 1.02942(19) 0.12608(17) 0.0207(5) Uani 1 1 d . . . 
Mo6 Mo 0.42462(18) 1.10482(18) 0.32757(17) 0.0196(5) Uani 1 1 d . . . 
Mo7 Mo 0.38342(18) 0.86639(19) 0.42317(18) 0.0233(6) Uani 1 1 d . . . 
Mo8 Mo 0.1665(2) 0.75732(19) 0.3793(2) 0.0296(6) Uani 1 1 d . . . 
Mo9 Mo -0.00443(19) 0.89441(19) 0.23675(18) 0.0240(6) Uani 1 1 d . . . 
Mo10 Mo 0.06528(18) 1.12775(18) 0.35953(17) 0.0202(5) Uani 1 1 d . . . 
Co1 Co 0.2629(3) 1.1987(3) 0.1896(3) 0.0179(8) Uani 1 1 d . . . 
Co2 Co 0.2179(3) 0.9971(3) 0.2774(3) 0.0168(8) Uani 1 1 d . . . 
O1 O 0.3672(16) 0.8040(17) 0.5434(16) 0.040(6) Uani 1 1 d . . . 
O2 O 0.3591(16) 0.9367(17) 0.0834(15) 0.035(5) Uani 1 1 d . . . 
O3 O 0.3347(19) 1.5310(18) 0.1354(18) 0.048(6) Uani 1 1 d U . . 
O4 O 0.1113(15) 1.1898(14) 0.0099(13) 0.026(4) Uani 1 1 d . . . 
O5 O 0.6004(17) 1.2386(18) 0.0615(16) 0.042(6) Uani 1 1 d U . . 
O6 O 0.2920(14) 1.2818(15) 0.0584(14) 0.028(5) Uani 1 1 d . . . 
O7 O 0.0412(15) 0.9959(15) 0.1172(14) 0.029(5) Uani 1 1 d . . . 
O8 O 0.2094(14) 0.9051(14) 0.4084(13) 0.026(4) Uani 1 1 d . . . 
O9 O -0.0358(14) 1.3740(14) 0.2296(13) 0.025(4) Uani 1 1 d U . . 
O10 O 0.4201(15) 1.1418(16) 0.0150(14) 0.031(5) Uani 1 1 d . . . 
O11 O 0.1555(15) 1.4209(15) 0.1113(15) 0.029(5) Uani 1 1 d U . . 
O12 O 0.4509(16) 1.3764(15) 0.0915(15) 0.033(5) Uani 1 1 d . . . 
O13 O 0.4111(13) 1.1657(14) 0.1859(12) 0.021(4) Uani 1 1 d . . . 
O14 O 0.5568(14) 1.0699(16) 0.3093(14) 0.030(5) Uani 1 1 d . . . 
O15 O 0.2472(14) 1.1124(14) 0.3146(13) 0.020(4) Uani 1 1 d . . . 
O16 O 0.3242(15) 0.7750(14) 0.3644(14) 0.026(4) Uani 1 1 d U . . 
O17 O 0.1468(19) 0.6989(18) 0.4995(16) 0.050(7) Uani 1 1 d . . . 
O18 O 0.0693(14) 1.0292(13) 0.2804(12) 0.018(4) Uani 1 1 d . . . 
O19 O -0.0201(18) 0.7999(17) 0.1844(17) 0.043(6) Uani 1 1 d . . . 
O20 O 0.1056(14) 1.2592(14) 0.3624(13) 0.022(4) Uani 1 1 d U . . 
O21 O 0.1775(14) 0.8821(14) 0.2374(14) 0.024(4) Uani 1 1 d . . . 
O22 O 0.2776(14) 1.3209(13) 0.2280(13) 0.021(4) Uani 1 1 d U . . 
O23 O 0.4255(17) 1.2083(16) 0.3677(15) 0.036(5) Uani 1 1 d . . . 
O24 O 0.3855(14) 1.0006(15) 0.4411(13) 0.024(4) Uani 1 1 d . . . 
O25 O 0.0278(15) 0.8186(14) 0.3654(14) 0.028(5) Uani 1 1 d . . . 
O26 O 0.2382(13) 1.0834(13) 0.1518(12) 0.017(4) Uani 1 1 d . . . 
O27 O 0.3688(14) 0.9802(14) 0.2685(12) 0.021(4) Uani 1 1 d . . . 
O28 O 0.1588(18) 0.6666(16) 0.3196(19) 0.046(6) Uani 1 1 d . . . 
O29 O 0.1275(19) 1.4602(15) 0.2908(18) 0.044(6) Uani 1 1 d . . . 
O30 O 0.3059(14) 1.4910(15) -0.0394(15) 0.032(5) Uani 1 1 d . . . 
O31 O 0.4776(16) 1.3259(18) -0.0853(16) 0.043(6) Uani 1 1 d . . . 
O32 O -0.0718(15) 1.1373(16) 0.3661(14) 0.030(5) Uani 1 1 d U . . 
O33 O 0.0942(15) 1.0587(16) 0.4728(13) 0.030(5) Uani 1 1 d . . . 
O34 O -0.0699(15) 1.1633(16) 0.1347(15) 0.033(5) Uani 1 1 d U . . 
O35 O 0.5388(14) 1.0037(14) 0.1431(13) 0.023(4) Uani 1 1 d U . . 
O36 O 0.5196(15) 0.8620(15) 0.3852(17) 0.036(5) Uani 1 1 d . . . 
O37 O 0.1118(13) 1.2156(14) 0.2002(12) 0.020(4) Uani 1 1 d . . . 
O38 O -0.1338(16) 0.9329(16) 0.2603(16) 0.037(5) Uani 1 1 d . . . 
O1W O 0.7257(16) 0.9491(17) 0.4067(14) 0.035(5) Uani 1 1 d U . . 
O2W O 0.544(2) 0.802(2) 0.220(2) 0.068(8) Uani 1 1 d U . . 
O3W O 0.7195(19) 0.7567(19) 0.3338(17) 0.046(6) Uani 1 1 d U . . 
O4W O 0.742(2) 0.891(2) 0.111(2) 0.068(8) Uani 1 1 d U . . 
O5W O 0.7332(18) 1.0900(18) 0.1698(17) 0.045(6) Uani 1 1 d U . . 
O6W O -0.275(2) 1.436(2) 0.365(2) 0.065(8) Uani 1 1 d U . . 
O7W O -0.4033(19) 1.406(2) 0.2191(18) 0.051(6) Uani 1 1 d U . . 
O8W O -0.100(2) 1.561(2) 0.264(2) 0.061(7) Uani 1 1 d U . . 
O9W O -0.1705(19) 1.3493(17) 0.0819(17) 0.044(6) Uani 1 1 d U . . 
O10W O -0.0872(17) 1.5526(17) 0.0694(16) 0.041(5) Uani 1 1 d U . . 
O11W O -0.298(2) 1.611(2) 0.1922(19) 0.057(7) Uani 1 1 d U . . 
O12W O -0.2318(17) 1.2715(17) 0.2852(16) 0.041(5) Uani 1 1 d U . . 
OW1 O -0.095(2) 1.357(2) -0.1155(19) 0.058(7) Uani 1 1 d U . . 
OW2 O 0.181(4) 0.839(4) 0.051(4) 0.148(18) Uani 1 1 d U . . 
OW3 O 0.475(4) 1.389(4) 0.404(4) 0.144(17) Uani 1 1 d U . . 
OW4 O 0.577(3) 0.596(3) 0.400(3) 0.096(11) Uani 1 1 d U . . 
OW5 O 0.142(2) 1.298(2) 0.529(2) 0.070(8) Uani 1 1 d U . . 
OW6 O 0.414(5) 0.620(5) 0.282(4) 0.070(16) Uani 0.50 1 d PU . . 
OW7 O 0.076(6) 1.480(5) 0.542(5) 0.09(2) Uani 0.50 1 d PU . . 
 
 
_geom_special_details 
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
; 
 
loop_ 
 _geom_bond_atom_site_label_1 
 _geom_bond_atom_site_label_2 
 _geom_bond_distance 
 _geom_bond_site_symmetry_2 
 _geom_bond_publ_flag 
Eu1 O1W 2.34(2) . ? 
Eu1 O5W 2.40(2) . ? 
Eu1 O36 2.40(2) . ? 
Eu1 O3W 2.41(2) . ? 
Eu1 O35 2.417(16) . ? 
Eu1 O4W 2.44(3) . ? 
Eu1 O38 2.487(19) 1_655 ? 
Eu1 O2W 2.50(3) . ? 
Eu1 O14 2.59(2) . ? 
Eu2 O10W 2.39(2) . ? 
Eu2 O9W 2.41(2) . ? 
Eu2 O7W 2.42(2) . ? 
Eu2 O9 2.444(16) . ? 
Eu2 O11W 2.44(3) . ? 
Eu2 O6W 2.44(3) . ? 
Eu2 O12W 2.47(2) . ? 
Eu2 O30 2.50(2) 2_585 ? 
Eu2 O8W 2.51(3) . ? 
Mo1 O4 1.669(18) . ? 
Mo1 O34 1.717(19) . ? 
Mo1 O7 1.87(2) . ? 
Mo1 O37 1.964(18) . ? 
Mo1 O18 2.288(16) . ? 
Mo1 O26 2.288(16) . ? 
Mo1 Co1 2.976(4) . ? 
Mo2 O29 1.67(2) . ? 
Mo2 O9 1.708(17) . ? 
Mo2 O11 1.90(2) . ? 
Mo2 O20 1.916(18) . ? 
Mo2 O22 2.284(18) . ? 
Mo2 O37 2.309(18) . ? 
Mo3 O3 1.69(2) . ? 
Mo3 O30 1.70(2) . ? 
Mo3 O12 1.921(19) . ? 
Mo3 O11 1.928(19) . ? 
Mo3 O22 2.250(18) . ? 
Mo3 O6 2.28(2) . ? 
Mo4 O5 1.67(2) . ? 
Mo4 O31 1.68(2) . ? 
Mo4 O12 1.92(2) . ? 
Mo4 O10 1.93(2) . ? 
Mo4 O6 2.249(17) . ? 
Mo4 O13 2.286(18) . ? 
Mo5 O2 1.68(2) . ? 
Mo5 O35 1.699(17) . ? 
Mo5 O10 1.89(2) . ? 
Mo5 O27 1.968(17) . ? 
Mo5 O26 2.237(16) . ? 
Mo5 O13 2.265(19) . ? 
Mo5 Co2 2.986(4) . ? 
Mo6 O23 1.67(2) . ? 
Mo6 O14 1.721(18) . ? 
Mo6 O24 1.880(19) . ? 
Mo6 O13 1.979(17) . ? 
Mo6 O15 2.215(17) . ? 
Mo6 O27 2.239(19) . ? 
Mo6 Co1 2.957(4) . ? 
Mo7 O1 1.69(2) . ? 
Mo7 O36 1.732(19) . ? 
Mo7 O16 1.868(19) . ? 
Mo7 O24 1.94(2) . ? 
Mo7 O8 2.226(17) . ? 
Mo7 O27 2.350(16) . ? 
Mo8 O17 1.68(2) . ? 
Mo8 O28 1.70(2) . ? 
Mo8 O25 1.908(18) . ? 
Mo8 O16 1.954(19) . ? 
Mo8 O8 2.26(2) . ? 
Mo8 O21 2.266(19) . ? 
Mo9 O19 1.68(2) . ? 
Mo9 O38 1.719(19) . ? 
Mo9 O25 1.916(17) . ? 
Mo9 O7 1.93(2) . ? 
Mo9 O21 2.255(18) . ? 
Mo9 O18 2.324(18) . ? 
Mo10 O32 1.695(18) . ? 
Mo10 O33 1.698(18) . ? 
Mo10 O20 1.895(18) . ? 
Mo10 O18 1.980(18) . ? 
Mo10 O37 2.289(18) . ? 
Mo10 O15 2.312(17) . ? 
Mo10 Co2 2.986(4) . ? 
Co1 O26 1.845(18) . ? 
Co1 O15 1.849(18) . ? 
Co1 O37 1.880(16) . ? 
Co1 O13 1.886(16) . ? 
Co1 O6 1.912(19) . ? 
Co1 O22 1.920(18) . ? 
Co1 Co2 2.766(5) . ? 
Co2 O15 1.852(18) . ? 
Co2 O26 1.857(17) . ? 
Co2 O27 1.877(17) . ? 
Co2 O18 1.887(17) . ? 
Co2 O21 1.905(18) . ? 
Co2 O8 1.944(18) . ? 
O30 Eu2 2.50(2) 2_585 ? 
O38 Eu1 2.487(19) 1_455 ? 
 
loop_ 
 _geom_angle_atom_site_label_1 
 _geom_angle_atom_site_label_2 
 _geom_angle_atom_site_label_3 
 _geom_angle 
 _geom_angle_site_symmetry_1 
 _geom_angle_site_symmetry_3 
 _geom_angle_publ_flag 
O1W Eu1 O5W 91.4(8) . . ? 
O1W Eu1 O36 75.2(7) . . ? 
O5W Eu1 O36 136.1(7) . . ? 
O1W Eu1 O3W 81.5(8) . . ? 
O5W Eu1 O3W 142.9(8) . . ? 
O36 Eu1 O3W 77.2(7) . . ? 
O1W Eu1 O35 138.1(7) . . ? 
O5W Eu1 O35 70.6(7) . . ? 
O36 Eu1 O35 91.7(7) . . ? 
O3W Eu1 O35 134.9(7) . . ? 
O1W Eu1 O4W 138.1(8) . . ? 
O5W Eu1 O4W 78.9(9) . . ? 
O36 Eu1 O4W 137.3(9) . . ? 
O3W Eu1 O4W 82.5(9) . . ? 
O35 Eu1 O4W 76.8(8) . . ? 
O1W Eu1 O38 66.6(7) . 1_655 ? 
O5W Eu1 O38 70.0(7) . 1_655 ? 
O36 Eu1 O38 134.7(7) . 1_655 ? 
O3W Eu1 O38 73.9(8) . 1_655 ? 
O35 Eu1 O38 133.2(7) . 1_655 ? 
O4W Eu1 O38 71.8(8) . 1_655 ? 
O1W Eu1 O2W 135.3(9) . . ? 
O5W Eu1 O2W 132.2(9) . . ? 
O36 Eu1 O2W 66.3(9) . . ? 
O3W Eu1 O2W 68.8(9) . . ? 
O35 Eu1 O2W 66.8(8) . . ? 
O4W Eu1 O2W 71.4(10) . . ? 
O38 Eu1 O2W 129.9(9) 1_655 . ? 
O1W Eu1 O14 71.0(6) . . ? 
O5W Eu1 O14 67.8(7) . . ? 
O36 Eu1 O14 68.3(6) . . ? 
O3W Eu1 O14 140.1(7) . . ? 
O35 Eu1 O14 67.2(6) . . ? 
O4W Eu1 O14 137.0(8) . . ? 
O38 Eu1 O14 117.8(7) 1_655 . ? 
O2W Eu1 O14 112.3(8) . . ? 
O10W Eu2 O9W 75.9(8) . . ? 
O10W Eu2 O7W 138.9(8) . . ? 
O9W Eu2 O7W 94.6(8) . . ? 
O10W Eu2 O9 76.0(7) . . ? 
O9W Eu2 O9 72.5(7) . . ? 
O7W Eu2 O9 139.9(8) . . ? 
O10W Eu2 O11W 84.0(8) . . ? 
O9W Eu2 O11W 138.3(8) . . ? 
O7W Eu2 O11W 77.1(9) . . ? 
O9 Eu2 O11W 137.0(8) . . ? 
O10W Eu2 O6W 138.1(9) . . ? 
O9W Eu2 O6W 141.3(9) . . ? 
O7W Eu2 O6W 70.7(9) . . ? 
O9 Eu2 O6W 95.6(8) . . ? 
O11W Eu2 O6W 74.7(9) . . ? 
O10W Eu2 O12W 137.0(7) . . ? 
O9W Eu2 O12W 71.1(8) . . ? 
O7W Eu2 O12W 71.5(8) . . ? 
O9 Eu2 O12W 68.4(7) . . ? 
O11W Eu2 O12W 138.9(8) . . ? 
O6W Eu2 O12W 70.3(9) . . ? 
O10W Eu2 O30 71.6(7) . 2_585 ? 
O9W Eu2 O30 67.6(7) . 2_585 ? 
O7W Eu2 O30 67.8(7) . 2_585 ? 
O9 Eu2 O30 133.2(6) . 2_585 ? 
O11W Eu2 O30 71.6(8) . 2_585 ? 
O6W Eu2 O30 130.9(8) . 2_585 ? 
O12W Eu2 O30 117.8(7) . 2_585 ? 
O10W Eu2 O8W 69.2(8) . . ? 
O9W Eu2 O8W 133.7(9) . . ? 
O7W Eu2 O8W 131.7(9) . . ? 
O9 Eu2 O8W 70.3(8) . . ? 
O11W Eu2 O8W 67.1(9) . . ? 
O6W Eu2 O8W 69.4(10) . . ? 
O12W Eu2 O8W 117.4(8) . . ? 
O30 Eu2 O8W 124.8(8) 2_585 . ? 
O4 Mo1 O34 106.0(9) . . ? 
O4 Mo1 O7 104.8(9) . . ? 
O34 Mo1 O7 99.7(9) . . ? 
O4 Mo1 O37 101.3(9) . . ? 
O34 Mo1 O37 92.8(9) . . ? 
O7 Mo1 O37 146.5(7) . . ? 
O4 Mo1 O18 156.7(7) . . ? 
O34 Mo1 O18 97.0(8) . . ? 
O7 Mo1 O18 74.2(7) . . ? 
O37 Mo1 O18 73.5(7) . . ? 
O4 Mo1 O26 86.5(7) . . ? 
O34 Mo1 O26 164.0(8) . . ? 
O7 Mo1 O26 86.3(7) . . ? 
O37 Mo1 O26 74.7(6) . . ? 
O18 Mo1 O26 70.2(6) . . ? 
O4 Mo1 Co1 86.0(6) . . ? 
O34 Mo1 Co1 130.9(7) . . ? 
O7 Mo1 Co1 123.5(5) . . ? 
O37 Mo1 Co1 38.3(5) . . ? 
O18 Mo1 Co1 76.0(4) . . ? 
O26 Mo1 Co1 38.3(4) . . ? 
O29 Mo2 O9 104.1(10) . . ? 
O29 Mo2 O11 99.9(11) . . ? 
O9 Mo2 O11 99.7(8) . . ? 
O29 Mo2 O20 97.2(9) . . ? 
O9 Mo2 O20 102.5(8) . . ? 
O11 Mo2 O20 147.7(8) . . ? 
O29 Mo2 O22 94.2(9) . . ? 
O9 Mo2 O22 161.0(8) . . ? 
O11 Mo2 O22 71.5(7) . . ? 
O20 Mo2 O22 80.1(7) . . ? 
O29 Mo2 O37 162.1(8) . . ? 
O9 Mo2 O37 92.6(8) . . ? 
O11 Mo2 O37 83.1(7) . . ? 
O20 Mo2 O37 72.7(7) . . ? 
O22 Mo2 O37 69.9(6) . . ? 
O3 Mo3 O30 107.0(11) . . ? 
O3 Mo3 O12 98.8(10) . . ? 
O30 Mo3 O12 103.2(9) . . ? 
O3 Mo3 O11 100.4(10) . . ? 
O30 Mo3 O11 95.4(8) . . ? 
O12 Mo3 O11 148.0(8) . . ? 
O3 Mo3 O22 94.0(9) . . ? 
O30 Mo3 O22 157.2(9) . . ? 
O12 Mo3 O22 81.6(7) . . ? 
O11 Mo3 O22 71.8(7) . . ? 
O3 Mo3 O6 162.5(9) . . ? 
O30 Mo3 O6 90.0(9) . . ? 
O12 Mo3 O6 72.7(8) . . ? 
O11 Mo3 O6 81.6(7) . . ? 
O22 Mo3 O6 69.9(7) . . ? 
O5 Mo4 O31 106.6(10) . . ? 
O5 Mo4 O12 99.1(10) . . ? 
O31 Mo4 O12 100.5(10) . . ? 
O5 Mo4 O10 102.7(10) . . ? 
O31 Mo4 O10 93.2(10) . . ? 
O12 Mo4 O10 149.6(8) . . ? 
O5 Mo4 O6 159.3(9) . . ? 
O31 Mo4 O6 93.8(9) . . ? 
O12 Mo4 O6 73.4(8) . . ? 
O10 Mo4 O6 78.8(8) . . ? 
O5 Mo4 O13 90.0(9) . . ? 
O31 Mo4 O13 160.7(9) . . ? 
O12 Mo4 O13 86.1(8) . . ? 
O10 Mo4 O13 73.2(7) . . ? 
O6 Mo4 O13 70.5(6) . . ? 
O2 Mo5 O35 105.6(9) . . ? 
O2 Mo5 O10 104.3(10) . . ? 
O35 Mo5 O10 100.5(8) . . ? 
O2 Mo5 O27 102.9(10) . . ? 
O35 Mo5 O27 90.2(8) . . ? 
O10 Mo5 O27 146.7(8) . . ? 
O2 Mo5 O26 91.9(8) . . ? 
O35 Mo5 O26 159.1(8) . . ? 
O10 Mo5 O26 85.8(7) . . ? 
O27 Mo5 O26 74.4(6) . . ? 
O2 Mo5 O13 161.3(8) . . ? 
O35 Mo5 O13 92.9(8) . . ? 
O10 Mo5 O13 74.3(8) . . ? 
O27 Mo5 O13 73.8(7) . . ? 
O26 Mo5 O13 69.5(6) . . ? 
O2 Mo5 Co2 90.2(7) . . ? 
O35 Mo5 Co2 128.2(6) . . ? 
O10 Mo5 Co2 123.3(6) . . ? 
O27 Mo5 Co2 38.0(5) . . ? 
O26 Mo5 Co2 38.4(4) . . ? 
O13 Mo5 Co2 75.9(5) . . ? 
O23 Mo6 O14 108.3(11) . . ? 
O23 Mo6 O24 104.1(9) . . ? 
O14 Mo6 O24 97.3(8) . . ? 
O23 Mo6 O13 100.4(9) . . ? 
O14 Mo6 O13 93.5(8) . . ? 
O24 Mo6 O13 148.4(8) . . ? 
O23 Mo6 O15 92.3(9) . . ? 
O14 Mo6 O15 158.3(9) . . ? 
O24 Mo6 O15 83.5(7) . . ? 
O13 Mo6 O15 75.9(7) . . ? 
O23 Mo6 O27 161.9(8) . . ? 
O14 Mo6 O27 89.4(8) . . ? 
O24 Mo6 O27 76.4(7) . . ? 
O13 Mo6 O27 74.1(7) . . ? 
O15 Mo6 O27 69.7(6) . . ? 
O23 Mo6 Co1 89.3(7) . . ? 
O14 Mo6 Co1 132.2(6) . . ? 
O24 Mo6 Co1 121.5(5) . . ? 
O13 Mo6 Co1 38.9(5) . . ? 
O15 Mo6 Co1 38.6(5) . . ? 
O27 Mo6 Co1 75.5(4) . . ? 
O1 Mo7 O36 107.5(10) . . ? 
O1 Mo7 O16 102.0(10) . . ? 
O36 Mo7 O16 100.7(9) . . ? 
O1 Mo7 O24 96.7(10) . . ? 
O36 Mo7 O24 97.4(9) . . ? 
O16 Mo7 O24 148.7(7) . . ? 
O1 Mo7 O8 95.7(8) . . ? 
O36 Mo7 O8 156.8(9) . . ? 
O16 Mo7 O8 73.4(8) . . ? 
O24 Mo7 O8 80.0(7) . . ? 
O1 Mo7 O27 164.5(9) . . ? 
O36 Mo7 O27 85.5(8) . . ? 
O16 Mo7 O27 83.4(7) . . ? 
O24 Mo7 O27 72.7(7) . . ? 
O8 Mo7 O27 71.7(6) . . ? 
O17 Mo8 O28 106.2(13) . . ? 
O17 Mo8 O25 97.1(10) . . ? 
O28 Mo8 O25 103.0(10) . . ? 
O17 Mo8 O16 100.8(10) . . ? 
O28 Mo8 O16 97.6(10) . . ? 
O25 Mo8 O16 147.7(8) . . ? 
O17 Mo8 O8 92.5(10) . . ? 
O28 Mo8 O8 159.8(10) . . ? 
O25 Mo8 O8 81.5(7) . . ? 
O16 Mo8 O8 71.1(7) . . ? 
O17 Mo8 O21 160.2(10) . . ? 
O28 Mo8 O21 92.6(10) . . ? 
O25 Mo8 O21 72.1(7) . . ? 
O16 Mo8 O21 82.4(7) . . ? 
O8 Mo8 O21 69.8(6) . . ? 
O19 Mo9 O38 105.1(11) . . ? 
O19 Mo9 O25 99.8(10) . . ? 
O38 Mo9 O25 101.0(9) . . ? 
O19 Mo9 O7 96.6(10) . . ? 
O38 Mo9 O7 100.7(9) . . ? 
O25 Mo9 O7 148.2(8) . . ? 
O19 Mo9 O21 95.1(9) . . ? 
O38 Mo9 O21 159.6(9) . . ? 
O25 Mo9 O21 72.2(8) . . ? 
O7 Mo9 O21 79.3(7) . . ? 
O19 Mo9 O18 162.0(9) . . ? 
O38 Mo9 O18 91.1(9) . . ? 
O25 Mo9 O18 84.4(7) . . ? 
O7 Mo9 O18 72.2(7) . . ? 
O21 Mo9 O18 69.4(6) . . ? 
O32 Mo10 O33 105.2(9) . . ? 
O32 Mo10 O20 100.2(9) . . ? 
O33 Mo10 O20 101.6(9) . . ? 
O32 Mo10 O18 94.8(9) . . ? 
O33 Mo10 O18 104.1(9) . . ? 
O20 Mo10 O18 145.6(8) . . ? 
O32 Mo10 O37 101.5(8) . . ? 
O33 Mo10 O37 153.3(8) . . ? 
O20 Mo10 O37 73.6(7) . . ? 
O18 Mo10 O37 73.2(7) . . ? 
O32 Mo10 O15 166.9(8) . . ? 
O33 Mo10 O15 85.4(8) . . ? 
O20 Mo10 O15 84.8(7) . . ? 
O18 Mo10 O15 74.9(7) . . ? 
O37 Mo10 O15 68.1(6) . . ? 
O32 Mo10 Co2 132.9(7) . . ? 
O33 Mo10 Co2 87.3(7) . . ? 
O20 Mo10 Co2 122.0(6) . . ? 
O18 Mo10 Co2 38.3(5) . . ? 
O37 Mo10 Co2 74.2(4) . . ? 
O15 Mo10 Co2 38.3(4) . . ? 
O26 Co1 O15 83.4(8) . . ? 
O26 Co1 O37 88.2(8) . . ? 
O15 Co1 O37 87.4(7) . . ? 
O26 Co1 O13 86.9(8) . . ? 
O15 Co1 O13 87.6(8) . . ? 
O37 Co1 O13 173.3(8) . . ? 
O26 Co1 O6 94.6(8) . . ? 
O15 Co1 O6 174.5(8) . . ? 
O37 Co1 O6 97.7(7) . . ? 
O13 Co1 O6 87.2(7) . . ? 
O26 Co1 O22 175.8(7) . . ? 
O15 Co1 O22 97.1(8) . . ? 
O37 Co1 O22 87.7(8) . . ? 
O13 Co1 O22 97.3(8) . . ? 
O6 Co1 O22 85.2(8) . . ? 
O26 Co1 Co2 41.8(5) . . ? 
O15 Co1 Co2 41.7(6) . . ? 
O37 Co1 Co2 85.9(6) . . ? 
O13 Co1 Co2 87.4(6) . . ? 
O6 Co1 Co2 136.3(7) . . ? 
O22 Co1 Co2 138.4(6) . . ? 
O26 Co1 Mo6 94.1(5) . . ? 
O15 Co1 Mo6 48.4(5) . . ? 
O37 Co1 Mo6 134.9(5) . . ? 
O13 Co1 Mo6 41.3(5) . . ? 
O6 Co1 Mo6 126.8(5) . . ? 
O22 Co1 Mo6 89.3(5) . . ? 
Co2 Co1 Mo6 67.52(11) . . ? 
O26 Co1 Mo1 50.2(5) . . ? 
O15 Co1 Mo1 95.3(5) . . ? 
O37 Co1 Mo1 40.3(6) . . ? 
O13 Co1 Mo1 136.0(6) . . ? 
O6 Co1 Mo1 87.3(6) . . ? 
O22 Co1 Mo1 125.6(5) . . ? 
Co2 Co1 Mo1 67.60(11) . . ? 
Mo6 Co1 Mo1 135.12(15) . . ? 
O15 Co2 O26 83.1(8) . . ? 
O15 Co2 O27 86.1(8) . . ? 
O26 Co2 O27 86.2(7) . . ? 
O15 Co2 O18 89.1(8) . . ? 
O26 Co2 O18 89.3(7) . . ? 
O27 Co2 O18 173.8(8) . . ? 
O15 Co2 O21 175.9(8) . . ? 
O26 Co2 O21 96.1(8) . . ? 
O27 Co2 O21 97.9(8) . . ? 
O18 Co2 O21 86.9(8) . . ? 
O15 Co2 O8 96.6(8) . . ? 
O26 Co2 O8 175.3(7) . . ? 
O27 Co2 O8 89.1(7) . . ? 
O18 Co2 O8 95.4(7) . . ? 
O21 Co2 O8 84.6(8) . . ? 
O15 Co2 Co1 41.6(6) . . ? 
O26 Co2 Co1 41.5(5) . . ? 
O27 Co2 Co1 86.0(6) . . ? 
O18 Co2 Co1 87.8(5) . . ? 
O21 Co2 Co1 137.3(6) . . ? 
O8 Co2 Co1 138.1(6) . . ? 
O15 Co2 Mo5 94.0(6) . . ? 
O26 Co2 Mo5 48.4(5) . . ? 
O27 Co2 Mo5 40.2(5) . . ? 
O18 Co2 Mo5 136.6(5) . . ? 
O21 Co2 Mo5 88.4(6) . . ? 
O8 Co2 Mo5 127.0(5) . . ? 
Co1 Co2 Mo5 67.48(12) . . ? 
O15 Co2 Mo10 50.7(5) . . ? 
O26 Co2 Mo10 96.3(5) . . ? 
O27 Co2 Mo10 135.7(6) . . ? 
O18 Co2 Mo10 40.6(5) . . ? 
O21 Co2 Mo10 125.5(6) . . ? 
O8 Co2 Mo10 87.1(6) . . ? 
Co1 Co2 Mo10 68.67(12) . . ? 
Mo5 Co2 Mo10 136.15(14) . . ? 
Co1 O6 Mo4 101.3(7) . . ? 
Co1 O6 Mo3 102.0(9) . . ? 
Mo4 O6 Mo3 92.5(7) . . ? 
Mo1 O7 Mo9 118.7(10) . . ? 
Co2 O8 Mo7 100.8(8) . . ? 
Co2 O8 Mo8 102.2(8) . . ? 
Mo7 O8 Mo8 93.3(7) . . ? 
Mo2 O9 Eu2 159.3(11) . . ? 
Mo5 O10 Mo4 116.8(9) . . ? 
Mo2 O11 Mo3 118.3(9) . . ? 
Mo4 O12 Mo3 116.8(10) . . ? 
Co1 O13 Mo6 99.8(8) . . ? 
Co1 O13 Mo5 100.5(8) . . ? 
Mo6 O13 Mo5 102.6(8) . . ? 
Co1 O13 Mo4 100.8(7) . . ? 
Mo6 O13 Mo4 152.6(9) . . ? 
Mo5 O13 Mo4 91.1(6) . . ? 
Mo6 O14 Eu1 139.8(11) . . ? 
Co1 O15 Co2 96.7(8) . . ? 
Co1 O15 Mo6 92.9(7) . . ? 
Co2 O15 Mo6 102.7(8) . . ? 
Co1 O15 Mo10 102.1(7) . . ? 
Co2 O15 Mo10 90.9(7) . . ? 
Mo6 O15 Mo10 158.4(9) . . ? 
Mo7 O16 Mo8 117.2(10) . . ? 
Co2 O18 Mo10 101.1(8) . . ? 
Co2 O18 Mo1 99.6(8) . . ? 
Mo10 O18 Mo1 103.4(7) . . ? 
Co2 O18 Mo9 100.9(7) . . ? 
Mo10 O18 Mo9 151.7(9) . . ? 
Mo1 O18 Mo9 90.3(6) . . ? 
Mo10 O20 Mo2 117.6(9) . . ? 
Co2 O21 Mo9 102.8(8) . . ? 
Co2 O21 Mo8 103.3(8) . . ? 
Mo9 O21 Mo8 92.8(7) . . ? 
Co1 O22 Mo3 102.8(8) . . ? 
Co1 O22 Mo2 101.0(8) . . ? 
Mo3 O22 Mo2 93.0(6) . . ? 
Mo6 O24 Mo7 115.6(9) . . ? 
Mo8 O25 Mo9 117.8(10) . . ? 
Co1 O26 Co2 96.7(8) . . ? 
Co1 O26 Mo5 102.8(8) . . ? 
Co2 O26 Mo5 93.2(7) . . ? 
Co1 O26 Mo1 91.5(7) . . ? 
Co2 O26 Mo1 100.5(7) . . ? 
Mo5 O26 Mo1 158.9(8) . . ? 
Co2 O27 Mo5 101.9(7) . . ? 
Co2 O27 Mo6 101.0(8) . . ? 
Mo5 O27 Mo6 103.9(8) . . ? 
Co2 O27 Mo7 98.5(7) . . ? 
Mo5 O27 Mo7 152.9(9) . . ? 
Mo6 O27 Mo7 89.5(6) . . ? 
Mo3 O30 Eu2 154.0(10) . 2_585 ? 
Mo5 O35 Eu1 144.7(10) . . ? 
Mo7 O36 Eu1 147.5(11) . . ? 
Co1 O37 Mo1 101.4(8) . . ? 
Co1 O37 Mo10 101.9(7) . . ? 
Mo1 O37 Mo10 103.9(8) . . ? 
Co1 O37 Mo2 101.3(8) . . ? 
Mo1 O37 Mo2 149.9(8) . . ? 
Mo10 O37 Mo2 90.3(6) . . ? 
Mo9 O38 Eu1 154.5(12) . 1_455 ? 
 
_diffrn_measured_fraction_theta_max    0.973 
_diffrn_reflns_theta_full              25.00 
_diffrn_measured_fraction_theta_full   0.973 
_refine_diff_density_max    3.532 
_refine_diff_density_min   -3.401 
_refine_diff_density_rms    0.441 


#=====================END 

 
data_3 
 
_audit_creation_method            SHELXL-97 
_chemical_name_systematic 
; 
 ? 
; 
_chemical_name_common             ? 
_chemical_melting_point           ? 
_chemical_formula_moiety          ? 
_chemical_formula_sum 
 'H40 Co2 Mo10 N3 O50 Sm' 
_chemical_formula_weight          2109.96 
 
loop_ 
 _atom_type_symbol 
 _atom_type_description 
 _atom_type_scat_dispersion_real 
 _atom_type_scat_dispersion_imag 
 _atom_type_scat_source 
 'N'  'N'   0.0061   0.0033 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'H'  'H'   0.0000   0.0000 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'O'  'O'   0.0106   0.0060 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Co'  'Co'   0.3494   0.9721 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Mo'  'Mo'  -1.6832   0.6857 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Sm'  'Sm'  -0.1638   3.4418 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 
_symmetry_cell_setting            Monoclinic 
_symmetry_space_group_name_H-M    P2(1) 
 
loop_ 
 _symmetry_equiv_pos_as_xyz 
 'x, y, z' 
 '-x, y+1/2, -z' 
 
_cell_length_a                    10.5118(5) 
_cell_length_b                    18.6632(8) 
_cell_length_c                    12.2190(6) 
_cell_angle_alpha                 90.00 
_cell_angle_beta                  114.115(2) 
_cell_angle_gamma                 90.00 
_cell_volume                      2187.96(18) 
_cell_formula_units_Z             2 
_cell_measurement_temperature     296(2) 
_cell_measurement_reflns_used     9942 
_cell_measurement_theta_min       2.12  
_cell_measurement_theta_max       25.00 
 
_exptl_crystal_description        'block' 
_exptl_crystal_colour             'dark green'  
_exptl_crystal_size_max           0.24 
_exptl_crystal_size_mid           0.20
_exptl_crystal_size_min           0.18 
_exptl_crystal_density_meas       ? 
_exptl_crystal_density_diffrn     3.203 
_exptl_crystal_density_method     'not measured' 
_exptl_crystal_F_000              1994 
_exptl_absorpt_coefficient_mu     4.948 
_exptl_absorpt_correction_type    empirical 
_exptl_absorpt_correction_T_min   0.317 
_exptl_absorpt_correction_T_max   0.410  
_exptl_absorpt_process_details    'ABSCOR by T.Higashi 8 March, 1995' 
 
_exptl_special_details 
; 
 ? 
; 
 
_diffrn_ambient_temperature       296(2) 
_diffrn_radiation_wavelength      0.71073 
_diffrn_radiation_type            MoK\a 
_diffrn_radiation_source          'fine-focus sealed tube' 
_diffrn_radiation_monochromator   graphite 
_diffrn_measurement_device_type   'Bruker Smart Apex CCD' 
_diffrn_measurement_method        'ω-2θ' 
_diffrn_detector_area_resol_mean  0.01
_diffrn_standards_number          0 
_diffrn_standards_interval_count  0 
_diffrn_standards_interval_time   0
_diffrn_standards_decay_%         none  
_diffrn_reflns_number             9942 
_diffrn_reflns_av_R_equivalents   0.0000 
_diffrn_reflns_av_sigmaI/netI     0.0575 
_diffrn_reflns_limit_h_min        -8 
_diffrn_reflns_limit_h_max        12 
_diffrn_reflns_limit_k_min        -20 
_diffrn_reflns_limit_k_max        22 
_diffrn_reflns_limit_l_min        -14 
_diffrn_reflns_limit_l_max        12 
_diffrn_reflns_theta_min          2.12 
_diffrn_reflns_theta_max          25.00 
_reflns_number_total              9942 
_reflns_number_gt                 9820 
_reflns_threshold_expression      >2sigma(I) 
 
_computing_data_collection        ? 
_computing_cell_refinement        ? 
_computing_data_reduction         ? 
_computing_structure_solution     'SHELXS-97 (Sheldrick, 1990)' 
_computing_structure_refinement   'SHELXL-97 (Sheldrick, 1997)' 
_computing_molecular_graphics     'Bruker SHELXTL' 
_computing_publication_material   'Bruker SHELXTL' 
 
_refine_special_details 
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
; 
 
_refine_ls_structure_factor_coef  Fsqd  
_refine_ls_matrix_type            full 
_refine_ls_weighting_scheme       calc  
_refine_ls_weighting_details 
 'calc w=1/[σ²(Fo²)+(0.0262P)²+0.0000P] where P=(Fo²+2Fc²)/3' 
_atom_sites_solution_primary      direct 
_atom_sites_solution_secondary    difmap 
_atom_sites_solution_hydrogens    '.'
_refine_ls_hydrogen_treatment     'constr' 
_refine_ls_extinction_method      none 
_refine_ls_extinction_coef        ? 
_refine_ls_abs_structure_details 
 'Flack H D (1983), Acta Cryst. A39, 876-881' 
_refine_ls_abs_structure_Flack    0.025(8) 
_refine_ls_number_reflns          9942 
_refine_ls_number_parameters      605 
_refine_ls_number_restraints      31 
_refine_ls_R_factor_all           0.0283 
_refine_ls_R_factor_gt            0.0280 
_refine_ls_wR_factor_ref          0.0745 
_refine_ls_wR_factor_gt           0.0743 
_refine_ls_goodness_of_fit_ref    1.046 
_refine_ls_restrained_S_all       1.049 
_refine_ls_shift/su_max           0.002 
_refine_ls_shift/su_mean          0.000 
 
loop_ 
 _atom_site_label 
 _atom_site_type_symbol 
 _atom_site_fract_x 
 _atom_site_fract_y 
 _atom_site_fract_z 
 _atom_site_U_iso_or_equiv 
 _atom_site_adp_type 
 _atom_site_occupancy 
 _atom_site_symmetry_multiplicity 
 _atom_site_calc_flag 
 _atom_site_refinement_flags 
 _atom_site_disorder_assembly 
 _atom_site_disorder_group 
Sm1 Sm 0.56388(4) 0.916544(19) 0.35744(3) 0.01579(9) Uani 1 1 d . . . 
Mo1 Mo 0.57117(6) 1.12730(3) 0.29799(5) 0.01190(13) Uani 1 1 d . . . 
Mo2 Mo 0.48144(6) 1.03251(3) 0.05424(6) 0.01380(14) Uani 1 1 d . . . 
Mo3 Mo 0.64128(7) 1.05677(3) -0.12407(6) 0.01782(15) Uani 1 1 d . . . 
Mo4 Mo 0.89490(7) 1.17750(3) -0.04129(5) 0.01437(14) Uani 1 1 d . . . 
Mo5 Mo 1.01936(6) 1.24489(3) 0.23150(5) 0.01338(14) Uani 1 1 d . . . 
Mo6 Mo 0.68677(6) 1.30302(3) 0.11073(5) 0.01264(14) Uani 1 1 d . . . 
Mo7 Mo 0.81238(7) 1.38600(3) 0.37131(6) 0.01676(15) Uani 1 1 d . . . 
Mo8 Mo 0.93311(6) 1.28992(3) 0.61995(5) 0.01437(14) Uani 1 1 d . . . 
Mo9 Mo 0.94804(7) 1.11388(3) 0.60025(6) 0.01571(14) Uani 1 1 d . . . 
Mo10 Mo 0.86914(6) 1.03986(3) 0.33752(5) 0.01166(13) Uani 1 1 d . . . 
Co1 Co 0.74108(10) 1.14314(5) 0.13429(8) 0.0103(2) Uani 1 1 d . . . 
Co2 Co 0.83018(10) 1.21035(5) 0.35621(9) 0.0104(2) Uani 1 1 d . . . 
O1 O 0.9549(5) 1.0009(3) 0.2614(5) 0.0214(12) Uani 1 1 d . . . 
O2 O 0.8821(5) 1.2887(3) 0.2839(4) 0.0148(11) Uani 1 1 d . . . 
O3 O 0.7434(6) 0.9995(3) -0.1612(5) 0.0307(14) Uani 1 1 d . . . 
O4 O 0.9074(6) 1.2608(3) -0.0921(5) 0.0269(13) Uani 1 1 d . . . 
O5 O 0.7702(5) 1.1280(2) 0.4117(4) 0.0139(11) Uani 1 1 d . . . 
O6 O 0.8260(5) 1.0873(2) 0.0485(5) 0.0160(11) Uani 1 1 d . . . 
O7 O 0.4349(5) 1.1121(3) 0.1396(4) 0.0158(11) Uani 1 1 d . . . 
O8 O 0.6866(5) 1.0666(2) 0.2023(4) 0.0127(11) Uani 1 1 d U . . 
O9 O 1.0636(6) 1.3231(3) 0.1858(5) 0.0266(13) Uani 1 1 d . . . 
O10 O 0.7820(5) 0.9719(3) 0.3743(5) 0.0216(12) Uani 1 1 d . . . 
O11 O 0.7110(5) 1.1508(3) -0.1459(5) 0.0197(12) Uani 1 1 d . . . 
O12 O 0.9033(5) 1.1480(2) 0.2756(4) 0.0121(10) Uani 1 1 d . . . 
O13 O 0.9937(6) 1.1241(3) -0.0897(5) 0.0277(13) Uani 1 1 d . . . 
O14 O 0.6670(5) 1.2037(2) 0.2158(4) 0.0126(11) Uani 1 1 d . . . 
O15 O 0.3229(5) 1.0344(3) -0.0601(5) 0.0275(13) Uani 1 1 d . . . 
O16 O 0.5051(6) 1.1951(3) 0.3510(5) 0.0221(12) Uani 1 1 d . . . 
O17 O 0.5946(5) 0.9941(2) -0.0201(5) 0.0188(12) Uani 1 1 d . . . 
O18 O 0.4866(6) 1.0598(3) -0.2464(5) 0.0344(14) Uani 1 1 d . . . 
O19 O 0.8636(5) 1.1965(3) 0.6365(5) 0.0164(11) Uani 1 1 d . . . 
O20 O 0.9691(5) 1.3565(3) 0.5160(5) 0.0171(11) Uani 1 1 d . . . 
O21 O 0.9931(5) 1.2102(2) 0.5069(4) 0.0129(11) Uani 1 1 d . . . 
O22 O 1.0060(5) 1.0642(2) 0.4852(5) 0.0171(11) Uani 1 1 d . . . 
O23 O 0.5708(5) 1.1253(2) -0.0059(4) 0.0126(10) Uani 1 1 d . . . 
O24 O 0.8580(6) 1.0485(3) 0.6334(5) 0.0302(14) Uani 1 1 d . . . 
O25 O 1.0958(5) 1.2881(3) 0.7330(5) 0.0266(13) Uani 1 1 d . . . 
O26 O 0.6511(5) 1.3576(3) 0.2235(5) 0.0192(12) Uani 1 1 d . . . 
O27 O 1.1071(6) 1.1147(3) 0.7148(5) 0.0298(13) Uani 1 1 d . . . 
O28 O 1.1540(6) 1.2247(3) 0.3678(5) 0.0243(13) Uani 1 1 d . . . 
O29 O 0.7231(6) 1.4386(3) 0.4293(5) 0.0305(14) Uani 1 1 d . . . 
O30 O 0.5249(5) 1.2831(3) 0.0051(5) 0.0265(13) Uani 1 1 d . . . 
O31 O 0.4731(6) 0.9652(3) 0.1496(5) 0.0218(12) Uani 1 1 d . . . 
O32 O 0.7480(5) 1.3658(3) 0.0445(5) 0.0204(12) Uani 1 1 d . . . 
O33 O 0.8341(6) 1.3406(3) 0.6712(5) 0.0257(13) Uani 1 1 d . . . 
O34 O 1.0449(5) 1.1815(3) 0.1227(4) 0.0181(11) Uani 1 1 d . . . 
O35 O 0.5403(5) 1.0489(2) 0.3582(4) 0.0158(11) Uani 1 1 d . . . 
O36 O 0.8968(6) 1.4424(3) 0.3144(5) 0.0288(14) Uani 1 1 d . . . 
O37 O 0.8028(5) 1.2262(2) 0.0807(4) 0.0129(11) Uani 1 1 d . . . 
O38 O 0.7575(5) 1.2801(2) 0.4331(4) 0.0130(11) Uani 1 1 d . . . 
O1W O 0.5030(6) 0.8223(3) 0.4690(5) 0.0289(14) Uani 1 1 d . . . 
O2W O 0.3340(6) 0.9580(3) 0.3472(6) 0.0328(14) Uani 1 1 d . . . 
O3W O 0.6429(7) 0.8424(4) 0.2284(7) 0.053(2) Uani 1 1 d . . . 
O4W O 0.6215(7) 0.9629(3) 0.5618(5) 0.0372(16) Uani 1 1 d . . . 
O5W O 0.3711(6) 0.8387(3) 0.2150(5) 0.0374(15) Uani 1 1 d . . . 
O6W O 0.7698(6) 0.8475(3) 0.4800(6) 0.0403(17) Uani 1 1 d . . . 
OW1 O 0.4148(7) 0.6881(3) 0.3842(5) 0.0413(16) Uani 1 1 d . . . 
OW2 O 1.0368(7) 0.9768(3) -0.1222(7) 0.0481(18) Uani 1 1 d . . . 
OW3 O 0.9926(7) 1.4091(3) -0.0842(6) 0.0494(18) Uani 1 1 d . . . 
OW4 O 0.5842(7) 0.8574(3) 0.7098(6) 0.0419(16) Uani 1 1 d . . . 
OW5 O 0.3443(11) 1.0848(4) -0.5057(9) 0.088(3) Uani 1 1 d . . . 
OW6 O 0.1999(8) 1.0569(4) 0.1761(9) 0.077(3) Uani 1 1 d . . . 
N1 N 1.2702(10) 1.3594(5) 0.0210(10) 0.066(3) Uani 1 1 d U . . 
N2 N 0.2558(11) 1.2113(6) -0.0359(12) 0.088(4) Uani 1 1 d U . . 
N3 N 0.6350(15) 0.6908(7) 0.2229(16) 0.057(4) Uani 0.60 1 d PU . . 
N4 N 0.701(2) 0.6929(11) 0.350(2) 0.051(6) Uani 0.40 1 d PU . . 
 
 
_geom_special_details 
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
; 
 
loop_ 
 _geom_bond_atom_site_label_1 
 _geom_bond_atom_site_label_2 
 _geom_bond_distance 
 _geom_bond_site_symmetry_2 
 _geom_bond_publ_flag 
Sm1 O6W 2.437(6) . ? 
Sm1 O10 2.446(5) . ? 
Sm1 O1W 2.465(5) . ? 
Sm1 O4W 2.473(6) . ? 
Sm1 O3W 2.483(7) . ? 
Sm1 O35 2.483(5) . ? 
Sm1 O31 2.491(5) . ? 
Sm1 O2W 2.491(6) . ? 
Sm1 O5W 2.523(6) . ? 
Mo1 O16 1.694(5) . ? 
Mo1 O35 1.727(5) . ? 
Mo1 O7 1.901(5) . ? 
Mo1 O5 1.983(5) . ? 
Mo1 O14 2.210(5) . ? 
Mo1 O8 2.298(5) . ? 
Mo1 Co2 2.9562(11) . ? 
Mo2 O15 1.682(5) . ? 
Mo2 O31 1.740(5) . ? 
Mo2 O17 1.907(5) . ? 
Mo2 O7 1.987(5) . ? 
Mo2 O23 2.233(5) . ? 
Mo2 O8 2.268(5) . ? 
Mo3 O18 1.702(5) . ? 
Mo3 O3 1.702(6) . ? 
Mo3 O17 1.931(5) . ? 
Mo3 O11 1.962(5) . ? 
Mo3 O23 2.268(5) . ? 
Mo3 O6 2.279(5) . ? 
Mo4 O4 1.699(5) . ? 
Mo4 O13 1.710(5) . ? 
Mo4 O11 1.897(5) . ? 
Mo4 O34 1.981(5) . ? 
Mo4 O37 2.272(5) . ? 
Mo4 O6 2.283(5) . ? 
Mo5 O9 1.694(5) . ? 
Mo5 O28 1.730(5) . ? 
Mo5 O34 1.879(5) . ? 
Mo5 O2 1.980(5) . ? 
Mo5 O37 2.296(5) . ? 
Mo5 O12 2.363(5) . ? 
Mo5 Co2 3.0279(12) . ? 
Mo6 O32 1.694(5) . ? 
Mo6 O30 1.704(5) . ? 
Mo6 O26 1.871(5) . ? 
Mo6 O37 2.011(5) . ? 
Mo6 O2 2.284(5) . ? 
Mo6 O14 2.311(5) . ? 
Mo6 Co1 3.0294(11) . ? 
Mo7 O36 1.698(5) . ? 
Mo7 O29 1.700(5) . ? 
Mo7 O20 1.939(5) . ? 
Mo7 O26 1.979(5) . ? 
Mo7 O38 2.273(5) . ? 
Mo7 O2 2.369(5) . ? 
Mo8 O33 1.704(5) . ? 
Mo8 O25 1.704(5) . ? 
Mo8 O20 1.923(5) . ? 
Mo8 O19 1.932(5) . ? 
Mo8 O38 2.282(5) . ? 
Mo8 O21 2.287(5) . ? 
Mo9 O27 1.687(5) . ? 
Mo9 O24 1.693(5) . ? 
Mo9 O19 1.919(5) . ? 
Mo9 O22 1.976(5) . ? 
Mo9 O21 2.280(5) . ? 
Mo9 O5 2.314(5) . ? 
Mo10 O1 1.700(5) . ? 
Mo10 O10 1.728(5) . ? 
Mo10 O22 1.847(5) . ? 
Mo10 O8 2.017(5) . ? 
Mo10 O12 2.236(5) . ? 
Mo10 O5 2.320(5) . ? 
Mo10 Co1 2.9938(11) . ? 
Co1 O8 1.857(4) . ? 
Co1 O12 1.869(5) . ? 
Co1 O14 1.873(5) . ? 
Co1 O37 1.897(4) . ? 
Co1 O23 1.935(5) . ? 
Co1 O6 1.936(5) . ? 
Co1 Co2 2.7798(13) . ? 
Co2 O14 1.870(5) . ? 
Co2 O12 1.879(5) . ? 
Co2 O5 1.889(5) . ? 
Co2 O2 1.900(5) . ? 
Co2 O21 1.936(5) . ? 
Co2 O38 1.936(5) . ? 
N3 N4 1.41(3) . ? 
 
loop_ 
 _geom_angle_atom_site_label_1 
 _geom_angle_atom_site_label_2 
 _geom_angle_atom_site_label_3 
 _geom_angle 
 _geom_angle_site_symmetry_1 
 _geom_angle_site_symmetry_3 
 _geom_angle_publ_flag 
O6W Sm1 O10 66.73(18) . . ? 
O6W Sm1 O1W 69.45(19) . . ? 
O10 Sm1 O1W 134.54(18) . . ? 
O6W Sm1 O4W 77.0(2) . . ? 
O10 Sm1 O4W 86.1(2) . . ? 
O1W Sm1 O4W 72.7(2) . . ? 
O6W Sm1 O3W 69.6(2) . . ? 
O10 Sm1 O3W 75.1(2) . . ? 
O1W Sm1 O3W 100.6(2) . . ? 
O4W Sm1 O3W 146.0(2) . . ? 
O6W Sm1 O35 126.06(19) . . ? 
O10 Sm1 O35 70.78(16) . . ? 
O1W Sm1 O35 131.24(17) . . ? 
O4W Sm1 O35 68.40(18) . . ? 
O3W Sm1 O35 128.1(2) . . ? 
O6W Sm1 O31 133.9(2) . . ? 
O10 Sm1 O31 83.52(17) . . ? 
O1W Sm1 O31 138.26(18) . . ? 
O4W Sm1 O31 137.37(18) . . ? 
O3W Sm1 O31 69.1(2) . . ? 
O35 Sm1 O31 69.13(16) . . ? 
O6W Sm1 O2W 142.7(2) . . ? 
O10 Sm1 O2W 136.85(18) . . ? 
O1W Sm1 O2W 77.52(19) . . ? 
O4W Sm1 O2W 77.0(2) . . ? 
O3W Sm1 O2W 135.3(2) . . ? 
O35 Sm1 O2W 66.10(17) . . ? 
O31 Sm1 O2W 82.86(19) . . ? 
O6W Sm1 O5W 112.4(2) . . ? 
O10 Sm1 O5W 139.7(2) . . ? 
O1W Sm1 O5W 69.7(2) . . ? 
O4W Sm1 O5W 134.0(2) . . ? 
O3W Sm1 O5W 67.9(2) . . ? 
O35 Sm1 O5W 121.48(18) . . ? 
O31 Sm1 O5W 68.99(18) . . ? 
O2W Sm1 O5W 69.8(2) . . ? 
O16 Mo1 O35 107.0(2) . . ? 
O16 Mo1 O7 104.2(2) . . ? 
O35 Mo1 O7 96.4(2) . . ? 
O16 Mo1 O5 101.9(2) . . ? 
O35 Mo1 O5 92.0(2) . . ? 
O7 Mo1 O5 148.7(2) . . ? 
O16 Mo1 O14 91.5(2) . . ? 
O35 Mo1 O14 160.1(2) . . ? 
O7 Mo1 O14 85.85(19) . . ? 
O5 Mo1 O14 76.57(18) . . ? 
O16 Mo1 O8 161.2(2) . . ? 
O35 Mo1 O8 91.7(2) . . ? 
O7 Mo1 O8 75.13(19) . . ? 
O5 Mo1 O8 74.59(18) . . ? 
O14 Mo1 O8 69.72(17) . . ? 
O16 Mo1 Co2 89.85(18) . . ? 
O35 Mo1 Co2 131.04(16) . . ? 
O7 Mo1 Co2 124.08(15) . . ? 
O5 Mo1 Co2 39.06(14) . . ? 
O14 Mo1 Co2 39.19(12) . . ? 
O8 Mo1 Co2 75.81(12) . . ? 
O15 Mo2 O31 105.5(3) . . ? 
O15 Mo2 O17 102.2(3) . . ? 
O31 Mo2 O17 105.1(2) . . ? 
O15 Mo2 O7 92.7(2) . . ? 
O31 Mo2 O7 95.6(2) . . ? 
O17 Mo2 O7 150.0(2) . . ? 
O15 Mo2 O23 96.8(2) . . ? 
O31 Mo2 O23 157.5(2) . . ? 
O17 Mo2 O23 72.92(19) . . ? 
O7 Mo2 O23 79.65(19) . . ? 
O15 Mo2 O8 162.5(2) . . ? 
O31 Mo2 O8 87.7(2) . . ? 
O17 Mo2 O8 84.9(2) . . ? 
O7 Mo2 O8 74.29(18) . . ? 
O23 Mo2 O8 69.76(16) . . ? 
O18 Mo3 O3 105.5(3) . . ? 
O18 Mo3 O17 100.9(3) . . ? 
O3 Mo3 O17 98.8(2) . . ? 
O18 Mo3 O11 97.3(3) . . ? 
O3 Mo3 O11 102.4(2) . . ? 
O17 Mo3 O11 147.2(2) . . ? 
O18 Mo3 O23 95.5(2) . . ? 
O3 Mo3 O23 158.3(2) . . ? 
O17 Mo3 O23 71.69(18) . . ? 
O11 Mo3 O23 79.57(19) . . ? 
O18 Mo3 O6 162.1(2) . . ? 
O3 Mo3 O6 90.7(2) . . ? 
O17 Mo3 O6 83.8(2) . . ? 
O11 Mo3 O6 71.2(2) . . ? 
O23 Mo3 O6 69.30(16) . . ? 
O4 Mo4 O13 105.0(3) . . ? 
O4 Mo4 O11 101.7(2) . . ? 
O13 Mo4 O11 102.1(3) . . ? 
O4 Mo4 O34 100.8(2) . . ? 
O13 Mo4 O34 91.6(2) . . ? 
O11 Mo4 O34 149.6(2) . . ? 
O4 Mo4 O37 89.5(2) . . ? 
O13 Mo4 O37 160.3(2) . . ? 
O11 Mo4 O37 87.5(2) . . ? 
O34 Mo4 O37 72.41(19) . . ? 
O4 Mo4 O6 159.7(2) . . ? 
O13 Mo4 O6 95.3(2) . . ? 
O11 Mo4 O6 72.2(2) . . ? 
O34 Mo4 O6 79.6(2) . . ? 
O37 Mo4 O6 71.09(16) . . ? 
O9 Mo5 O28 106.2(3) . . ? 
O9 Mo5 O34 99.9(3) . . ? 
O28 Mo5 O34 104.3(2) . . ? 
O9 Mo5 O2 94.9(2) . . ? 
O28 Mo5 O2 101.3(2) . . ? 
O34 Mo5 O2 145.4(2) . . ? 
O9 Mo5 O37 100.5(2) . . ? 
O28 Mo5 O37 153.2(2) . . ? 
O34 Mo5 O37 73.61(19) . . ? 
O2 Mo5 O37 73.01(18) . . ? 
O9 Mo5 O12 166.2(2) . . ? 
O28 Mo5 O12 84.8(2) . . ? 
O34 Mo5 O12 85.21(19) . . ? 
O2 Mo5 O12 74.29(18) . . ? 
O37 Mo5 O12 68.40(16) . . ? 
O9 Mo5 Co2 132.41(19) . . ? 
O28 Mo5 Co2 85.20(19) . . ? 
O34 Mo5 Co2 122.36(16) . . ? 
O2 Mo5 Co2 37.76(14) . . ? 
O37 Mo5 Co2 74.46(12) . . ? 
O12 Mo5 Co2 38.35(11) . . ? 
O32 Mo6 O30 104.2(3) . . ? 
O32 Mo6 O26 101.8(2) . . ? 
O30 Mo6 O26 103.7(2) . . ? 
O32 Mo6 O37 91.6(2) . . ? 
O30 Mo6 O37 101.5(2) . . ? 
O26 Mo6 O37 147.3(2) . . ? 
O32 Mo6 O2 98.7(2) . . ? 
O30 Mo6 O2 156.6(2) . . ? 
O26 Mo6 O2 75.88(19) . . ? 
O37 Mo6 O2 72.74(18) . . ? 
O32 Mo6 O14 163.4(2) . . ? 
O30 Mo6 O14 87.6(2) . . ? 
O26 Mo6 O14 86.4(2) . . ? 
O37 Mo6 O14 74.26(18) . . ? 
O2 Mo6 O14 69.03(16) . . ? 
O32 Mo6 Co1 129.29(18) . . ? 
O30 Mo6 Co1 87.05(19) . . ? 
O26 Mo6 Co1 123.58(15) . . ? 
O37 Mo6 Co1 37.85(13) . . ? 
O2 Mo6 Co1 74.55(12) . . ? 
O14 Mo6 Co1 38.17(12) . . ? 
O36 Mo7 O29 106.4(3) . . ? 
O36 Mo7 O20 99.1(3) . . ? 
O29 Mo7 O20 101.1(3) . . ? 
O36 Mo7 O26 100.9(3) . . ? 
O29 Mo7 O26 97.0(3) . . ? 
O20 Mo7 O26 148.0(2) . . ? 
O36 Mo7 O38 157.1(2) . . ? 
O29 Mo7 O38 96.0(2) . . ? 
O20 Mo7 O38 71.77(18) . . ? 
O26 Mo7 O38 80.29(19) . . ? 
O36 Mo7 O2 88.9(2) . . ? 
O29 Mo7 O2 162.8(2) . . ? 
O20 Mo7 O2 83.65(19) . . ? 
O26 Mo7 O2 72.01(18) . . ? 
O38 Mo7 O2 69.54(16) . . ? 
O33 Mo8 O25 106.0(3) . . ? 
O33 Mo8 O20 101.4(2) . . ? 
O25 Mo8 O20 98.3(2) . . ? 
O33 Mo8 O19 98.6(2) . . ? 
O25 Mo8 O19 101.2(2) . . ? 
O20 Mo8 O19 146.9(2) . . ? 
O33 Mo8 O38 92.6(2) . . ? 
O25 Mo8 O38 160.6(2) . . ? 
O20 Mo8 O38 71.83(18) . . ? 
O19 Mo8 O38 81.15(19) . . ? 
O33 Mo8 O21 160.7(2) . . ? 
O25 Mo8 O21 92.5(2) . . ? 
O20 Mo8 O21 81.04(19) . . ? 
O19 Mo8 O21 71.67(19) . . ? 
O38 Mo8 O21 69.75(16) . . ? 
O27 Mo9 O24 105.7(3) . . ? 
O27 Mo9 O19 101.3(2) . . ? 
O24 Mo9 O19 99.7(2) . . ? 
O27 Mo9 O22 96.1(2) . . ? 
O24 Mo9 O22 101.4(2) . . ? 
O19 Mo9 O22 147.9(2) . . ? 
O27 Mo9 O21 94.0(2) . . ? 
O24 Mo9 O21 160.0(2) . . ? 
O19 Mo9 O21 72.0(2) . . ? 
O22 Mo9 O21 80.03(19) . . ? 
O27 Mo9 O5 161.7(2) . . ? 
O24 Mo9 O5 91.0(2) . . ? 
O19 Mo9 O5 82.90(19) . . ? 
O22 Mo9 O5 72.76(19) . . ? 
O21 Mo9 O5 70.16(16) . . ? 
O1 Mo10 O10 106.5(2) . . ? 
O1 Mo10 O22 105.3(2) . . ? 
O10 Mo10 O22 102.1(2) . . ? 
O1 Mo10 O8 101.4(2) . . ? 
O10 Mo10 O8 88.1(2) . . ? 
O22 Mo10 O8 147.1(2) . . ? 
O1 Mo10 O12 90.4(2) . . ? 
O10 Mo10 O12 157.8(2) . . ? 
O22 Mo10 O12 86.55(19) . . ? 
O8 Mo10 O12 74.33(18) . . ? 
O1 Mo10 O5 160.0(2) . . ? 
O10 Mo10 O5 92.8(2) . . ? 
O22 Mo10 O5 74.83(19) . . ? 
O8 Mo10 O5 73.49(18) . . ? 
O12 Mo10 O5 69.58(17) . . ? 
O1 Mo10 Co1 88.92(17) . . ? 
O10 Mo10 Co1 125.57(18) . . ? 
O22 Mo10 Co1 123.98(15) . . ? 
O8 Mo10 Co1 37.48(13) . . ? 
O12 Mo10 Co1 38.55(12) . . ? 
O5 Mo10 Co1 75.28(12) . . ? 
O8 Co1 O12 87.5(2) . . ? 
O8 Co1 O14 87.4(2) . . ? 
O12 Co1 O14 84.2(2) . . ? 
O8 Co1 O37 174.0(2) . . ? 
O12 Co1 O37 88.1(2) . . ? 
O14 Co1 O37 88.0(2) . . ? 
O8 Co1 O23 85.5(2) . . ? 
O12 Co1 O23 172.5(2) . . ? 
O14 Co1 O23 98.0(2) . . ? 
O37 Co1 O23 99.1(2) . . ? 
O8 Co1 O6 97.1(2) . . ? 
O12 Co1 O6 94.5(2) . . ? 
O14 Co1 O6 175.3(2) . . ? 
O37 Co1 O6 87.4(2) . . ? 
O23 Co1 O6 83.8(2) . . ? 
O8 Co1 Co2 87.30(15) . . ? 
O12 Co1 Co2 42.26(15) . . ? 
O14 Co1 Co2 42.00(14) . . ? 
O37 Co1 Co2 86.67(15) . . ? 
O23 Co1 Co2 139.68(15) . . ? 
O6 Co1 Co2 136.48(16) . . ? 
O8 Co1 Mo10 41.38(14) . . ? 
O12 Co1 Mo10 48.22(14) . . ? 
O14 Co1 Mo10 95.25(14) . . ? 
O37 Co1 Mo10 135.32(15) . . ? 
O23 Co1 Mo10 124.30(14) . . ? 
O6 Co1 Mo10 87.25(15) . . ? 
Co2 Co1 Mo10 67.87(3) . . ? 
O8 Co1 Mo6 136.02(15) . . ? 
O12 Co1 Mo6 96.03(14) . . ? 
O14 Co1 Mo6 49.68(15) . . ? 
O37 Co1 Mo6 40.58(15) . . ? 
O23 Co1 Mo6 90.86(14) . . ? 
O6 Co1 Mo6 126.12(14) . . ? 
Co2 Co1 Mo6 67.89(3) . . ? 
Mo10 Co1 Mo6 135.76(4) . . ? 
O14 Co2 O12 84.1(2) . . ? 
O14 Co2 O5 87.7(2) . . ? 
O12 Co2 O5 87.3(2) . . ? 
O14 Co2 O2 87.4(2) . . ? 
O12 Co2 O2 88.6(2) . . ? 
O5 Co2 O2 173.9(2) . . ? 
O14 Co2 O21 175.0(2) . . ? 
O12 Co2 O21 96.0(2) . . ? 
O5 Co2 O21 87.3(2) . . ? 
O2 Co2 O21 97.6(2) . . ? 
O14 Co2 O38 95.4(2) . . ? 
O12 Co2 O38 175.9(2) . . ? 
O5 Co2 O38 96.7(2) . . ? 
O2 Co2 O38 87.3(2) . . ? 
O21 Co2 O38 84.9(2) . . ? 
O14 Co2 Co1 42.10(15) . . ? 
O12 Co2 Co1 41.98(14) . . ? 
O5 Co2 Co1 87.37(15) . . ? 
O2 Co2 Co1 86.58(15) . . ? 
O21 Co2 Co1 137.90(15) . . ? 
O38 Co2 Co1 137.25(15) . . ? 
O14 Co2 Mo1 48.33(15) . . ? 
O12 Co2 Mo1 94.77(14) . . ? 
O5 Co2 Mo1 41.41(15) . . ? 
O2 Co2 Mo1 134.65(15) . . ? 
O21 Co2 Mo1 126.74(15) . . ? 
O38 Co2 Mo1 87.82(14) . . ? 
Co1 Co2 Mo1 67.58(3) . . ? 
O14 Co2 Mo5 95.57(16) . . ? 
O12 Co2 Mo5 51.30(14) . . ? 
O5 Co2 Mo5 137.57(15) . . ? 
O2 Co2 Mo5 39.64(14) . . ? 
O21 Co2 Mo5 88.36(15) . . ? 
O38 Co2 Mo5 124.87(14) . . ? 
Co1 Co2 Mo5 68.53(3) . . ? 
Mo1 Co2 Mo5 136.07(4) . . ? 
Co2 O2 Mo5 102.6(2) . . ? 
Co2 O2 Mo6 101.6(2) . . ? 
Mo5 O2 Mo6 104.3(2) . . ? 
Co2 O2 Mo7 100.4(2) . . ? 
Mo5 O2 Mo7 149.7(2) . . ? 
Mo6 O2 Mo7 90.09(16) . . ? 
Co2 O5 Mo1 99.5(2) . . ? 
Co2 O5 Mo9 101.4(2) . . ? 
Mo1 O5 Mo9 152.7(2) . . ? 
Co2 O5 Mo10 99.7(2) . . ? 
Mo1 O5 Mo10 103.6(2) . . ? 
Mo9 O5 Mo10 89.95(17) . . ? 
Co1 O6 Mo3 103.2(2) . . ? 
Co1 O6 Mo4 99.80(19) . . ? 
Mo3 O6 Mo4 93.30(18) . . ? 
Mo1 O7 Mo2 113.7(2) . . ? 
Co1 O8 Mo10 101.1(2) . . ? 
Co1 O8 Mo2 103.0(2) . . ? 
Mo10 O8 Mo2 149.3(2) . . ? 
Co1 O8 Mo1 99.9(2) . . ? 
Mo10 O8 Mo1 103.2(2) . . ? 
Mo2 O8 Mo1 90.93(16) . . ? 
Mo10 O10 Sm1 150.1(3) . . ? 
Mo4 O11 Mo3 118.5(3) . . ? 
Co1 O12 Co2 95.8(2) . . ? 
Co1 O12 Mo10 93.23(18) . . ? 
Co2 O12 Mo10 103.0(2) . . ? 
Co1 O12 Mo5 100.8(2) . . ? 
Co2 O12 Mo5 90.35(17) . . ? 
Mo10 O12 Mo5 159.6(2) . . ? 
Co2 O14 Co1 95.9(2) . . ? 
Co2 O14 Mo1 92.5(2) . . ? 
Co1 O14 Mo1 102.6(2) . . ? 
Co2 O14 Mo6 101.5(2) . . ? 
Co1 O14 Mo6 92.2(2) . . ? 
Mo1 O14 Mo6 158.6(2) . . ? 
Mo2 O17 Mo3 117.5(2) . . ? 
Mo9 O19 Mo8 118.1(2) . . ? 
Mo8 O20 Mo7 117.5(2) . . ? 
Co2 O21 Mo9 101.1(2) . . ? 
Co2 O21 Mo8 102.6(2) . . ? 
Mo9 O21 Mo8 92.63(18) . . ? 
Mo10 O22 Mo9 117.9(3) . . ? 
Co1 O23 Mo2 101.7(2) . . ? 
Co1 O23 Mo3 103.7(2) . . ? 
Mo2 O23 Mo3 93.60(17) . . ? 
Mo6 O26 Mo7 117.6(3) . . ? 
Mo2 O31 Sm1 147.4(3) . . ? 
Mo5 O34 Mo4 117.0(2) . . ? 
Mo1 O35 Sm1 143.6(3) . . ? 
Co1 O37 Mo6 101.6(2) . . ? 
Co1 O37 Mo4 101.38(19) . . ? 
Mo6 O37 Mo4 149.1(2) . . ? 
Co1 O37 Mo5 102.3(2) . . ? 
Mo6 O37 Mo5 102.79(19) . . ? 
Mo4 O37 Mo5 92.24(18) . . ? 
Co2 O38 Mo7 102.7(2) . . ? 
Co2 O38 Mo8 102.8(2) . . ? 
Mo7 O38 Mo8 92.93(16) . . ? 
 
_diffrn_measured_fraction_theta_max    0.994 
_diffrn_reflns_theta_full              25.00 
_diffrn_measured_fraction_theta_full   0.994 
_refine_diff_density_max    1.585 
_refine_diff_density_min   -1.575 
_refine_diff_density_rms    0.170 


#=====================END 
 
data_4 
 
_audit_creation_method            SHELXL-97 
_chemical_name_systematic 
; 
 ? 
; 
_chemical_name_common             ? 
_chemical_melting_point           ? 
_chemical_formula_moiety          ? 
_chemical_formula_sum 
 'H40 Co2 Eu Mo10 N3 O50' 
_chemical_formula_weight          2111.57 
 
loop_ 
 _atom_type_symbol 
 _atom_type_description 
 _atom_type_scat_dispersion_real 
 _atom_type_scat_dispersion_imag 
 _atom_type_scat_source 
 'O'  'O'   0.0106   0.0060 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'H'  'H'   0.0000   0.0000 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'N'  'N'   0.0061   0.0033 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Co'  'Co'   0.3494   0.9721 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Mo'  'Mo'  -1.6832   0.6857 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Eu'  'Eu'  -0.1578   3.6682 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 
_symmetry_cell_setting            Monoclinic 
_symmetry_space_group_name_H-M    P2(1) 
 
loop_ 
 _symmetry_equiv_pos_as_xyz 
 'x, y, z' 
 '-x, y+1/2, -z' 
 
_cell_length_a                    10.5122(5) 
_cell_length_b                    18.6663(9) 
_cell_length_c                    12.2157(6) 
_cell_angle_alpha                 90.00 
_cell_angle_beta                  114.060(2) 
_cell_angle_gamma                 90.00 
_cell_volume                      2188.76(18) 
_cell_formula_units_Z             2 
_cell_measurement_temperature     296(2) 
_cell_measurement_reflns_used     8771  
_cell_measurement_theta_min       1.83 
_cell_measurement_theta_max       25.00 
 
_exptl_crystal_description        'block' 
_exptl_crystal_colour             'dark green' 
_exptl_crystal_size_max           0.22 
_exptl_crystal_size_mid           0.18 
_exptl_crystal_size_min           0.15  
_exptl_crystal_density_meas       ? 
_exptl_crystal_density_diffrn     3.204 
_exptl_crystal_density_method     'not measured' 
_exptl_crystal_F_000              1996 
_exptl_absorpt_coefficient_mu     5.037 
_exptl_absorpt_correction_type    empirical 
_exptl_absorpt_correction_T_min   0.350 
_exptl_absorpt_correction_T_max   0.470 
_exptl_absorpt_process_details    'ABSCOR by T.Higashi 8 March, 1995' 
  
 
_exptl_special_details 
; 
 ? 
; 
 
_diffrn_ambient_temperature       296(2) 
_diffrn_radiation_wavelength      0.71073 
_diffrn_radiation_type            MoK\a 
_diffrn_radiation_source          'fine-focus sealed tube' 
_diffrn_radiation_monochromator   graphite 
_diffrn_measurement_device_type   'Bruker Smart Apex CCD'
_diffrn_measurement_method        'ω-2θ' 
_diffrn_detector_area_resol_mean  0.01 
_diffrn_standards_number          0 
_diffrn_standards_interval_count  0
_diffrn_standards_interval_time   0 
_diffrn_standards_decay_%         none 
_diffrn_reflns_number             8771 
_diffrn_reflns_av_R_equivalents   0.0000 
_diffrn_reflns_av_sigmaI/netI     0.0597 
_diffrn_reflns_limit_h_min        -12 
_diffrn_reflns_limit_h_max        12 
_diffrn_reflns_limit_k_min        -18 
_diffrn_reflns_limit_k_max        22 
_diffrn_reflns_limit_l_min        -10 
_diffrn_reflns_limit_l_max        14 
_diffrn_reflns_theta_min          1.83 
_diffrn_reflns_theta_max          25.00 
_reflns_number_total              8771 
_reflns_number_gt                 8742 
_reflns_threshold_expression      >2sigma(I) 
 
_computing_data_collection        ? 
_computing_cell_refinement        ? 
_computing_data_reduction         ? 
_computing_structure_solution     'SHELXS-97 (Sheldrick, 1990)' 
_computing_structure_refinement   'SHELXL-97 (Sheldrick, 1997)' 
_computing_molecular_graphics     'Bruker SHELXTL' 
_computing_publication_material   'Bruker SHELXTL' 
 
_refine_special_details 
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
; 
 
_refine_ls_structure_factor_coef  Fsqd  
_refine_ls_matrix_type            full 
_refine_ls_weighting_scheme       calc  
_refine_ls_weighting_details 
 'calc w=1/[σ²(Fo²)+(0.0374P)²+1.1019P] where P=(Fo²+2Fc²)/3' 
_atom_sites_solution_primary      direct 
_atom_sites_solution_secondary    difmap 
_atom_sites_solution_hydrogens    '.' 
_refine_ls_hydrogen_treatment     'constr' 
_refine_ls_extinction_method      none 
_refine_ls_extinction_coef        ? 
_refine_ls_abs_structure_details 
 'Flack H D (1983), Acta Cryst. A39, 876-881' 
_refine_ls_abs_structure_Flack    0.042(8) 
_refine_ls_number_reflns          8771 
_refine_ls_number_parameters      605 
_refine_ls_number_restraints      25 
_refine_ls_R_factor_all           0.0302 
_refine_ls_R_factor_gt            0.0301 
_refine_ls_wR_factor_ref          0.0813 
_refine_ls_wR_factor_gt           0.0812 
_refine_ls_goodness_of_fit_ref    1.054 
_refine_ls_restrained_S_all       1.054 
_refine_ls_shift/su_max           0.001 
_refine_ls_shift/su_mean          0.000 
 
loop_ 
 _atom_site_label 
 _atom_site_type_symbol 
 _atom_site_fract_x 
 _atom_site_fract_y 
 _atom_site_fract_z 
 _atom_site_U_iso_or_equiv 
 _atom_site_adp_type 
 _atom_site_occupancy 
 _atom_site_symmetry_multiplicity 
 _atom_site_calc_flag 
 _atom_site_refinement_flags 
 _atom_site_disorder_assembly 
 _atom_site_disorder_group 
Eu1 Eu 0.56449(3) 0.29941(2) 0.85785(3) 0.01713(9) Uani 1 1 d . . . 
Mo1 Mo 0.64143(7) 0.43889(4) 0.37609(6) 0.01883(15) Uani 1 1 d . . . 
Mo2 Mo 0.48169(6) 0.41487(4) 0.55462(6) 0.01506(14) Uani 1 1 d . . . 
Mo3 Mo 0.57136(6) 0.51006(3) 0.79812(6) 0.01294(14) Uani 1 1 d . . . 
Mo4 Mo 0.68634(6) 0.68560(3) 0.61005(6) 0.01384(14) Uani 1 1 d . . . 
Mo5 Mo 0.93347(6) 0.67327(4) 1.11993(6) 0.01555(14) Uani 1 1 d . . . 
Mo6 Mo 0.86956(6) 0.42257(3) 0.83849(6) 0.01289(13) Uani 1 1 d . . . 
Mo7 Mo 0.81177(7) 0.76915(4) 0.87062(6) 0.01752(15) Uani 1 1 d . . . 
Mo8 Mo 0.94915(6) 0.49700(4) 1.10108(6) 0.01697(15) Uani 1 1 d . . . 
Mo9 Mo 1.01957(6) 0.62764(4) 0.73147(6) 0.01424(14) Uani 1 1 d . . . 
Mo10 Mo 0.89495(6) 0.56003(3) 0.45881(6) 0.01562(14) Uani 1 1 d . . . 
Co1 Co 0.83034(9) 0.59319(5) 0.85628(9) 0.0115(2) Uani 1 1 d . . . 
Co2 Co 0.74156(10) 0.52561(5) 0.63461(8) 0.0117(2) Uani 1 1 d . . . 
O1 O 0.9080(6) 0.6437(3) 0.4081(5) 0.0287(14) Uani 1 1 d . . . 
O2 O 1.1083(6) 0.4982(3) 1.2154(5) 0.0286(14) Uani 1 1 d . . . 
O3 O 0.7215(6) 0.8224(4) 0.9257(5) 0.0297(14) Uani 1 1 d . . . 
O4 O 0.5390(5) 0.4319(3) 0.8584(4) 0.0172(11) Uani 1 1 d . . . 
O5 O 0.8020(5) 0.6089(3) 0.5805(4) 0.0144(11) Uani 1 1 d . . . 
O6 O 0.7471(6) 0.7485(3) 0.5442(5) 0.0232(13) Uani 1 1 d . . . 
O7 O 0.7422(6) 0.3820(3) 0.3377(5) 0.0314(15) Uani 1 1 d . . . 
O8 O 0.5240(5) 0.6654(4) 0.5042(5) 0.0262(14) Uani 1 1 d . . . 
O9 O 0.9562(5) 0.3829(3) 0.7632(5) 0.0263(13) Uani 1 1 d . . . 
O10 O 0.8330(6) 0.7237(3) 1.1700(5) 0.0282(14) Uani 1 1 d . . . 
O11 O 0.8967(6) 0.8252(3) 0.8151(6) 0.0310(15) Uani 1 1 d . . . 
O12 O 0.9037(5) 0.5303(3) 0.7757(4) 0.0130(11) Uani 1 1 d . . . 
O13 O 0.7578(5) 0.6633(3) 0.9335(4) 0.0139(11) Uani 1 1 d . . . 
O14 O 0.7110(5) 0.5330(3) 0.3545(5) 0.0224(12) Uani 1 1 d . . . 
O15 O 0.8823(5) 0.6721(3) 0.7842(4) 0.0132(10) Uani 1 1 d . . . 
O16 O 0.3241(5) 0.4155(4) 0.4408(5) 0.0274(14) Uani 1 1 d . . . 
O17 O 1.0641(6) 0.7053(3) 0.6850(6) 0.0280(14) Uani 1 1 d . . . 
O18 O 0.4364(5) 0.4950(3) 0.6405(5) 0.0191(12) Uani 1 1 d . . . 
O19 O 0.4751(6) 0.3475(3) 0.6508(5) 0.0220(12) Uani 1 1 d . . . 
O20 O 0.5035(5) 0.5776(3) 0.8502(5) 0.0216(12) Uani 1 1 d . . . 
O21 O 0.9930(6) 0.5065(3) 0.4105(6) 0.0297(14) Uani 1 1 d . . . 
O22 O 0.8255(5) 0.4691(3) 0.5497(4) 0.0148(11) Uani 1 1 d . . . 
O23 O 1.1544(5) 0.6078(3) 0.8690(5) 0.0280(14) Uani 1 1 d . . . 
O24 O 1.0470(5) 0.5648(3) 0.6238(5) 0.0176(12) Uani 1 1 d . . . 
O25 O 0.6858(4) 0.4486(3) 0.7020(4) 0.0139(11) Uani 1 1 d . . . 
O26 O 1.0076(5) 0.4460(3) 0.9857(5) 0.0190(12) Uani 1 1 d . . . 
O27 O 0.9927(5) 0.5932(3) 1.0078(4) 0.0141(11) Uani 1 1 d . . . 
O28 O 0.6660(5) 0.5865(3) 0.7152(4) 0.0136(11) Uani 1 1 d . . . 
O29 O 0.4862(6) 0.4430(4) 0.2532(5) 0.0344(16) Uani 1 1 d . . . 
O30 O 0.7811(5) 0.3544(3) 0.8765(5) 0.0218(12) Uani 1 1 d . . . 
O31 O 0.5940(6) 0.3763(3) 0.4803(5) 0.0222(12) Uani 1 1 d . . . 
O32 O 0.9693(5) 0.7406(3) 1.0148(5) 0.0196(12) Uani 1 1 d . . . 
O33 O 0.8629(5) 0.5799(3) 1.1360(5) 0.0198(12) Uani 1 1 d . . . 
O34 O 0.7698(5) 0.5109(3) 0.9128(4) 0.0129(11) Uani 1 1 d . . . 
O35 O 0.5699(5) 0.5075(3) 0.4930(4) 0.0153(11) Uani 1 1 d . . . 
O36 O 0.6511(5) 0.7404(3) 0.7226(5) 0.0219(13) Uani 1 1 d . . . 
O37 O 0.8588(6) 0.4316(3) 1.1350(5) 0.0270(13) Uani 1 1 d . . . 
O38 O 1.0966(5) 0.6718(3) 1.2333(5) 0.0285(14) Uani 1 1 d . . . 
O1W O 0.6226(7) 0.3453(4) 1.0621(5) 0.0363(16) Uani 1 1 d . . . 
O2W O 0.5022(6) 0.2060(3) 0.9663(6) 0.0293(14) Uani 1 1 d . . . 
O3W O 0.6419(7) 0.2255(5) 0.7305(7) 0.061(3) Uani 1 1 d . . . 
O4W O 0.7700(6) 0.2303(4) 0.9791(7) 0.046(2) Uani 1 1 d . . . 
O5W O 0.3722(7) 0.2204(4) 0.7146(6) 0.0424(18) Uani 1 1 d . . . 
O6W O 0.3369(6) 0.3398(4) 0.8478(6) 0.0360(16) Uani 1 1 d . . . 
OW1 O 0.4165(7) 0.7402(4) 0.7902(6) 0.0450(18) Uani 1 1 d . . . 
OW2 O 1.0055(7) 0.2914(4) 0.5828(6) 0.0481(18) Uani 1 1 d . . . 
OW3 O 1.0361(7) 0.3590(4) 0.3803(7) 0.0442(18) Uani 1 1 d . . . 
OW4 O 0.4135(7) 0.0716(4) 0.8843(6) 0.0385(16) Uani 1 1 d . . . 
OW5 O 0.2002(8) 0.4391(5) 0.6778(9) 0.077(3) Uani 1 1 d . . . 
OW6 O 0.3462(11) 0.4683(5) -0.0022(9) 0.080(3) Uani 1 1 d . . . 
N1 N 0.2712(9) 0.7392(6) 0.5229(9) 0.057(3) Uani 1 1 d U . . 
N2 N 0.2539(10) 0.5933(6) 0.4600(10) 0.065(3) Uani 1 1 d U . . 
N3 N 0.6372(16) 0.0734(9) 0.7268(17) 0.074(5) Uani 0.70 1 d PU . . 
N4 N 0.696(3) 0.0746(17) 0.853(3) 0.043(7) Uani 0.30 1 d PU . . 
 
 
_geom_special_details 
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
; 
 
loop_ 
 _geom_bond_atom_site_label_1 
 _geom_bond_atom_site_label_2 
 _geom_bond_distance 
 _geom_bond_site_symmetry_2 
 _geom_bond_publ_flag 
Eu1 O30 2.423(5) . ? 
Eu1 O4W 2.432(6) . ? 
Eu1 O2W 2.436(6) . ? 
Eu1 O3W 2.453(8) . ? 
Eu1 O6W 2.464(6) . ? 
Eu1 O19 2.480(6) . ? 
Eu1 O4 2.489(6) . ? 
Eu1 O1W 2.467(6) . ? 
Eu1 O5W 2.537(6) . ? 
Mo1 O7 1.696(6) . ? 
Mo1 O29 1.710(5) . ? 
Mo1 O31 1.937(5) . ? 
Mo1 O14 1.961(6) . ? 
Mo1 O35 2.264(5) . ? 
Mo1 O22 2.283(5) . ? 
Mo2 O16 1.673(5) . ? 
Mo2 O19 1.742(6) . ? 
Mo2 O31 1.901(5) . ? 
Mo2 O18 1.993(6) . ? 
Mo2 O35 2.233(5) . ? 
Mo2 O25 2.256(5) . ? 
Mo3 O20 1.695(5) . ? 
Mo3 O4 1.729(5) . ? 
Mo3 O18 1.890(5) . ? 
Mo3 O34 1.982(5) . ? 
Mo3 O28 2.207(5) . ? 
Mo3 O25 2.302(5) . ? 
Mo3 Co1 2.9577(11) . ? 
Mo4 O6 1.689(6) . ? 
Mo4 O8 1.711(5) . ? 
Mo4 O36 1.868(6) . ? 
Mo4 O5 2.004(5) . ? 
Mo4 O15 2.294(5) . ? 
Mo4 O28 2.312(5) . ? 
Mo4 Co2 3.0339(12) . ? 
Mo5 O10 1.703(6) . ? 
Mo5 O38 1.710(5) . ? 
Mo5 O32 1.940(6) . ? 
Mo5 O33 1.935(6) . ? 
Mo5 O27 2.279(5) . ? 
Mo5 O13 2.281(5) . ? 
Mo6 O9 1.704(6) . ? 
Mo6 O30 1.746(5) . ? 
Mo6 O26 1.845(5) . ? 
Mo6 O25 2.030(5) . ? 
Mo6 O12 2.233(5) . ? 
Mo6 O34 2.328(5) . ? 
Mo6 Co2 2.9967(12) . ? 
Mo7 O11 1.686(6) . ? 
Mo7 O3 1.692(6) . ? 
Mo7 O32 1.936(5) . ? 
Mo7 O36 1.980(6) . ? 
Mo7 O13 2.274(5) . ? 
Mo7 O15 2.363(5) . ? 
Mo8 O2 1.687(5) . ? 
Mo8 O37 1.699(6) . ? 
Mo8 O33 1.927(6) . ? 
Mo8 O26 1.994(5) . ? 
Mo8 O27 2.271(5) . ? 
Mo8 O34 2.319(5) . ? 
Mo9 O17 1.691(6) . ? 
Mo9 O23 1.739(5) . ? 
Mo9 O24 1.870(5) . ? 
Mo9 O15 1.986(5) . ? 
Mo9 O5 2.305(5) . ? 
Mo9 O12 2.369(5) . ? 
Mo9 Co1 3.0278(12) . ? 
Mo10 O21 1.704(6) . ? 
Mo10 O1 1.706(6) . ? 
Mo10 O14 1.900(5) . ? 
Mo10 O24 2.000(5) . ? 
Mo10 O5 2.276(5) . ? 
Mo10 O22 2.303(5) . ? 
Co1 O28 1.882(5) . ? 
Co1 O34 1.897(5) . ? 
Co1 O15 1.906(5) . ? 
Co1 O12 1.887(5) . ? 
Co1 O13 1.942(5) . ? 
Co1 O27 1.940(5) . ? 
Co1 Co2 2.7811(14) . ? 
Co2 O12 1.868(5) . ? 
Co2 O25 1.866(5) . ? 
Co2 O28 1.879(5) . ? 
Co2 O5 1.898(5) . ? 
Co2 O22 1.927(5) . ? 
Co2 O35 1.954(5) . ? 
N3 N4 1.40(3) . ? 
 
loop_ 
 _geom_angle_atom_site_label_1 
 _geom_angle_atom_site_label_2 
 _geom_angle_atom_site_label_3 
 _geom_angle 
 _geom_angle_site_symmetry_1 
 _geom_angle_site_symmetry_3 
 _geom_angle_publ_flag 
O30 Eu1 O4W 66.4(2) . . ? 
O30 Eu1 O2W 134.7(2) . . ? 
O4W Eu1 O2W 70.0(2) . . ? 
O30 Eu1 O3W 75.9(2) . . ? 
O4W Eu1 O3W 69.3(3) . . ? 
O2W Eu1 O3W 100.1(3) . . ? 
O30 Eu1 O6W 137.0(2) . . ? 
O4W Eu1 O6W 142.7(2) . . ? 
O2W Eu1 O6W 77.0(2) . . ? 
O3W Eu1 O6W 135.0(2) . . ? 
O30 Eu1 O19 83.87(18) . . ? 
O4W Eu1 O19 133.3(2) . . ? 
O2W Eu1 O19 137.71(19) . . ? 
O3W Eu1 O19 69.0(2) . . ? 
O6W Eu1 O19 83.23(19) . . ? 
O30 Eu1 O4 71.12(17) . . ? 
O4W Eu1 O4 126.5(2) . . ? 
O2W Eu1 O4 131.08(19) . . ? 
O3W Eu1 O4 128.7(3) . . ? 
O6W Eu1 O4 65.97(19) . . ? 
O19 Eu1 O4 69.31(18) . . ? 
O30 Eu1 O1W 85.5(2) . . ? 
O4W Eu1 O1W 77.0(3) . . ? 
O2W Eu1 O1W 73.1(2) . . ? 
O3W Eu1 O1W 145.8(2) . . ? 
O6W Eu1 O1W 77.2(2) . . ? 
O19 Eu1 O1W 137.8(2) . . ? 
O4 Eu1 O1W 68.6(2) . . ? 
O30 Eu1 O5W 139.9(2) . . ? 
O4W Eu1 O5W 111.9(3) . . ? 
O2W Eu1 O5W 69.1(2) . . ? 
O3W Eu1 O5W 67.2(2) . . ? 
O6W Eu1 O5W 70.0(2) . . ? 
O19 Eu1 O5W 69.1(2) . . ? 
O4 Eu1 O5W 121.5(2) . . ? 
O1W Eu1 O5W 134.3(2) . . ? 
O7 Mo1 O29 105.4(3) . . ? 
O7 Mo1 O31 99.2(3) . . ? 
O29 Mo1 O31 101.2(3) . . ? 
O7 Mo1 O14 102.4(3) . . ? 
O29 Mo1 O14 96.7(3) . . ? 
O31 Mo1 O14 147.0(2) . . ? 
O7 Mo1 O35 159.2(2) . . ? 
O29 Mo1 O35 94.9(3) . . ? 
O31 Mo1 O35 71.7(2) . . ? 
O14 Mo1 O35 79.4(2) . . ? 
O7 Mo1 O22 91.3(2) . . ? 
O29 Mo1 O22 161.5(3) . . ? 
O31 Mo1 O22 83.5(2) . . ? 
O14 Mo1 O22 71.5(2) . . ? 
O35 Mo1 O22 69.38(16) . . ? 
O16 Mo2 O19 105.5(3) . . ? 
O16 Mo2 O31 101.7(3) . . ? 
O19 Mo2 O31 104.6(3) . . ? 
O16 Mo2 O18 93.7(3) . . ? 
O19 Mo2 O18 95.9(2) . . ? 
O31 Mo2 O18 149.8(2) . . ? 
O16 Mo2 O35 96.9(2) . . ? 
O19 Mo2 O35 157.4(2) . . ? 
O31 Mo2 O35 73.0(2) . . ? 
O18 Mo2 O35 79.5(2) . . ? 
O16 Mo2 O25 163.4(3) . . ? 
O19 Mo2 O25 87.1(2) . . ? 
O31 Mo2 O25 85.0(2) . . ? 
O18 Mo2 O25 74.01(19) . . ? 
O35 Mo2 O25 70.27(17) . . ? 
O20 Mo3 O4 106.4(3) . . ? 
O20 Mo3 O18 103.7(3) . . ? 
O4 Mo3 O18 96.5(2) . . ? 
O20 Mo3 O34 102.2(2) . . ? 
O4 Mo3 O34 92.2(2) . . ? 
O18 Mo3 O34 149.0(2) . . ? 
O20 Mo3 O28 91.6(2) . . ? 
O4 Mo3 O28 160.8(2) . . ? 
O18 Mo3 O28 85.4(2) . . ? 
O34 Mo3 O28 77.16(19) . . ? 
O20 Mo3 O25 161.8(2) . . ? 
O4 Mo3 O25 91.8(2) . . ? 
O18 Mo3 O25 74.78(19) . . ? 
O34 Mo3 O25 75.30(19) . . ? 
O28 Mo3 O25 70.18(19) . . ? 
O20 Mo3 Co1 90.37(19) . . ? 
O4 Mo3 Co1 131.44(16) . . ? 
O18 Mo3 Co1 123.91(16) . . ? 
O34 Mo3 Co1 39.26(15) . . ? 
O28 Mo3 Co1 39.49(12) . . ? 
O25 Mo3 Co1 76.27(12) . . ? 
O6 Mo4 O8 104.3(3) . . ? 
O6 Mo4 O36 101.4(3) . . ? 
O8 Mo4 O36 103.9(3) . . ? 
O6 Mo4 O5 92.0(2) . . ? 
O8 Mo4 O5 101.4(3) . . ? 
O36 Mo4 O5 147.2(2) . . ? 
O6 Mo4 O15 98.5(2) . . ? 
O8 Mo4 O15 156.8(3) . . ? 
O36 Mo4 O15 75.5(2) . . ? 
O5 Mo4 O15 72.97(19) . . ? 
O6 Mo4 O28 163.7(2) . . ? 
O8 Mo4 O28 87.4(2) . . ? 
O36 Mo4 O28 86.5(2) . . ? 
O5 Mo4 O28 74.28(19) . . ? 
O15 Mo4 O28 69.41(17) . . ? 
O6 Mo4 Co2 129.6(2) . . ? 
O8 Mo4 Co2 87.1(2) . . ? 
O36 Mo4 Co2 123.62(18) . . ? 
O5 Mo4 Co2 37.73(14) . . ? 
O15 Mo4 Co2 74.74(14) . . ? 
O28 Mo4 Co2 38.23(13) . . ? 
O10 Mo5 O38 106.4(3) . . ? 
O10 Mo5 O32 101.3(3) . . ? 
O38 Mo5 O32 98.4(3) . . ? 
O10 Mo5 O33 98.1(3) . . ? 
O38 Mo5 O33 101.7(3) . . ? 
O32 Mo5 O33 146.7(2) . . ? 
O10 Mo5 O27 159.9(2) . . ? 
O38 Mo5 O27 92.7(2) . . ? 
O32 Mo5 O27 81.5(2) . . ? 
O33 Mo5 O27 71.3(2) . . ? 
O10 Mo5 O13 92.0(2) . . ? 
O38 Mo5 O13 160.7(2) . . ? 
O32 Mo5 O13 71.9(2) . . ? 
O33 Mo5 O13 80.8(2) . . ? 
O27 Mo5 O13 69.80(17) . . ? 
O9 Mo6 O30 106.6(3) . . ? 
O9 Mo6 O26 104.4(2) . . ? 
O30 Mo6 O26 101.9(3) . . ? 
O9 Mo6 O25 101.5(2) . . ? 
O30 Mo6 O25 87.8(2) . . ? 
O26 Mo6 O25 148.3(2) . . ? 
O9 Mo6 O12 90.6(2) . . ? 
O30 Mo6 O12 157.6(2) . . ? 
O26 Mo6 O12 87.1(2) . . ? 
O25 Mo6 O12 74.63(19) . . ? 
O9 Mo6 O34 160.5(2) . . ? 
O30 Mo6 O34 92.2(2) . . ? 
O26 Mo6 O34 75.7(2) . . ? 
O25 Mo6 O34 73.85(19) . . ? 
O12 Mo6 O34 69.94(18) . . ? 
O9 Mo6 Co2 89.3(2) . . ? 
O30 Mo6 Co2 125.53(18) . . ? 
O26 Mo6 Co2 124.49(18) . . ? 
O25 Mo6 Co2 37.75(14) . . ? 
O12 Mo6 Co2 38.47(12) . . ? 
O34 Mo6 Co2 75.42(12) . . ? 
O11 Mo7 O3 105.7(3) . . ? 
O11 Mo7 O32 98.0(3) . . ? 
O3 Mo7 O32 102.1(3) . . ? 
O11 Mo7 O36 101.3(3) . . ? 
O3 Mo7 O36 96.6(3) . . ? 
O32 Mo7 O36 148.3(3) . . ? 
O11 Mo7 O13 157.0(2) . . ? 
O3 Mo7 O13 96.8(3) . . ? 
O32 Mo7 O13 72.1(2) . . ? 
O36 Mo7 O13 80.5(2) . . ? 
O11 Mo7 O15 89.0(2) . . ? 
O3 Mo7 O15 163.2(2) . . ? 
O32 Mo7 O15 83.5(2) . . ? 
O36 Mo7 O15 71.99(19) . . ? 
O13 Mo7 O15 69.61(18) . . ? 
O2 Mo8 O37 105.8(3) . . ? 
O2 Mo8 O33 101.8(3) . . ? 
O37 Mo8 O33 99.4(2) . . ? 
O2 Mo8 O26 95.9(3) . . ? 
O37 Mo8 O26 101.2(3) . . ? 
O33 Mo8 O26 148.0(2) . . ? 
O2 Mo8 O27 94.0(3) . . ? 
O37 Mo8 O27 159.7(2) . . ? 
O33 Mo8 O27 71.7(2) . . ? 
O26 Mo8 O27 80.8(2) . . ? 
O2 Mo8 O34 161.9(3) . . ? 
O37 Mo8 O34 90.8(2) . . ? 
O33 Mo8 O34 82.2(2) . . ? 
O26 Mo8 O34 73.31(19) . . ? 
O27 Mo8 O34 70.26(17) . . ? 
O17 Mo9 O23 106.2(3) . . ? 
O17 Mo9 O24 99.1(3) . . ? 
O23 Mo9 O24 104.3(2) . . ? 
O17 Mo9 O15 95.1(3) . . ? 
O23 Mo9 O15 100.9(2) . . ? 
O24 Mo9 O15 146.2(2) . . ? 
O17 Mo9 O5 100.4(2) . . ? 
O23 Mo9 O5 153.2(2) . . ? 
O24 Mo9 O5 74.29(19) . . ? 
O15 Mo9 O5 73.02(18) . . ? 
O17 Mo9 O12 166.5(2) . . ? 
O23 Mo9 O12 84.8(2) . . ? 
O24 Mo9 O12 85.4(2) . . ? 
O15 Mo9 O12 74.8(2) . . ? 
O5 Mo9 O12 68.39(17) . . ? 
O17 Mo9 Co1 132.8(2) . . ? 
O23 Mo9 Co1 85.0(2) . . ? 
O24 Mo9 Co1 122.80(17) . . ? 
O15 Mo9 Co1 38.00(15) . . ? 
O5 Mo9 Co1 74.31(13) . . ? 
O12 Mo9 Co1 38.55(12) . . ? 
O21 Mo10 O1 105.2(3) . . ? 
O21 Mo10 O14 101.9(3) . . ? 
O1 Mo10 O14 102.1(3) . . ? 
O21 Mo10 O24 91.6(3) . . ? 
O1 Mo10 O24 100.2(3) . . ? 
O14 Mo10 O24 149.8(2) . . ? 
O21 Mo10 O5 160.4(3) . . ? 
O1 Mo10 O5 89.4(2) . . ? 
O14 Mo10 O5 87.4(2) . . ? 
O24 Mo10 O5 72.74(19) . . ? 
O21 Mo10 O22 95.2(3) . . ? 
O1 Mo10 O22 159.6(2) . . ? 
O14 Mo10 O22 72.0(2) . . ? 
O24 Mo10 O22 80.0(2) . . ? 
O5 Mo10 O22 71.09(18) . . ? 
O28 Co1 O34 87.7(2) . . ? 
O28 Co1 O15 87.6(2) . . ? 
O34 Co1 O15 174.4(2) . . ? 
O28 Co1 O12 84.2(2) . . ? 
O34 Co1 O12 87.4(2) . . ? 
O15 Co1 O12 89.1(2) . . ? 
O28 Co1 O13 95.4(2) . . ? 
O34 Co1 O13 96.4(2) . . ? 
O15 Co1 O13 87.0(2) . . ? 
O12 Co1 O13 176.1(2) . . ? 
O28 Co1 O27 174.7(2) . . ? 
O34 Co1 O27 87.0(2) . . ? 
O15 Co1 O27 97.7(2) . . ? 
O12 Co1 O27 96.3(2) . . ? 
O13 Co1 O27 84.5(2) . . ? 
O28 Co1 Co2 42.27(16) . . ? 
O34 Co1 Co2 87.58(15) . . ? 
O15 Co1 Co2 86.94(15) . . ? 
O12 Co1 Co2 41.95(14) . . ? 
O13 Co1 Co2 137.41(14) . . ? 
O27 Co1 Co2 138.12(16) . . ? 
O28 Co1 Mo3 48.21(16) . . ? 
O34 Co1 Mo3 41.40(14) . . ? 
O15 Co1 Mo3 134.70(14) . . ? 
O12 Co1 Mo3 94.61(15) . . ? 
O13 Co1 Mo3 87.98(15) . . ? 
O27 Co1 Mo3 126.50(16) . . ? 
Co2 Co1 Mo3 67.51(3) . . ? 
O28 Co1 Mo9 95.72(16) . . ? 
O34 Co1 Mo9 137.91(15) . . ? 
O15 Co1 Mo9 39.89(15) . . ? 
O12 Co1 Mo9 51.48(15) . . ? 
O13 Co1 Mo9 124.78(16) . . ? 
O27 Co1 Mo9 88.70(15) . . ? 
Co2 Co1 Mo9 68.57(3) . . ? 
Mo3 Co1 Mo9 136.04(4) . . ? 
O12 Co2 O25 87.8(2) . . ? 
O12 Co2 O28 84.8(2) . . ? 
O25 Co2 O28 87.6(2) . . ? 
O12 Co2 O5 88.5(2) . . ? 
O25 Co2 O5 174.3(2) . . ? 
O28 Co2 O5 87.7(2) . . ? 
O12 Co2 O22 94.4(2) . . ? 
O25 Co2 O22 96.4(2) . . ? 
O28 Co2 O22 175.9(2) . . ? 
O5 Co2 O22 88.2(2) . . ? 
O12 Co2 O35 172.4(2) . . ? 
O25 Co2 O35 85.1(2) . . ? 
O28 Co2 O35 97.6(2) . . ? 
O5 Co2 O35 98.8(2) . . ? 
O22 Co2 O35 83.6(2) . . ? 
O12 Co2 Co1 42.48(16) . . ? 
O25 Co2 Co1 87.78(16) . . ? 
O28 Co2 Co1 42.37(14) . . ? 
O5 Co2 Co1 86.58(16) . . ? 
O22 Co2 Co1 136.63(15) . . ? 
O35 Co2 Co1 139.69(16) . . ? 
O12 Co2 Mo6 48.06(16) . . ? 
O25 Co2 Mo6 41.77(14) . . ? 
O28 Co2 Mo6 95.46(16) . . ? 
O5 Co2 Mo6 135.62(15) . . ? 
O22 Co2 Mo6 86.99(15) . . ? 
O35 Co2 Mo6 124.37(16) . . ? 
Co1 Co2 Mo6 67.86(3) . . ? 
O12 Co2 Mo4 96.36(16) . . ? 
O25 Co2 Mo4 136.09(16) . . ? 
O28 Co2 Mo4 49.60(16) . . ? 
O5 Co2 Mo4 40.24(15) . . ? 
O22 Co2 Mo4 126.61(16) . . ? 
O35 Co2 Mo4 90.70(16) . . ? 
Co1 Co2 Mo4 67.94(3) . . ? 
Mo6 Co2 Mo4 135.81(4) . . ? 
Mo3 O4 Eu1 142.9(3) . . ? 
Co2 O5 Mo4 102.0(2) . . ? 
Co2 O5 Mo10 101.1(2) . . ? 
Mo4 O5 Mo10 149.0(3) . . ? 
Co2 O5 Mo9 102.1(2) . . ? 
Mo4 O5 Mo9 103.0(2) . . ? 
Mo10 O5 Mo9 91.91(18) . . ? 
Co2 O12 Co1 95.6(2) . . ? 
Co2 O12 Mo6 93.5(2) . . ? 
Co1 O12 Mo6 102.9(2) . . ? 
Co2 O12 Mo9 100.7(2) . . ? 
Co1 O12 Mo9 90.0(2) . . ? 
Mo6 O12 Mo9 159.8(2) . . ? 
Co1 O13 Mo5 102.8(2) . . ? 
Co1 O13 Mo7 102.7(2) . . ? 
Mo5 O13 Mo7 93.10(18) . . ? 
Mo10 O14 Mo1 118.8(3) . . ? 
Co1 O15 Mo9 102.1(2) . . ? 
Co1 O15 Mo4 101.3(2) . . ? 
Mo9 O15 Mo4 104.0(2) . . ? 
Co1 O15 Mo7 100.7(2) . . ? 
Mo9 O15 Mo7 150.1(2) . . ? 
Mo4 O15 Mo7 90.20(17) . . ? 
Mo3 O18 Mo2 114.0(2) . . ? 
Mo2 O19 Eu1 147.8(3) . . ? 
Co2 O22 Mo1 103.6(2) . . ? 
Co2 O22 Mo10 99.3(2) . . ? 
Mo1 O22 Mo10 92.86(18) . . ? 
Mo9 O24 Mo10 116.6(2) . . ? 
Co2 O25 Mo6 100.5(2) . . ? 
Co2 O25 Mo2 103.3(2) . . ? 
Mo6 O25 Mo2 150.0(3) . . ? 
Co2 O25 Mo3 99.5(2) . . ? 
Mo6 O25 Mo3 102.7(2) . . ? 
Mo2 O25 Mo3 91.21(16) . . ? 
Mo6 O26 Mo8 117.1(3) . . ? 
Co1 O27 Mo8 101.5(2) . . ? 
Co1 O27 Mo5 102.9(2) . . ? 
Mo8 O27 Mo5 93.24(19) . . ? 
Co2 O28 Co1 95.4(2) . . ? 
Co2 O28 Mo3 102.5(2) . . ? 
Co1 O28 Mo3 92.3(2) . . ? 
Co2 O28 Mo4 92.2(2) . . ? 
Co1 O28 Mo4 101.4(2) . . ? 
Mo3 O28 Mo4 159.0(2) . . ? 
Mo6 O30 Eu1 150.0(3) . . ? 
Mo2 O31 Mo1 117.5(3) . . ? 
Mo5 O32 Mo7 117.1(2) . . ? 
Mo8 O33 Mo5 117.8(3) . . ? 
Co1 O34 Mo3 99.3(2) . . ? 
Co1 O34 Mo8 101.2(2) . . ? 
Mo3 O34 Mo8 153.6(3) . . ? 
Co1 O34 Mo6 99.2(2) . . ? 
Mo3 O34 Mo6 103.3(2) . . ? 
Mo8 O34 Mo6 89.65(17) . . ? 
Co2 O35 Mo2 101.3(2) . . ? 
Co2 O35 Mo1 103.4(2) . . ? 
Mo2 O35 Mo1 93.7(2) . . ? 
Mo4 O36 Mo7 118.0(3) . . ? 
 
_diffrn_measured_fraction_theta_max    0.984 
_diffrn_reflns_theta_full              25.00 
_diffrn_measured_fraction_theta_full   0.984 
_refine_diff_density_max    1.014 
_refine_diff_density_min   -1.228 
_refine_diff_density_rms    0.181 

#=======================END

